Preparation and Use of Lime Mortars (revised 2003) Conservatioll of Plasterwork (revised 2002) Perfornlance Standards for Timber Sash and Case Windows (1994) (deleted) Thatch & Thatching Techniques (1996) The Hebridean Blackhouse (1996) Earth Structures and Construction in Scotland (1996) Access to the Built Heritage (1996) Historic Scotland Guide to International Conservation Charters (1997) Stoneclealling of Granite Buildings (1997) Biological Growths on Sandstone Buildings (1997) Fire Protection Measures in Scottish Historic Buildings (1997)
Quarries of Scotland (1997) The Archaeology of Scottish Thatch (1998) The Installation of Sprinkler Systems in Historic Buildi~lgs(1998) Exten~alLime Coatings on Traditional Buildings (2001) Burrowing Aninials and Archaeology (1 999) Bracken and Archaeology (1999) The Treatment of Graffiti on Historic Surfaces (1999) Scottish Aggregates for Building Conservation (1999) Corrosion in Masonry Clad Early 20th Century Steel Fra~nedBuildi~igs(2000) Scottish Slate Quarries (2000) Fire Risk Management in Heritage Buildings (2001)
Non-Destructive Investigatioil of Standing Structures (2001)
Thc Environ~nentalControl of Dry Rot (2002)
Stonecleaning in Scotland - Research Suniniary Research Report: Volulnes l , 2, 3 Biological Growths, Biocide Treatment, Soiling and Decay of Salldstolle Buildings ancl Monuments in Scotland Cleaning of Granite Buildings A Future for Stone in Scotland Historic Landuse Assessment: Development and Potential of a Technique for Assessing Landuse Patterns Scottish Slate: The Potential for Usc The Future of the Scottish Burgh Survey The Pattern of Scottish Roofing The Historical and Technical Developn~entof the Sash and Case Window in Scotland Impact of the Braer Oil Spill on Historic Scotlalld Monuments in Shetland Studies of the Doinestic Dry Rot Fungus S e ~ p ~ rLcrcl.ynlcrr1s ln with Relevance to the Management of Decay in Buildings Evaluation of Limestone and Building Lirnes in Scotland
LITERATURE REVIEW Mortars in Historic Buildings Available from: Historic Scotland Technical Conservatio11, Research and Education Division Scottish Conservation Bureau Lollgmore House Salisbury Place EDINBURGH EH9 ISH
01 3 1 668 8668 0 13 1 668 8669
BUILDINGS. A REVIEW OF THE CONSERVATION, TECHNICAL AND SCIENTIFIC LITERATURE
by John J Hughes and Jan Vdek
Published by Historic Scotland
ISBN 1903570 82 4 O Crown Copyright Edinburgh ZOO3
TECHNICAL CONSERVATION, RESEARCH AND EDUCATION DIVISION
Author Dr. John J. Hughes (B.Sc., Ph.D.) Dr. Jan VBlek (M.Sc., Ph.D.) The Advanced Concrete and Masonry Centre School of Engineering and Science University of Paisley High Street Paisley PAl2BE
Note: This Literature Review covers documentation available up to May 2000
ACKNOWLEDGEMENTS Thanks go to Ingval Maxwell of Historic Scotland, who understood the need for this reveiw and commissioned the research, and to Historic Scotland who provided financial backing for this work. Thanks must also go to the University of Paisley for support, both financial and infrastructural, that underpinned the majority of the cost of this work. Final thanks must go to Neil Ross of Historic Scotland for reading the first draft, and to Janet Kleboe also of Historic Scotland, who braved the complete final draft and drove it onwards to final publication.
Context of report - need for conservation and compatibility requirements 1.1. Manufacturing of Lime Based and Ceinentitious Binders 1.2. History and Context of Mortars in Buildings
Repair Techniques and Specific Functions of Mortars Used in Conservation 2.3.1. Pointing, repointing 2.3.2. Rough racking
1.2.1. Earliest uses
2.3.4. Bedding mortar, replacement of rnasolsry units
1.2.2.Classical Greek and Roman Occurrences
2.3.5. Internal and external coating plasters, renders and their repair
1.2.3. Other world-wide occurrences
2.3.6. Plastic repair
1.2.4. The Renaissance to the 19th Ce~ltury:the development of hydraulic mortars and cement
2.3.7. Injection, grouting
DEFINITIONS AND FUNCTIONS OF MORTAR IN HISTORIC BUILDINGS
Co~lstructionof Stone Masonry Rubble masonry Ashlar lnasonry Roman masonry
Key Terms Definitions
2. l . l . Mortar
Definition of Conipatibility
2.1.2. Coilcrete Ro~nanmortar and concrete
Compatibility With Regard to Conservation Philosophical and Ethical Issues
2.1.3. Binders Lirne Non-hydraulic lime, air lime, air hardening lime Hydraulic l i ~ n e Cement Portland cement (PC), Ordinary Portland cement (OPC) Natural cement Pouolan, Pozzolanic material 2.1.4. Aggregate Sand
Compatibility With Regard to Physical, Chemical and Mechanical Properties Compatibility With Regard to Mortar and Masonry Interaction
ANALYSIS OF HISTORIC MORTARS
2.2. Classification of Mortars 2.2.1. Historic and modern mortar. original and new mortar 2.2.2. Distinction based nature of binder
Compatibility With Regard to Traditional Approach and Conservation Practice
2.2.3. Distinction based on the puspose of application
Sampling, Damage Diagnosis, Hypothesis Formation and On-Site Visual Analysis Methods Used for Technical Characterisation 4.2.1. Acid dissolution and wet chemical analysis
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSERVATI~N, TLCIINICAL AND SCIENTIFIC LITER,\TURt
4.2.2. Optical microscopy/ Petrographic analysis
5.3. Research into Nature of Mortar Properties 5.3.1. Porosity, pore structure & transport process
4.2.3. X-ray Diffraction (XRD) 4.2.4. Infra Red Spectrometry
4.2.5. Thermal Analysis (DTA and TGA, also known as TG) 4.2.6. Microstructi~restudies using Scanning Electron Microscopy
4.2.7. Electron Microbeam analysis
5.3.4. Bond between mortar and lnasoilry
4.2.8. Physical and Mechanical testing 4.3.
General Analysis Schemes
Characterisatioll With a View to Repair
'Secondary' carbonation and other reactions
5.4. Testing of Mortars 5.4.1. Examples of experimental studies and testing of mortars 5.4.2. Factors affecting the preparatioll of specimens and testing mortars Water Aggregate Casting Specimens into Moulds Workability Mixing Curing
DESIGN AND DEVELOPMENT OF NEW MORTARS
5.1. Specification and Performance of New Mortars 5.1.1. Examples of design of new mortars 5.1.2. Design based on composition and/or properties
5.4.3 Fresh mortars Workability Testing
Factors affecting the design of new mortar based on composition
5.4.4 Hardened Mortars Shrinkage Mechanical Strength Strain Testing Adhesion Bond Carbonation Porosity and Pore Structure Permeability
Factors affecting the design of new mortar based on performance characteristics 5.2. Lime-Based Mortars 5.2.1. General composition and strength
5.4.5 Durability of Mortars
5.2.2. Properties and compatibility of nonhydraulic lime mortars 5.2.3. Modern and traditio~lalrenders 5.2.4. Hot mixing 5.2.5. Ageing of lime putty 5.2.6. Addition of brick dust 5.2.7. Carbonation of lime mortars
5.4.6 'In-situ' testing of properties of mortars
MORTARS 1P HISTORIC BUILDINGS: A REVIEW OF
C ~ ~ S E K V I TECTINICAL \ I I O N , AND SCIENTIFIC I ITERAIUKL
CONTEXT OF REPORT - NEED FOR CONSERVATION AND COMPATIBILITY REQUIREMENTS This review document is intended to synthesise published inforination regarding research carried out into mortar materials, including bedding mortars, repointing mortars, renders and grouts as found in historic buildings, b ~ excluding ~ t clay or earth based materials. It will concentrate on masonry binders produced by the calcination (bunling) of limestone and impurities, either natural or artificially added, that produce non-hydraulic and hydraulic lime based binders, natural cements, Ronlan cements and inodern Portland Cements. However, it is also not intended to condense all the possible available information in one exhaustive book, but to select and organise a bibliography to cover the nlajor subdivisions of this developing subject. Additionally this review will include work published predominantly in English. The need for this review grew from the increasing interest paid to the study of mortars in historic buildings, both ancient mortars, original to the building fabric and their subsequent replace~nents.This not only covers traditional nlasonry binders such as nonhydraulic lime mortars, but also many hydraulic and artificial cements produced during the past two hundred years. As the built heritage of the past two centuries beconles increasingly valued in its own right the need for the conservation and understanding of a variety of binder, render and grouting materials has surfaced (e.g. Kirst et al. 1999). Increasing sophistication in conservation, mirrored by increasi~lg technical understanding of traditional, and other modern man-made building materials has resulted in greater den-rands for better performance of the tllaterials used in conservation and restoration, and their compatibility with the historic originals. Technical advances in analysis of old nlaterials and in the production and testing of new replacements promises the possibility of meeting these demands. The emphasis in this doculllent is on the analysis of the denlands of building conservation activities, their relationship with and influence on the choice and application of technical and scientific measures needed to fulfil these demands. In the following sections mortars as used in historic buildings are placed in their proper context historically
and technologically. Following this the concept of conlpatibility is introduced, as the driving force behind building conservation, and the steps currently taken by researchers and practitioners in the analysis of historic materials and the fornlulation and testing of their contemporary replacements. The third section will begin to review this analysis, firstly of historic Illortar materials, froin a conservation/practitio~lerangle and then from a technical point of view. The final section will cover the fonl~ulation of new replacement materials, and their testing and analysis, and consider to what extent this activity is indeed infor~lledby the analysis of historic buildings and their original nnaterials and a search for effective compatibi1it)i of replacements with original fabric.
1.1. Manufacturing of li~llebased and celllelltitious binders. The vast nlajority of binders in historic buildin,OS are made from lime. Historic Scotland's Technical Advice Note No.1 "Preparation and Use of Lime Mortars" (Gibbons 1995) states that lime is produced by calcining or "burning" limestone, and that lime inortars are made by "mixing linle with sand or some other form of aggregate". The basic processes of production and use of lime can be summarised in the "lime cycle" (Figure I ) . Lime can refer to different related materials, for exanlple materials with different chemical compositions. In the production of lime a source of Calcium Carbonate (CaCO,) in limestone, chalk, marble, marl, shells or coral, is calcined, (raised to an elevated temperature below its ~nelti~lg point) for a time long enough for the disassociation of Carbon Dioxide from the ~nineral lattice. This process takes place in calciurn carbonate at temperatures over approximately 890째C (Boynton 1980). Calciunl Oxide (CaO) or "Quicklime", is then produced which can be mixed with water, or "slaked" to form a workable putty composed of Calcium Hydroxide (Ca(OH)?, or Portlandite). This Inass can then be mixed with an aggregate to make a mortar which can be used for building. The inortar will then dry out and harden followed by a longer period of hardening and strength gain t h r o ~ ~ gthe h absorption of CO2 from the atmosphere, which returns the material to Calci~lnlCarbonate, this ti~llenot in a limestone, or other natural raw material, but in a mortar.
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSEKV,\I ION, TECIINICAL AND SCIENTIFIC LITERATURk
/ k, Water Aggregate Dry Hydrate, Lime Pufty Calcium Hydroxide
This apparently simple process is in practice a co~nplex one, as variatioils in the co~nposition of the raw materials and conditions and nlethods of application can alter the behaviour of the materials. Lilnestones vary considerably in composition, and are not often pure Calcium Carbonate. They can contain what are sometimes referred to, inaccurately, as "impurities", that is minerals of other compositions, most colnrnonly Magnesium Carbonates (Magnesite (MgC03) and Dolomite Ca: Mg (CO3)), and various silicates (mineral compounds containing SiO,), most often clays. The properties of lime will vary depending on the type and amount of colnpounds other than Calcium Carbonate in the raw material, but also on the temperature and length of burning. There are two basic types of lime used in building, non-hydraulic and hydraulic. Non-hydraulic limes are produced when limestone is used that is nearly pure Calcium Carbonate (at least 85% BS 890:1995), and call be referred to also as High Calcium Lime. Their production is typified by the lime cycle in Figure 1. Ilydraulic limes on the other hand are made from carbonate sources that contail1 a significant amount of silicate "impurities". These can be refened to as "Argillaceous" lirnestones, that contain quantities of clay. On firing within a kiln, a more complex set of chemical reactions take place that produce "hydraulic" compounds that give the material the ability to set in wet conditions (Gibbons 1995) or under water entirely. In addition to the fornlation of lime (CaO), the co~npoundsthat forlll are Calcium, Aluminiuill and Iron Silicates (C$ Alite, (3C2S Belite, aC2S Felite, C6A2F- C6AF2 Celite). These are also the main constitueats of Portland Cement, and react with water to generate a chemical set. The degree to which each of these components is formed depends on the original
compositio~i of the raw materials and on the temperature and length of time of kiln firing (Ashurst 1998). The controls on the formation of hydraulic components are well understood, due to the huge interest in the properties of cement and the large aiuount of research done over the past 100 years (e.g. Hewlett 1998, Soroka 1979, Taylor 1990). 111 cement production tenlperatures of up to 1450째C are used. Sintering takes place at this temperature and a recrystallised clinker is formed which is ground to form a usable powder. In addition, the raw nlaterials are finely ground and well mixed in a slmry before firing or used direct as a dry powder. Traditional lime production methods employ rnaxi~llumtemperatures of around llOO째C, and often lower. The raw materials are also not ground to ensure thorough rnixing of calcareous and siliceous components, meaning that the natural distribution and type of silica and carbonate are inlportant in determining the final composition of the lime. The lower te~nperaturesused in lime production favour the formation of certain hydraulic compounds over others, particularly Belite (C,S forms <1250UC) over Alite (C,S forms >1250째C). This means that even if a hydraulic lime has the same bulk chemical conlposition as Portland Cement it would behave differently, because Belite hydrates and gains strength differently from Alite. The time of burning is also i~nportantin determining the nature of a hydraulic lime. The St. Astier company in France currently produce three types of hydraulic linle from a single stone type, the difference being controlled by lengthening the burning time and not the temperature reached. The relationships between the chemistry of the raw materials and the temperature of production are
described by chemists in "phase diagrams". These record the characteristics of chemical reactions and the stability of different compounds dependant on the composition and temperature and allow the prediction of what will be formed from processing materials through a kiln. The phase chemistr~iis well covered in standard texts on Cement Chemistry (e.g. Hewlett 1998, Taylor 1990) and will not be collsidered further here. It is possible therefore to produce a wide range of materials with differing degrees of l~ydraulicity.These are classified as feebly, moderately and eminently, depending on the content of hydraulic components, their speed of set and eventual strength. There is a fundamental, continuous compositional variation running from pure non-hydraulic high calcium limes to Portland Cement. Historically, the use of local limestone resources that vary compositionally on a regional scale will have resulted in a variety of lime types being in use, with each area having its own lime type. Overall, traditionally produced historic materials will be more variable than modern materials, from place to place related to raw material characteristics. Modern industrial high calcium lime production operates at temperatures of around 1250째C to reduce calcining times. Current production in the UK is almost entirely non-hydraulic, high calcium lime, made not for construction, but for the demands of the chemical industry. This material is very consistellt and produced using large scale processes and very efficient kilns. Boynton (1980) and Oates (1998) give a very thorough treatment of limestone extraction, processing and calcination, particularly on an industrial scale.
1.2. History and context of mortars in buildings When considering mortars in historic buildings it is useful to have an understanding of the history of their compositional development and use. On approach to a building of known age, an early expectation of the nature of the mortars can be formulated, and tested once the mortars are examined. Conversely, if the building is not well understood, the type of mortar may help to constrain its age. In general however, natural hydraulic binders and modern cements are not common in structures before the 19th century, when these began to be deliberately manufactured. Most mortars will consist of a lime based binder, of a varying degree of hydraulicity related to local limestone characteristics. Gypsum mortars and additions of gypsum to lime based mortars are known (e.g. Middendorf 2001) in certain circumstances, but are not generally very common. In Scotland dry stone construction was the norm for indigenous peoples for many thousands of years and the earliest mortared buildings contained earth, used primarily as a waterproofing agent to improve internal conditions (Maxwell2000). Lime was
presumably introduced to Scotland by the Romans, allnost 2000 years ago, but the technology apparently disappeared after they left, only to be reintroduced at the end of the first millennium. This part of the introduction will outline the international history of cementitious binders as revealed by selected literature. The focus here will be OII demonstrable occurrences verified by direct observation, sampling and analysis. Many of the publications discussed are arcl~aeological in nature, and the discussion below often centres on the assu~nptionsmade and the processes used to analyse and verify material occulsences.
1.2.1. Earliest uses In a study of Neolithic lime plasters, Gourdin and Kingery (1975) identified lime processing dating from 7000-6000BC, from sites in Anatolia, Syria, Turkestan, Sinai and Jericho. The materials examined were predominantly wall and floor plasters and ornainents. The importance of this study is that they established that at this time only very rudimentary ceramics were found associated with some of the sites and that the societies that were producing the lime were "aceramic", that is the production of lime predates the development of ceramics firing technology. The production of lime requires a larger technological expertise than for the production of gypsum plasters, needing temperatures around 850-900째C compared to 100-200째C for the formation of the hemihydrate form of gypsum plaster. The volume of material needed at Cayonu, Anatolia (6500BC), is in the order of 0.67 m3 of recarbonated lime, requiring the calcination of 40001bs (1816kg) of limestone. Approxin~ately 1000 lbs. (454kg) would be required per house. They postulate that rudimentary kilns must have been employed for the production of the lime, and that this provided some sti~nulusfor the rapid development of fired pottery. In a later paper Kingery et crl. (1988) identify the "invention" of lime calcination and plaster at around 12,000BC. They extended and reapplied the methodology adopted by Gourdin and Kingery (1975) in comparing ~nicrostructuresof materials to identify processed carbonated lime. The oldest material, dated at 12,000BC, is an adhesive used to fix a stone blade to a wooden shaft. Other non-architectural uses of lime and some gypsum "plasters" include storage jars, coatings on pottery and other jars, plaster balls, plastered skulls and sculpture. In a cave site dated to 10,400 - 10,000BC, the remains of what is co~lsidered to be a lime burning hearth were found, conlposed of rounded structures with a 20cm thick layer of white porous material. Examination of this material by Scanning Electron Microscopy revealed a microstructure of li~nestonefragments surrounded by
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF TIIE CONSERV~ITION: TECHNICAL AND SCIENTIFIC I.ITERI\TUIIE
small calcium carbonate particles - clearly interpreted as a processed lime structure. Kingery ef rrl. suggest this as the earliest example of the production of quicklime. The architectural plasters examined include floor coverings, wall plasters and one case of a benchlike structure. The floor coverings were often of a single layer, polished 011 the top and comnionly grey or white in colour, with the exception of one from Catal Huyuk which consists of up to 50 layers of 0.5mm thick. Others can be red in colour or contain larger pebbles as aggregate. Another contains the recycled red stained fragment of a previous floor covering. Blackmall (1982) exanlined the occurrence of lime plasters in Anshan, Iran, dating froin 3500BC. As with most of the papers already discussed he suggests that clay or earth plasters were superseded once the thermal alteration of natural materials was discovered that could produce more durable gypsum and lime. He also concurs with Gourdill and Kingery (1975), that the identification of processed plasters is difficult because they are cliemically identical to tlie raw ~naterials,and that closer textural analysis is required. After Gourdin and Kingery's identification of lime plaster technology at 7500BC it is not surprising that the settlenlent studied dated at 3500BC also shows similar evidence. Their purpose was to document the occurrence, distributioli and function of the materials. The materials were classified into four forms: portable (bowls etc), decorative but non-structural (wall plasters, including coloured varieties), structural and waste products from the processing of lime and the construction process. Some bowls were exanlined and found to contaill Calciuiii Hydroxide - tlie hydrated forin of quicklime. Blackrnan interprets this as "..direct evidence for burned lirne plaster at Anshan". So~lleplasters are multi-layered and colo~lredwith pigments, and on closer aiialysis Blackl~ialiidentifies it as fine grained quartz and carbonate, "finely gro~11idiiicolnpletely calcined lime plaster to which no material other than pigment has been added." He does not adequately explain why tlie quartz is not deliberately added as an aggregate, as we might expect in a wall plaster. Lime was not used to bed tlie nlud bricks used to build houses, but rather a inixture of mud and straw. Lime is reserved for use in decorating and plastering interior walls and floors, where it is soinetinles ~ilixedin with rrlud to increase strength and rrioisture resistance. On co~lsidering the social and technological implications of the evidence of lime burning at Anshan, Black~lian likens lime production to contemporary activities in tlie area, where liiiie burning is a sunllner activity. He postulates that li~iieburning would have taken place only durilig the building season, and no stockpiles of material would have bee11kept, due to the difficulties of preserving tlie material during the winter. Blackman states that calcined and slaked lime must be kept dry, to avoid spoilage, thus preventing stockpiling.
This reveals some lack of understanding of the real nature of the material, especially as once slaked, even to a dry hydrate, quicklilne call hardly be spoiled further. It also shows a tendency for tlie Archaeological writer to interpret past events with reference to current practice. Blackman concludes by stating that fill1 time li~neburning specialists were not needed. However, as lime burning appears associated with ceramic production it is reasonable to suggest that these activities were performed by the s a n e people who were experienced in pyrotechnology. Lucas (1948, first published in 1926), in an oft quoted description of the nature of the mortars used in Egypt prior to tlie Ptolomaic period (before 285BC) states quite categorically that there is no "..instance of the use of linle mortar in Egypt, or of lime in any form .. known to the author.." The mortars and plasters analysed by Lucas are con~posedof Gypsum, which is co~i~inonly found as a cushion between large dressed blocks of stone. Wall plasters were of tlie same composition and can be coloured depending on their constituents. He also states that the finishing coats of plaster can contain a large proportion of calcium carbonate and very little gypsum. This could be "poor of gypsum and quality" gypsum, a deliberate rnixt~~re calcium carbonate to produce a white colour or material processed from the naturally occurring gyps~1~11 deposits which often contain a significant proportio~i of carbonate. Occasio~ially it is just a "whitewash" that contains no gypsum at all. It is surprising that Lucas could not accept the possibility that this calcium carbonate whitewash could be lime, and that lime and gypsum plasters could have been lnixed to alter the properties of tlie material. Samples of Egyptian Plaster froill Tiillna (dated 14001200BC) were identified by Gourdin and Kinger)! (op. cit.) as lilile plasters mixed with quartz sand in a 1: 1 ratio. This discovery contradicts Lucas's (1948) assertion that only gjipsum was known before 285BC i ~ Egypt. i Gourdi~land Kingery (1975) also refer to other analysis that shows lime was used in tlie Cheops Pyramid as well. Gourdin and Kingery's (1975) work is also interesting in the context of historic Inortar analysis. They take an ailalogous approach to the identification of historic processed gypsunl and l i ~ n e materials and their separation from natural limestone and gj~psu111 deposits. This is important because the natural and processed nliaterials are chemically indistinguishable. They conclude that Lucas's examination was only cursory and his silnple analysis was insufficient. They visually compared the microstructures of processed g)/psum and lime with their natural counterparts and use this to positively identify the nlatrix of several samples as being of recarbonated lime. Differential thermal analysis (see section 4.4.6 ) was also applied to sa~ilples of l i ~ n e plaster and natural limestone. A displacement of the peaks was found between the
~naterials which suggested that calcined and recarbo~latedlime call be distinguished in this way from its natural raw material. Mixtures of the two produced an intermediate peak position. However, they did not speculate on the general applicability of this method in distinguishing between natural carbonate and recarbonated lime. In probably the earliest paper on the analysis of historic mortar, Wallace (1865) looked at the composition of nlortars from Egypt, Cyprus, Greece and Rome ageing from 3000 to 1600 years old. The Egyptian mortar, from the Pyramid of Cheops was found to be of gypsum, in support of Lucas's later claims. The other Illortars were found to be of lime, and the Roman Inortar to contain pozzolana and a large quantity of silicic acid. Wallace concludes that lime ~ I Imortars of this age are completely carbonated and do not form a mixture of Ca(OH), and CaCO?, and that where they have been exposed. weathered or especially kept wet during hardening; that alkali-silicate will form, which may confer additional durability and hardness. Despite Lucas's (1948) assertions, lime was being used contemporaneously with co~lstructionin anciellt Egypt. Kleinln & Klemm (1990) explicitly challenged Lucas's versioll of mortar occurrence in the old Kingdom of Egypt before the Roman Occupation, finding lime used alongside gypsum in mortars from early structures, though the pattern does vary. They also consider one of Lucas' assertions that lime was not used due to a scarcity of fuel to burn at the higher temperatures required, near 900" compared to 450째C for gypsum. They also detected a very fine quartz intergrown with carbonates in some mortars dating to around 2490 BC. These could be interpreted as decoinposition products of the hydraulic mineral C$, however this is ~mcertain, but indicates the possibility that the a~lcientEgyptians could have discovered and controlled the production of hydraulic lime mortars. During the late 1980's a controversy developed over a theory that the Pyramids in Egypt were actually co~lstructedfrom a form of "geopolymer" concrete. This was put forward by a respected ceme~ltchemist J.Davidovits (e.g. 1987). However, this attracted a co~lsiderableamount of criticism and has been the subject of detailed criticisin (Folk and Campbell 1992).
1.2.2. CIassical Greek and Ronzarz Occurrerzces It is generally held that the Greeks began the large scale use of lime-based mortars in Europe and it was from there that the technology spread to Ronle (Davey 1961). Evidence exists for Greek use of li~lle in hydraulic worlts, for example a 7th century BC water channel at Olympia, and for the li11i11gof aqueducts and cisterns (Dix 1982). In particular, the Greeks, and
especially the Romans. are credited with the development of hydraulic nort tars, through the use of inortar ad~nixtures,usually volcanic ash, crushed brick or pottery, that resulted in a faster and stronger set and also made the mortars resistant to the action of water. However, there is evidence that earlier societies, such as the Phoenicians (Baronio et al. 1996) and the Minoans (Blezard 1998), knew of these effects. Co~lophagos (1982) presents an example of early sophisticated use of lime mortars in Ancient Greece around 500BC. Mortar was used as a waterproofing for cisterils a11d other ore enrichment facilities in an ore s~neltiilgplant, that produced silver and lead. Two layers of mortar were used: the first being conventional, that used poor ore and tailings from the washi~lg plant as aggregate. The second layer comprised very thin layers of a hydraulic plaster. Analysis of this shows a very high content of lead, manganese and zinc oxides and XRD analysis showed a diffuse spectrum indicating the presence of glassy material. It appears that lead oxide was added to the mortar in quantities of approxi~nately 20-30%. The mortar without the waterproofing has normal permeability but the thin outer layer has zero permeability. Further lab experime~ltsfound that this mortar could be made by first pouring molte~llead oxide into water, produci~lg a glass, followed by powdering and addition to lime plaster. This indicates an early advanced understanding of the relationship between ~naterial properties and fu~lction in the Ancient world. However, it was the Romans who developed the technology of building with burnt-lime nort tars to a very high level. They were, however, ignorant of the chemistry of what they applied (Baronio et al. 1996, Harries 1995, Blezard 1998) but developed a sophisticated empirical understanding of the effects of ~roduction methods and mortar additives. Roman progress in construction using mortars and their most significant material, concrete, is considered by Inally to go hand in hand with social and eco~lomicprogress as the empire grew (Harries 1995, Lechtman & Hobbs 1987). Dix (1982) reviews the productioll of lime by the Romans, providing a valuable overview of the nature of different kilns in use at the time. Most were "flare" kilns where fuel and stone remained separate, and calcination of li~llestollewas by radiant heat from a fire ~naintainedbelow the stone, not intimately mixed with it as would occur later. Dix also discusses the development of concrete, or 01111s c a e l ~ e ~ l t i c i lThis i~~. nlaterial was not widely used until the final ce~lturies BC. Mortars were coill~nonlyused, but Etruscan and Greek building did not require large quantities as illost buildillgs were caref~~lly crafted fro111 precisely cut
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF TI1E CONSERV.ATION, TECHNICAL AND SCIENTIFIC LITERAI'URE
stone, mortars only being used for reducing the friction between blocks and for cushioning. The hydraulic properties of mortar were perhaps first identified in the 7th Century BC, where they were used in a water channel in Olympia. Again the Greeks used lime to line aqueducts and cisterns in Sicily, where perhaps the Romans first encountered its use. Lime-based concretes were perhaps not developed until the 3rd Century BC. The earliest apparent uses, or at least the foreshadow of concrete, was in Cosa, used for rubble masonry house collstruction and at Pompeii, where rubble construction, again of houses, using pozzolanic volcanic sand allowed stronger walls to be erected to Inore than one storey. Other buildings at Pompeii and Ostia (where housing developments sprang up) were walled in concrete from the third Century BC (Dix 1982). Early in the second century some temples had podiums of concrete and hydraulic limes were being used in linings. In the third Century BC lime mortars recommended for houses and for floors where reinforced by hydraulic additives. By the end of the second century concretes were commonly incorporated into the foundations of major temples in Rome, and from there their use extended to more public and domestic buildings. Vitruvius, however, doubted the reliability of Roman concrete, by the close of the first Century BC concrete was well established along with mortars and various kinds were in use (Dix 1982). Lechtman and Hobbs (1987) describe how the advent of monolithic concrete construction heralded an architectural revolution, where building forrn became moulded or "cast to shape" rather than assembled. This paper discusses the form rather than the chronological history of concrete construction in Roman ti~nesand there is also a detailed survey of hydraulic binder chemistry and reactions. However, Roman construction was quite distinctive, none more so than in the use of concrete. This material permitted the use of relatively unskilled labour to erect large structures rapidly. Form-work was erected and concrete layered to form building masses (Hawies 1995). Eventually wooden form-work gave way to brick, but the cores of walls remained composed of a lime-pozzolana concrete.
Roman concrete is a mixture of mortar and with a coarse aggregate. Sand was probably screened for size from the beginning of the E~npireonwards. Sand type appears to have been important to the Romans. Vitruvius recommends the use of "pit sand", a sharp clean sand, considered better than river or sea sand. Lechtman and Hobbs (1987) contend that "pit sand" was clearly pozzolana. Concrete was placed by layering, and ramming where possible, and so was essentially a form of rubble lnasonry construction. Aggregate varied from rock, commonly volcanic or
pozzolallic in nature, to fragments of demolished buildings, ceramic tile or crushed brick (Lechtman and Hobbs 1987). Pozzolana is esse~ltially volcanic ash, composed of aluminium-silicates that are reactive when in contact witli lime, produci~lga network of hydrated calciurn and aluminium silicon hydrates, that bring about a strong set in a mortar or concrete, and allow the111 to be placed under water. It is named after the town of Pozzuoli on the Italian coast near Naples, where it was first used in mortars and concretes for the construction of the town harbour, in the first half of the seco~ld Century BC (Lechtman and Hobbs 1987). Material was exported widely from the region for numerous harbour projects. It is in the developmetlt of harbours that the Rornans gained their first experience in the handling of concrete. Between 22-9BC King Herod built what was the largest harbour of the age at Sabastos, 45 km south of Haifa (Oleson et crl. 1984). Artificial breakwaters were constructed of enormous concrete blocks on a bed of loose rubble, that ellclosed an area of some 20 hectares. Much of the materials used were imported from as far away as Italy, including the reactive pozzolana sands. Some of the concrete blocks have a volume of up to 125in'. The remains of sophisticated wooden form work have been found, that have hollow wall sections and no floors. They are interpreted as being floated out into position and then the hollow walls filled witli mortar to sink the moulds. They were then filled wit11 concrete and left in place. Concrete remained a material primarily used for hydraulic works until the 1st and 2nd Centuries AD. Considerable experience had been developed in this application, but Letclman and Hobbs (op. cit.) bring into question how the Romans transferred this technology to large vaulted buildings. Form work for buildings became standardised on brick or stone, from the end of the second Century BC (Harries 1995). However, it is clear that progress in application was slow and incremental as the quality of the Inortars and concretes used was not always high. By 40BC, during the reign of Julius Caesar, construction had become more reliable, based upon a better choice of materials, and their Inore sophisticated use. This includes the selection of aggregates depending on the building element being constructed, lighter aggregate being used for walls and denser for fou~ldations.During the period from 120BC until Nero built his Do~nusAurea in 64-68AD, which made much use of concrete, slow empirical progress took place. The paper by Letchman and Hobbs is aa excellent survey of Roman concrete technology. Harries (1 995) points out that Ro~nallaggregate of 50150mm, could not be mixed manually, so concrete was
MORTARS IN HISTORIC BUILDINGS: A KEVIE\I1 OF THE CONSERVATION, TECHNICAL AND SCIENTIFIC LITEKA~UKE
placed in layers by hand, resulting in a higher mortar: aggregate ratio than today. This different form of construction of brick-filler-brick changed the structural stability of constructions, as they were now essentially inonolithic. Brick arches were built in to strengthen vaults and left as an iinportant elernent of the concrete mass. Bonding courses were also common, throughwall brick tiles every 15-25 courses. It is doubtful if they actually served this bonding purpose, being more likely to have marked the end of a day's concrete placement, or for levelling. However, the bonding courses do have the effect of preventing seisinic damage, by absorbing energy through encouraging relative nloveInent between bonded units. Domes were the major architectural innovation of Roman Construction. Constructed over formwork, carefully graded aggregate was used from heaviest at the bottoni to lightest at the top. The dome would also thin toward the top reducing the weight of the structure further. The Pantheon in Rome (128AD) is the most i~npressiveexample, and relies partly on its immense concrete ring foundations (4.5111 deep by 10.3m wide) for stability in such a seis~nicallyactive region. During the late Roman era and into the Byzantine period, nort tars were co~nmonlyproduced with crushed brick aggregate which acted as a pozzolana. The joint thickness of brick wall facings also increased from 10mm to 70mm (Baronio et rrl 1996). Aggregate size also increased to up to 251n1n in these mortars. The role of the thick mortar joints is not entirely clear but they do allow greater deformation of a structure without catastrophic damage, especially at an early age, thus allowing settlement of differcntial movement (Binda et 01. 2000). Despite the preponderance of pozzolanic mortars in Roman Construction and their hydraulic properties there is little evidence that they deliberately calcined limestone to produce hycllziulic Dinrler S . Mishara (1982) reviews the con~positionof artificial Portland Cements and natural hydraulic mortars, and considers to what extent bindel. inanufacturers in the ancient world deliberately produced hydraulic binders. She asserts that evidence for this is missing. Pozzolans were used extensively and clearly deliberately, however, documentary evidence of the time warns builders away froin the use of "grey variegated" stones - those that nlay well have produced hydraulic binders. For exanlple Vitruvius in 'The Ten Books on Architecture' (Morgan 1960) writing around 25BC described how to use lime and prepare mortars;
n7i.v ~ ~ ~ rniortcrr; r r . i f usir~gpit scrrlrl, in the pr.011ortion.s of three pur.ts cgsarlcl to orre o f lilue; if l(si11g1.iver. 01. sea-sancl, 111i.v t 1 1 ~parts of .scrncl 14~itl7one of lir7le. Tl~leses ill be right p~.ol~or.tiorl.s for. the conlpositiorzs of the 117i.vtz/re.F~rr.ther;in. ~rsir~g r.i~,er. 01. sea-sar~clthe arlclitior? of thircl pcirt con~l~oserlof brrrnt brick, pol[r~clecl1/11 ari7cl sifted, will nmke yo~rr.111ortc11. of cr betrer con2positior7 to me.' This work set, for that time, very iinportant standards but also certain prejudices towards non-hydraulic and hydraulic mortars. It was believed that only the hardest li~nestonecould be used to produce hard and durable inortars. (Sickels 1987). Portland cement manufacture depends on the forination of clinker, which needs to be ground to a powder before use. This would have been difficult in allcient times, and large lumps of clinker would not have performed very well, putting inany users off. Vitruvius advises that the "best white stone" be chosen, and advice is given to avoid lnixtures of limestone and clay. Mishara suggests that the analysis of artefacts Inay allow us to decide what people actually knew and what influence advice like Vitruvius had. Relationships between materials and building patterns nlay allow a judgement of whether considered choices had been made to select a particular material for a particular job. The link with ceramic production, identified by othess (above) may be very strong whese the use of artificial pozzolans is concerned. The techniques and materials of Roman construction are well researched. The publications mentioned above only cover a sinall fraction of the available literature. The intention in this section was to give the reader some idea of the breadth of the subject and of the basic chronological evolution of Roman mortar and concrete technologies.
1.2.3. Other world-wide occzcrrerzces The use of lime-based nlortars through history is not limited to Europe, Northern Africa and the Middle East. Malinowski (1981) notes their use over the past 2000 years in the Great Wall of China, monuments in India and in Central America.
Lime was extensively used by the Mayan civilisation in Central America, or "Mesoamerica". Littman (1957) comlllents that the use of lime is restricted to that area, and is a distinguishing feature that Inay have played a role in the development of "more advanced forms of architecture" compared to other parts of the New '. . . , ne.vt ~ i ~ i~.e,qrrr.r( th to lir~leM>eI I ~ L [be S ~ ccrrq'irl tl~at World. In the samples he collected from the steps of a Maya temple at Comalcalco, Mexico (dating to it is bur.r~t,fi-or~z cr stor2e 14,11ic11, ~ ~ l ~ e t l soft l e r .01. hm.rl, it is irz a17y ease ~112ite.Li171e r~~crcle of close-g~.ainccl approximately post 200 AD). Littman identifies lime storze of the Izrr~.clersort 14,ill be good in str.~rctlirvl plasters, wash coats and "lime-aggregates" (monolithic pcr1.t~;Iinze nfpor.o~/sstone, in sfzrcco.After slcrkirig it, lilne masses). On analysis of these he found that the
MORTARS IN HISTORIC BIJILDINGS: A RE\'IE\V
reaction between silica and calcium, increasing strength and increasing control and uniformity of manufacture. The development of the rotary kiln around 1878 (Davey 1962, Bye 1983) is perhaps the most critical step in the production of modes11 cements, resulting in a high degree of controllability and uniformity of product. From then on, the higher temperatures used for production produced a very fast setting cement, so from 1890 Gypsum has been added in a small quantity to all Portland Cement as a set retarder. Since then, in modern building, cement based mortars and concretes gradually replaced the limebased mortars. After the invention of Portland cement, research has concentrated mainly on its development and a new, 'modern' way of building has begun. Cement mortars were considered better, stronger, more durable and with a more reliable hardening process than lime-based mortars, which were soon superseded by the cement gauged or pure cement mortars. Approximately from
COWSERI~ATION, TECI-INICAL AND SCIENTIF~C LIEKATGRE
the First World War onwards celllent rich mortars and renders were used in the repair and restoration of historic buildings (Busman 1998), where they had most often not been part of the original fabric. It was only after serious failures, where inappropriate use of the cernent rnortars apparently damaged the valuable original masonry, that a growing interest in lime-based mortars reappeared. However, the advent of Portland cernent as the dominant mortar binder during the 20th Century, resulted in all research efforts being focussed away from lime-based mortars, and particularly its use in building conservatio~~. This was redressed partly by events like the publication of the Venice Charter (1964), that was approved during the 2nd I~lternational Congress of Architects and Technicians of Historic Monuments held in Venice that year. Although it did not affect directly the use of mortars, it set out conservation a ~ l d restoration principles that supported scientific research to underpin the better conservation of the architectural heritage.
MORTARS IN HISTORIC BUILDINGS: A REVIEW
OF 'THE CONSERV,~TION, TECHNIC.\L AND
2 DEFINITIONS AND FUNCTIONS OF MORTAR IN HISTORIC BUILDINGS
The use of Inortars (bedding, rendering, grouting etc) deteriniiles their function (structural, protective, decorative etc.) within the structure. The inortars are required to possess certain properties imposed by their use. Careful consideration of the use, f~inctions, classifications and materials used in mortars of historic buildings is very important for the effective analysis of historic mortar properties as well as for the specifications of modern mortars. The way in which a definition is expressed for~lls and limits the understailding of the defined material. Therefore, definitions vary according to their purposes. Definitions in standards (e.g. British Standard) are usually limited to a minimal description of the compositioil of a material. Next to these basic standard definitions there are definitions incorporatiilg correct use and desired property of the material. Such detailed definitions are often needed in practice to provide further explanation according to a particular area of study.
The aim of this short co~nparativestudy is a discussioil of basic definitions related to mortars and lllasoilry conservation. On the other hand it is not to form new precise definitions or to list and cover all definitions related to this subject. The key terms were already defined and published in special technical dictionaries and standards (e.g. Walker 1988, BS 6100: Glossary of building and civil engineering terms) or as a terminology of scientific and technical literature (e.g. Holmes and Willgate 1997: Sickels 1987). These publications should be refessed to for a full list of terms and definitions.
In this definition the main objective is on the requirement for workability (albeit trowelled is not a very exact requiremeilt) and description of the use of mortar. It does not specify any material requirements. On the other hand, a definition presented by Goins (2000) is more explicit about the cornposition of mortar. It states that mortar is:
2.1. Key terms definitions Definitions of the most relevant terms such as 'mortar', 'concrete', 'binder', 'cement' and 'aggregate' are discussed and often more than one version of the definitio~lis presented here to cover all aspects. The intention is to review all these viewpoints. It also aims to highlight discrepancies between terms caused by their different comprehension in different contexts. For example, Goins (2000) pointed out that the term 'mostar' is ambiguous as it ineans a co17lpounrl that holrls hlocks of i71~soiz1.y as well as having a broader meaning of m ~ 11istoi.ic y cenlelit a ~ i dcrggi.egate.
The analysis of various definitio~lsof mortar illustrates their interrelation with their purpose. The 111ost general definitioil is stated by British Standard (BS 6100 part 6.6.1:1992 Building and civil eilgineeriilg terms). It defines mortar as: 'Mixture of Diiiclei; fiile aggi.egate ailcl \t)atei. tl~at hai.clens.' The definition states the general inortar coinposition and process of hardening but it leaves out the use, functions and properties. For building practice, however, there Inay exist a need to extend this definition and express additional requirements. Holines and Wingate (1997) define mortar from a more practical point of view as: 'Aiiy i71ute1.ialin a plastic stcrte vt~hichccr~~ be tl-on~ellecl, beconzes hu~.cl in place, allcl uhicli can be itsecl foi. beclcli~lingand jointirlg 17iasoii1.y~iiiits.'
" A pas^ szlbsta~icefo1.17ierl1i(jrr11allyby the 171inix-i11gof cer7lerit, saiicl crilcl watei; or. cei~ieiit,lime, saiid ailcl ~'crterin varyi~zgpr.ol~o~.tions. Usecl iioi.nzally for the 17i1zcling of b~.ickwo~.k 01. nlasoii~y," from Cambridge Dictionary of Science and Technology (Walker 1988). The RILEM Technical Committee- 167 COM 'Characterisation of old mortars, with respect to their repair' discussed a detailed definition which would explicitly express even quality requirements for the inortar. It states that: 'Mortm is a 111i.y of ( I I ; ~ C I I I ~ CN I I ~i ~ i o ~ ~ a ibiiidei.~, iic 11icii111yj5fille aggregates, water. aiid crcli~iist~riesur~d organic ailcl iiioi.gaiiic d d i t i ~ i e si71ised , in o~.clei.to gi~,e to the fi.esh nlo~.tal.a goocl ~ ! o ~ . k a h iallincl l i ~ to the kcrrcleiiecl 17101.tc11.adeqzlate physical (l~orosit)~, ~~apolrl. pei~i7iecrbilit)~ etc.) rr~irl niechcri~ical (sti.eizgt11, ~lefo1~17icrl7ility, aclhesion etc.) beka~~iozri. crild goorl alq~earai~ce aiicl h(l.abilit~1.'
MORTARS IN HISTORIC BUILDINGS: A REVIEW Or T l l l CONSER\ ITION. TECHUICAL A N D S C I LI1~ICI LITrR?\TURE
This definition is the nlost relevant for mortars ill historic buildings and conservation. It is based 011 findings fro111 a recent research into requireme~ltsfor a compatible mortar used for conservatioll of masonry. The words such as good workability, adequate physical and mechanical behaviour and good appearance need to be defined further according to the use and required function of the mortar.
2.1.2. Concrete British Standard (BS 6100:6.2:1986) defines both mortar and concrete in a similar way. However, there is a distinction between them as concrete contains hydraulic binder and may or Inay not colltaili fine aggregate. The BS defines concrete as: 'Mr\tlo.e of aggregate, 11yclr.crulrcb~rlclercrrlcl lisrrter:thcrt I~ardens' Hollnes and Wingate (1997) use the distinction based 011 the size of aggregate. On the other hand, Goins (2000) pointed out that the terms 'mortar' and 'concrete' are used interchangeably. I11 historic structures a nlassive wall was often built as a multipleleaf wall with a mortar/concrete infill containing a larger aggregate and stones. Strictly by definition, it should be called concrete, however, the word concrete is more associated with Portland cement. For historic structures where lime based mortar was used it is Illore common to call it mortar. Terms such as 'Roman ii~ortar','Roina11 concrete' and/or 'natural concrete' are also terms which are used to describe illfill inortar based on hydraulic binders. Any illisconception should be avoided in the case of concrete made from modern Portland cement. Ku~narMehta and Monteiro (1993) define concrete as:
Their definition describes concrete from a structural and functiollal point of view rather than by its coinposition. This definition indirectl}! suggests something that is omitted in the previous two definitions. Unlike mortar, concrete Inay be used by itself to build structures. Mortar is used for jointing masonry units or for their surface coating. Rorllnr~iMor.far.arlcl Corlcr.ete There is more than one description of 'Roman mortar' and/or 'concrete'. In general it contained lime (could also have been hydraulic), sand, a certain amount of pozzolana and often also pulverised bricks. A nu~nberof different Roman building techniques have been described (e.g. Vitruvius). For example, Opus
Caernenticium is a name for a building technique used bp Roman builders when 'Roman mortar/concrete was used to set undressed stones called caementa' (Sickels 1987). 2.1.3. Biizders Binder is defined in the British Standard as: 'Mater-ial ~rscclfor- tlle p~rrpo.se of holclirlg solicl par-ticles fogether. ill r c.olzer.erlt 171crs.s.' (BS 6100:Section 6.1). This definition covers the lnost colllrnonly used Portland cement but also lilne or clay. This term is in solile cases interchangeable with the term cement. Binder can be subdivided by its hydraulic nature into hydraulic binder and air hardenilig binder. Linle Lime covers a wide range of lime products such as hydrated lime, l i ~ n eputty, quicklime, hydraulic lime, non-hydraulic lime (air lime) etc, in general 'all of the oxides and hydroxides of calciunl and magnesium, but excludes the carbonates' (Holrnes and Wingate 1997). The 111ost fu~lda~nelltal distinction between building liines is the same as for binders and that is their subdivisioll by hydraulic nature. Norl-Hydrn~rlicLir71e,Air. Lime, Air. Hcr7.clerlirzg Lir~le Air hardening lime is defined by prEN 1996 as: 'Lirlle 17lair~lyconsisfir~gof a calcilrn~ osicle or. hyclr.o.\-icle ~jlhich,uherl ir~co~po~.ated ir~toa ~liortcr~. 171i.v, slon~l~l lirrr-clens ill crir by r.eacting ~ v i t latr~losphe~-ic ~ ccrr~bor?cliosirlc. Ger~ernllythey clo 11ot h u ~ ~ c ~rrlcler. le~~ M ~ N ~ CNS I . tlzey lirr~~e no hydrnlrlic pr-oper.fies.'
It is a hydraulic binder. 'It sets and hardens by chemical interaction with water and is capable of doing so under water.' Defined by BS 6100:Section 6.1. Hollnes and Wingate (1997) define Hydraulic limes as Class C limes. They 'NI-cncrt~ir~crlIlycl~.altlic lin~espr.epcrr.er1 ,fi.oru lir~?estorzcor. cl~all~s with c l w ir71p~cr.itie.s.Ar.tiJi'cinl hyrlr.rrulic lir~lescr1.e r~~crr~~facr~o~ecI by 111i.virigporrolcrrl ~ ' i t hC C I ~ C ~ I ~ I7yclr.osirle III ~ ~ h i cerlcrhle h the liriles to hnrrlen elwi in dcrr~lpco1zc1irion.s.' Hydraulic lililes are classified accordillg to their quality. Hughes & Swan (1998) pointed out some discrepancy between current systems of classifications. They explained that Vicat (reprinted edition 1997) classified hydraulic limes according to their setting
MOIC~ARS IN HISTORICBUILDINGS: A REVIE\\'
tiines as feebly hydraulic, (moderately) hydraulic and enlineiltly hydraulic. Eckel (1922) shortens the classification to feebly and eminently based on cementation index 0.3-0.7 and 0.7-1.1 respectively. Cementation index was also used by. Boynton (1980) . *ho divided lilnes illto feebly (0,3-0.5), (0.5-0.7) and emi~lently (0.7- 1.1) hydraulic. On the otller 'land British Standard (DD ENV 459-1: 1995) uses a system of classification based on coinpressive strength where, for example, the denomination HL 2 coisesponds to the compressi\~e strength from 2 to 5N/mm2 at 28 days (Holmes 1998). These classification systems are contradictory for sonle hydraulic limes, and for conservation purposes an impro\red system based on actual perforrnance would be beneficial (Hughes & Swan 1998).
CONSERVATION. TECHNICAL AND SCIENTIF~C LITERATURE
Natzri.al Ceiile~lt The distinction between natural ceinent and Portland ceinent is expressed in the definition of cemeat by Holn~esand Willgate (1997). Goins (2000) defines n a t ~ ~ r ceinent al simply by its composition and stresses that it is a natural mixture: 'Macle 11y calciiiirig izrrtirr.ci1 nii.riio.es of calca,uoz~sir11c1 crigi//crceous rilc~rei.in/s.E.~eriiz1;7lesu1.e Roiiza~zcorzcrete riiacle c$ the ~~crtzri~al cer7ielit cr~zclenzirzelltly l~ycli.azrlic ,, , i117ze. Po:_:olcrlz,PoZrolcr~licMcrter.icrl Holines and Wingate (1997) defined pozzolan as the following:
generally c11~1iiii11ia orid re~icti1:esiliccr, vi'hich ~ v i l l ' A 17zcrtei.ialfor llrzitiiig otlzer nzatei.ials oi. articles. It is conzbine with hycli-atecl lirlle crt rzor171aIfeii111er.at~~r~es iii c q ~ ~ e r 11lastic ~ I I y crt the tirize ofa~~l~liccrtio~i but hur~clei~s the pi-esence of n1oistrn.e to foinz stable ii1solzrble 11~11eiz ill place.' Cement by this definition (Walker 1'1%)13el.fie~.' 1988) includes all lilne Illortars and Portlalld cements c0"71'oL""CI" "'irk "'7'""~ (Goins 2000). Pozzolan possesses by itself little or no cemeatitious As defined above, the terms cement and binder can be used interchangeably. However, in the coiltext of traditional building material, cement is defined by Hol~nesand Wingate (1997) as:
value and could be regarded as an aggregate, however, when it cheinically reacts it gains certain cementitious properties (e.g. crushed bricks or brick dust added to lime based mortar).
'Qliick-setting billdel for nlakiiig ~izortcrr.~errid conci-etes. By ,far the 17zost 1~'iclespi-earl cenieizt is t l ~ e 2.1.4. Aggregate Portlmlcl cer~ze~lt foi.111ecl h)]gr.ri~cllnger cllrzker- \r,lllch Hol~nesand Wingate (1997) define aggregate as: /!as bee11 pr-epm.ec1 crt hlgh kiln tenlperatzrr.es $.or11 cl
el~idothei- hycli.alrlic lirizes is tlzcrt cements iizzrst gr.olrnd to cl f i ~ ~po~vclei e before they car1 slcrke' .
In this context, cemeat is considered as quick setting hydraulic binder. In the building i~ldustry the term 'cement' is understood to mean Portland cement or mortar made of Portland cement. The term 'cement' in its meaning as a general binder is not used in the building industry. Poi.rlanel Cei71e1zt(PC), Oi~e/iiiai:\iPoi.tln~~d Cenlerzt (OPC) Holmes and Wingate (1997) define Portland ceinent as: 'Coinillorl foi.171 of ceriient e01~foi.r1zi11~~ to certairz stanclcrr.cls cr11r1nlacle hy gi-illcling c1 cliriker ,foi.i7zecl h!, fii.ii79 a sllri.i.ied rizi.~tl.t~i.e of c l a ~ c11le1lirl~estoizent high teii~pei.at~ri.e i11 a kilrz. Ccrlcizriil szrl1~kateis crlso gi.oirrlcl iiz to iilod(fi tlie setti~zg/.ate.'
'any grcinrrlcr~.rizntei.icr1, such as scrr~cl,gr.avel, ci-~rshed stone, or iron hlcrst-fzrr~zance slag, zised ~jitl7 a cerizentilzg nzecli~mito ,foi.iii a ~izortcrr.It is L I S Z I C I I I the ~ 1m;qest ~~olzrnzef~.ic co~istituerzfof a moi.tcrr:' In general, an aggregate can be regarded as any solid material apart from cement (binder) and reinforcelnent added to a [nix iinmediately before or after mixing. Fibres and other materials added to a mix, which are soinetiines called reinforcement but do not act as the reinforcing agent, should be regarded as an aggregate. un-burnt and/or un-slaked Similar un-reacted pozzola~~, lilne lulllps originally meant as cemeatillg lnaterials act example, when analysing a" aggregate. bi1lder:aggre~ateratio of lilne mortars colltaining lime lumps (un-burnt and/or ~ln-slakedlime) by acid dissolution the effective binder content is less than the actual figure derived (Leslie and Gibbons 2000).
MORTARS IN HISIORIC BUILDINGS: A REVIt\I
CORSERVATION. TECHNICAL AND SCIENTI~IC LITERAIUIlt
MORTARSI N HISTORIC B1111IIINGS A
REbIEW OF S H t
C O N S ~ KION, V ATI I C IIVILAL AND S C I E ~ T ILITERATURE F~C
The reality of masonry conservation practice is that stone or brick is treated and preserved while the lnortar (pointing, bedding) is replaced or partly replaced and therefore lost. Although the value of original nlortar is recognised at present and the rnortar is preserved whenever possible, it is often necessary to repoint or apply another repair method utilising a new rnortar mix in order to prevent a fi~rtherdamage of the masonry units. Any new material and treatment introduced to a historic fabric should, however, be compatible with the fabric. Compatibility is relatively easy to understand in general, but its interpretation to a real conservation task may be rather indeterminate. Co~npatibility can be co~nprehendedfrom several points of view. It should be in agreement with the philosophical and ethical issues in conservation. Depending on the actual design of mortar it can be regarded as traditional or scientific. These aspects are sonletirnes thought of as distinct, but in fact they are highly interrelated and complementary.
usually the selection of a new repair nlortar is based on the 'like for like' philosophy. However, any modern or 'dissi~nilarmaterials should not be ruled out' as long as there are 'no negative consequences' (Teutonico et al. 1997). The Burra Charter deals with this problenl by a general limitation of 'no change to the cultural significance'. 'Minimum impact' or 'as little as possible' are general rules of repair and conservation philosophy that should be maintained for any conservation treatment. There are still mortars currently applied in remedial conservation works which can cause damage or accelerate deterioration to the historic substrate. Therefore the prilnary aim of these definitions is to be able to determine materials which are appropriate ('at least' not to cause any damage) for use in conservation by considering Inany different aspects. This leads to a technical understanding of compatibility as specifications or general requirements for design of a new lnortar based on material characteristics.
3.1. Definition of compatibility Bell (1 997) in the 'Guide to International Conservation Charters' published by Historic Scotland (TAN 8) explains the term 'compatible use' based on the definition of the B u m Charter as: 'a use which involves no change to the culturally significant fabric, changes which are substantially reversible, or changes which require a minilnal impact'. In a silnple description of compatibility, Teutonico et rrl. (1997) state that the 'introduced treatments or materials will not have negative consequences'. Van Hees (2000) suggested a definition of compatibility related directly to mortars as follows: 'The new lnortar should be as durable as possible, without (directly or indirectly) causing damage to the original material'. The ~nutualsubject of these three definitions is that any material can be used as far as there is no further damage to the original material. Technically it means a consideration of mechanical, physical and chemical properties of new and original materials and their interaction. On the other hand, strictly speaking, a new lnortar which would not cause any danlage to the original masonry Inay still not be compatible. Colow, texture and aesthetic values should be considered and
3.2. Compatibility with regard to conservation philosophical and ethical issues Basic conservation guidelines are formalised by intenlational conservation charters and standards. The problem of compatibility was perhaps officially introduced by the Athens Charter (1931) which approved the use of modern materials for restoration of monuments. Later on, the Venice Charter (1964) appended that modern techniques for conservation can be used if supported by experience and scientific data, and where traditional techniques were proved inadequate. The Venice Charter stressed that restoration should respect thc original material. It also stated that any replacelnent should be distinguishable from the original so that restoration does not falsify the artistic or historic evidence. This requirement may be in contradiction with the most widespread current approach of designing a compatible mortar as a copy of the original one. Another important point was made in the Declaration of San Antonio (1996) about the authenticity of ~naterials.It expressed an idea that only the historic fabric is authentic and the restored fabric is not. However, it acknowledged that some materials (it was not specified, but lime nlortar could be considered one of them) do weather and require a periodic replacement or maintenance. In such cases, the traditional techniques should be followed.
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSERVATION, TECHNICAL AND SCIENTLFIC LITERATURE
Philosophical and ethical issues in conservation are very complex and develop with society. They apply as guidelines in general but they should also be able to provide a specific answer about policy and conservation treatment for every individual structure. Every historic structure is unique and so are the values to be preserved (Buman 1997). The values to be preserved primarily define and limit functions and properties required from the conservation treatment. In the case of this review they limit and define functions and properties of repair mortar. The cultural significance of the structure enshrines all its possible values (emotional, cultural, architectural etc.) and its formulation leads to a determination of correct conservation policy (Buman 1997). For example, a conservation treatment of a fresco painting lies in the preservation of the artistic value of the work rather than the authenticity of the mortar. However, such a conservation approach is not an inflexible rule - it should be established individually through the cultural significance of the work. This example may be seen as an obvious extreme, but it also illustrates the point that
the authenticity of historic mortar is often 'sacrificed' to preserve some other values. The most common situation of where historic pointing or bedding mortar is "sacrificed" is in connection with structural stability and the integrity of masonry; and hence the preservation of the whole structure. Another example is the weathering of pointing mortar, which is supposed to protect the masonry as a form of seal. Therefore, its replacement when even partially damaged is a logical step of any building maintenance. However, when a new mortar is used to repair original it must not the mortar and it should attract all the adverse agents before they affect the original material. However, the colour of a new mortar could be a matter of whether it should or should not be visually distinguishable from the original mortar, especially when a 'like for like' approach is applied. Also, when a different, modern material is used for repair, should it try to match the original colour and texture? The Athens Charter suggests concealing consolidation whenever it is possible 'in
Figure 3.1: Tantallon Castle and detail of its deteriorated masoniy. There are many historic buildings with repointed masonry, which have undergone some preservation treatment that resulted in a loss of original pointing and bedding mortal: For example Tantallon Castle with its 4m thick, red sandstone ashlar curtain walls which were repointed and consolidated before the Second World War The appropriateness of this kznd of inteivention may be questioned. However, the work was done with the best knowledge and skills of that time. On the other hand, how much of the original mortar was there when it was treated? Pointing mortar is often the first to deteriorate so repointing has been a common pl-actzce in building maintenance in the past. The compatibility of such treatments and application of ti-aditzonal techniques should be considered.
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSERVATION, TECHNICAL AND SCIENTIFIC LITERATURE
order that the aspect and character of the restored monument may be preserved'. Although this part of the Athens Charter may now be seen as a bit obsolete, as consolidation work is clearly visible on most historic structures, the character of the repointed masonry is certainly a part of its value and should be preserved.
Historic Stone Structures', Sass and Snethlage (1997) pointed out that today strict reversibility must be replaced by compatibility and 'retreatability' measures. If that should become standard practice then there is a need for compatibility to be better understood and defined. Compatibility should describe the properties which newly added material or original material after conservation treatment should have in relation to the original material. Research into compatibility of mortars is still in its infancy and no guide or standardised techniques for determination of the correct material for repair are available. The current approach towards the design of a compatible mortar can be found in practical conservation literature. It offers general requirements for the formulation of restoration mortars based on generally accepted conservation principles, basic physical properties and compositional requirements for new mortars (e.g. Maxwell 1998 and Ashurst and Ashurst 1990, Ontario Ministry of Citizenship 1988, Feilden 1998, Croci 1998). The principles are derived from the general consideration of the properties of masonry materials. However, it is rare to find specific technical rationales behind conservation practitioner driven requirements, and justification with reference to published research is also rare. This may be because such research is itself rare (Vglek 2000).
Figure >.L:Aanastone masonry nas aeen repozntea wztn cement gauged mortar where a technique called 'Stirling grit wash' was applied to make the repointing look more weathered by exposing the aggregate. Although the pointing is done to resemble historic, weathered surface masonly, repointing in this or some other modern technique can be easily distinguished by any careful observer. However, when a traditional technique and materials are used, the distinction after some time and when it weathers, is much more difficult to make, without more detailed analytical techniques. Tantallon Castle, pound coin for scale.
The views on each individual conservation task vary according to national conservation policies. In Scotland, Historic Scotland published 'The Historic Scotland Guide to International Conservation Charters' (TAN 8, Bell 1997). It explains and discusses the basic conservation terms in a context of international conservation charters. For practical conservation tasks, reference should be made to 'The Repair of Historic Buildings in Scotland' by Knight (1995) where the principles of repair adapted by Historic Scotland and reflecting Scottish practice can be found. Compatibility is now becoming an increasingly important issue. During the Dahlem workshop 'Saving our Architectural Heritage: The Conservation of
Groot et al. (2000) divided the approach to specify new mortars into 'traditional' and 'modern'. The 'traditional' approach is based on the use of traditional material which is subsequently altered or treated in order to achieve all compatibility requirements. On the other side, there is the 'modem' approach based on compatible requirements to develop a formulation of a new mortar, and if necessary it would use modern materials. Groot et al. (2000) concluded that mutual understanding of both approaches would lead to better development of mortar for conservation.
3.3. Compatibility with regard to traditional approach and conservation practice Practical experience gained from conservation projects is a valuable source of knowledge about performance and behaviour of mortars. 'Hands on' experience is highly valued in conservation and practical experience is considered to be particularly useful for the design of a compatible mortar. A review of contemporary practice of using lime mortars in conservation was presented at Historic Scotland's International Lime Conference (Ward & Maxwell 1995). Lime-based mortars in particular are good examples of a traditional material used in conservation, where good skills and practical experience have a significant influence on
performance. Bur~nan(1995) described the advantages of using lime in various co~lservatio~l techniques and the successful revival of lime into wider conservation practice. For traditional lime-based mortars, often the conservation technique, good site practice, woskmanship and skills are considered to be the key instruments for their successful application (Gibbons 1995, Johnston 1995). Many failures of lime-based mortars are caused by their inappropriate use or by a lack of practice and training in their correct application (Gibbons 1995, Holmstrii~nPart l , 1995). The most basic specifications for new mortars are from practical building and masonry conservation guides (e.g. McAfee 1997). The usual advice is to carry out basic analysis to obtain the composition of the mortar (usually by dissolving the mortar in an acid) in the first instance and, if the original mortar has performed well, then the new lnortar mix should resemble it as closely as possible. However, it is advised that the new rnortar should be softer than the stone. Ashurst (1990) in the 'English Heritage Technical Handbook' specifies that the original aggregate should be copied, however, the mix may need to be ~nodified to improve the weathering characteristics. Milner (1972) points out that natural materials should be used to match the colour and texture. He also suggested that soft mortars should not be used for repairs on buildings originally constructed with hard mortar. The basic specifications for mortar required by conservation practice can be summarised as follows: The formula of the new mortar should match that of the original one; natural materials should be used when matching colours and textures. The new mortar should be softer than the original mortar or masonry but, on the other hand, the mortar should not be too soft if the original masonry was constructed with hard mortar. Under no circumstances should the new lnortar cause deterioration to the existing host material (mortar, masonry). Side-effects and long-term effects caused by repair should also be considered. For example, new plastering or repointing may change the indoor moisture conditions. Larsen (2000) described the importance of stable moisture conditions inside a chapel with salt-contaminated painted plasters in Denmark. These basic requirements are applicable in general and can be extended depending on the particular function and application of the mortar. For instance, Holmstrom (1992) presented a list of co~npatibilitycriteria for lime mortar renders used by contractors in Sweden.
Materials and colnponents used ~ n u s be t removable, and must not change the physical or chemical balance of the building and nlust not change the aesthetics. Each layer of render (mortar) should be weaker than the substrate. Materials with the same properties as the original should be used. If the original nlaterials are not used, this must be justified and all relevant properties of the original and the substitute must be declared. These suggestions enshrine minimum intervention and the preservation of existing historic fabric. In addition, Holmstrom's (1992) criteria emphasise the need for reversibility of the ~naterialapplied. The final point arrives at the heart of the co~npatibilityissue and the desire of conservationists to replace like with like. It nlakes demands for analysis of historic mortars in order to formulate compatible replacements that resemble the original. Basic perfornlance testing and in-situ trials are common and recommended. However, there is less demand for testing and characterising the new mortar properties, as it is a copy of the original one and therefore it is assumed to perfor~nin the same way. Such assumption Inay not always be correct. Vilek (2000) in his PhD thesis discussed a theoretical co~npatibilitymodel for two mortars, one designed on a 'like to like' basis and one on a 'compatible properties' basis. The performance of both mortars relied strongly on the curing and ageing conditions. However, the curing conditions of the new mortar may not match the ones of the past.
3.4. Co~npatibilitywith regard to physical, chemical and ~nechanicalproperties Alongside the traditional approach to the specification of a new nort tar there is a growing need for the scientific description of its compatibility, as was concluded by the ICCROM conference in 1981. It appears that the selection criteria for new mortars s h o ~ ~ be l d based strictly on material characteristics of the mortars, providing that the mortar complies with the conservation requirements and principles. The need for exact description and characterisation of the rnortar led to a more technical description of compatibility. It was reflected in some specifications for new mortars, as they became more detailed and technical. For example, Historic Scotland's Technical Advice Note 1, Preparation and Use of Lime Mortar (Gibbons 1993) defines that the new mortar should have porosity and strength close to the original one. It should be less dense and more permeable than the host masomy and at the same time it should be sufficiently durable.
MORTARS IN HISTORICBUILDINGS: A REVIEW
OF T H E
CONSERVATION, TEC IINIC,\L
W h e n a new compatible mortar is to be designed the required properties I T I L I S ~ first be determined and consequently confirmed by testing. The technical design o f new mortar can be divided into two main activities. Analysis o f the original nort tar Analysis sl~ouldprovide all the information about the historic mortar (and masonry) that is needed for the design o f a new compatible mortar. In current practice analysis most colnrno~lly consists o f only the composition o f the historic mortar. However, recent research suggested that analysis is more con~plicated than it was thought to be. Hughes et (11. (1998) pointed out that the colnplexity o f historic materials that reflects their production, preparation and weathering over the lollg term Inay mitigate against the recognition o f the properties o f the original mortars at the time o f their application. Therefore, only the 'contemporary' properties and composition o f the historic mortars are known and simply copying these historic mortars without the knowledge o f their change Inay not lead to the same material performance quality. It is important to note that analysis can help to identify other important influential factors, for example mixing (Leslie 2000). There should be complex analysis o f the whole masonry, building, etc. in order to provide all relevant information. Specifications for new mortar, its properties and testing The specification o f a mortar from the point o f view o f technical compatibility is based on comparison o f properties. Preliminary research into this field was carried out by Pero~liet 01. (1981) and presented during the ICCROM symposium in Rome in 1981. From the beginning, the authors pointed out that it was not possible to set down a list o f detailed requirements for ideal conservation mortar, but instead general principles were used. The authors proposed a number o f tests (flexural strength, compressive strength, modulus under compression, alkaline elements concentration, total porosity and pore size distribution) which were carsied out to test specimens made o f various mortar mixes including lime putty mortar, hydraulic lime mortar and mortars gauged by cement, brick dust and pozzolanas. Although the paper neither came to any conclusion about what properties were important nor determined the tests for selection o f a new mortar, it set up a baseline for further research. Sasse and Snethlage (1997) studied methods for the evaluation o f stone conservation treatments. They identified properties to evaluate compatibility o f repair
S C ~ E N T I FLITERATURE IC
mortars and stone masonry. They also introduced preli~ninary tolerance limits established for various materials and property tests. Stone Repair Materials Property Syi11bol
Requirement (after 1 year)
E-IIIO~UIUS 20.100% (60)
Thermal dilatation coefficient
Water uptake coefficient M/
Value of water \ l a ~ )resistance ~~~r
0.5-0.8% PPOS stone
Tnhle 3.1: Irn~estigcitiorrnretlrocl 011~1~.equir.e~rier~ts (0s cr percerrtcigc. ($the ~ ~ i l l or fe tlre szrhstr.cite) to e~~cil~rcite storle r.e,~~cii~. rrrater~icrls.Tlie r.eqlrb.en7c~nt.srire 1.elatec1to tlre prol~er.tieso f tlre s~rl~str.cire ( F I z ) Scisse I ~ ~ rrr~clSlrethlrrge 1997).
3.5. Compatibility with regard to mortar and lnasonry interaction Interaction between mortar and masonry is an effect between them which results in some physical or chemical change to one or both o f them. It is as an evaluation o f compatibility performance. Bad interaction means that incompatible materials or repair techniques were applied. It results in deterioration and accelerated weathering o f masonry material. However, the use o f an incompatible mortar or treatment does not mean bad interaction a pi-iori, it merely brings about conditions favourable for deterioration. The deterioration itself happens through environmental agents. For example, a dense cement mortar containing salts used for repointing o f porous sandstone masonry may not cause any bad interaction without the presence o f moisture in very dry ageing conditions. Water or moisture is needed for a chemical and most physical deterioration processes to take place (Collepardi 1990). Sumlnarised by Amoroso & Fassina (1983), water is the main cause o f degradation mechanisms for masonry materials. When testing a new compatible mortar the interaction with masonry should be considered in a wider context comprising all the potentially influential factors. It should be kept in mind that properties o f mortars when determined on small specimens in the laboratory are different from the real masonry conditions in-situ (Depraetere et 01. 2000). Therefore, full-scale 'in-situ' trials are important for real evaluation o f the interaction. Full scale testing should be prefen-ed in any larger conservation tasks (Stewart et 01. 2001).
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSERVATION, TECHNICAL AND SCIENTIFIC LmRATURE
Bottom: Trial panel of repointing at Inverlochy
On the other hand, it should be emphasised that degradation connected to interaction of mortars and masonry is not the sole problem of new, modern replacement mortars. Maxwell (1994) described cases of deterioration related to the interaction of original lime mortars with sandstone andlor granite. Soiling and decay in the vicinity of joints observed on masonry of many structures suggest the interaction of the lime mortar and stone. Maxwell (1994) described cases of ashlar masonry being changed to square rubble-like masonry due to decay round the joints. The deterioration was caused by the conditions in which the masonry had been ageing.
A number of cases of masonry deterioration could be put down to salt formation and crystallisation. Rainwater can transport soluble salts from mortar to adjacent stone (Perry & Duffy 1997). The interface zone between two different materials is the place where potential salt crystallisation can occur (Baronio and Binda 1987). The exact position of the salt crystallisation depends on capillary migration between mortar and stone, and rate of evaporation (Charola & Lazzarini 1986). If the mortar is more porous than the stone, evaporation and salt crystallisation take place mainly within the mortar and vice versa (Charola & Lazzarini 1986).
Research into properties related to interaction of materials is driven mainly by the deterioration of the materials (see softer mortars).
Rainwater, 'acid rains' can facilitate the formation of gypsum and other salts (Charola & Lazzarini 1986). The susceptibility of mortars to react with air-borne
MORTARS IN HISTORIC BUILDINGS: A REVIFW
CONYFRVATION, TECHNICAL A N D SCIENTIFIC LITERATURE
sulphur dioxide was measured in a weathering chalnber by Zappia et ol. (1994). The authors co~lcludedthat the reactivity is related to porosity, specific surface and alkalinity of mortars. Perhaps surprisingly, the reactivity did not correlate to the quantity of calcium carbonate. The results suggested that the most reactive was a cement based lnortar (lowest quantity of the Calcium Carbonate) followed by lime-based mortar, and the least reactive was a limepozzolana inix (Zappia et al. 1994).
the argument for in-situ trials when assessing the con~patibilityand interaction of different materials.
Another mechanism of masonry degradation is caused by different expansions of masonry materials. A case study on defects of renders of a cathedral in Toledo, Spain (Macias 1992), showed that the differences between thermal and "hygric" (sic.), or I?ygr.oscopic, expansion of gypsum, lilne mortars and dolomite stone caused cracks, fissures and spalling off of the render. (Hygroscopic refers to the tendency for a substance to In general it concentrates on the usc of materials and take up moisture.) Lilnc mortar was found to have low their compatibility. However, a detailed understanding relative thermal and hygroscopic expansion (Macias of degradation requires study of its ~necl~anisms. 1992). Verlneltfoort et 01. (2000), who studied thermal Particular degradation lnecha~lislns are summarised expansio~lof mortar repointing and its compatibility below, but for masonry the waterlmoisture transport is with original masonry, described that the interaction the most crucial to understand. The way water between brick, bedding mortar and two types of transports through an interface between Inasonry units repointing mortar causes irregularities in the stress and and mortar significantly affects the lnoisture behaviour strain distributioll which consequently has an effect on of the whole historic masonry. For example, the durability of the mortar and masonry. They Depraetere et al. (2000) examined the influence of the concluded that strollg pointing mortar expands Inore mortarlbrick interface on moisture transport. The than soft bedding mortar. This represents one of the authors described a zone formed at the interface with few efforts to quantify compatibility and demonstrates different porous structure and related lnoisture conclusively that stronger, harder cement mortars are properties. They also pointed out that mortar cured in a less appropriate, in one physical aspect, for the repair joint between bricks has other moisture properties than of historic lnasotlry than softer mortars. the inortar cured in moulds. This indeed strengthens
A way of studying building materials from a conservation science point of view is to study their damage lnechanisrns and their deterioration (e.g. Torraca in Porous Building Materials, 1988). Possibly the best model for scientific studies of deterioration of masonry materials is based on a review of literature on deterioration of porous materials published by ICCROM in 1976 (Stambolov and van Asperen de Bore 1976). Torraca (1988) later on in 'Porous Building Materials' described material deterioration under the following categories: External mechanical deterioration. This is caused by excess of stress with respect to the strength of the material (load, thermal expansion, stress caused by transport or working techniques, dynanlic load and vibration). When excessive stress occurs, the material cracks and even small hair-cracks can lead, in combination with other deterioration factors, to accelerated deterioration. Internal mechanical deterioration. This is sonletinles called physical deterioration and is mostly due to a physical variation of water inside masonry like evaporation, capillary flow. A large stress can arise inside the pore structure when water freezes and crystals of ice or minerals are formed within the originally water filled pores damage caused by salt crystallisation and efflorescence or similar effects. Chemical deterioration. This is mostly connected with a reaction between sulphate and the other compounds in the masonry (Collepardi 1990) Chemical coivosioll almost always requires the presence of water (Torraca 1988). Water can play two roles in chemical corrosion: (a) water in the form of liquid and vapour is chemically active (b) water in the form of liquid acts as a transport medium for other components Water which has been in contact with other solid material of the same kind is not chemically active (rising damp) but it can still act as a transport medium for other deterioration agents, e.g. see physical deterioration. The danger of chemical corrosion increases with atmospheric pollution and acid rains (Charola 1986). Biodeterioration. This can be caused by bacteria, algae and/or fungi which produce acid. Lichens can also penetrate into several millimetres of the surfacc of the material. Moss commonly grows on the surface of alkaline inaterials (lime mortar, Torraca 1988). Roots of higher vegetation can penetrate deeply into joints and cause deterioration of the masonry.
MORTARS IN HTSTORIC RUII-DINGS:A
REVIEW OF 7HE
CONSERVATION, TECHNICAL AND SCI~NI'IFIC LITERATURE
ANALYSIS OF HISTORIC MORTARS
The analysis of historic mortars is carried out broadly for two reasons (Hughes & Callebaut 2000): For specific collservation and repair related investigations, looking to select replacement materials and/or deternline the cause of evident problems in the deterioration of a historic building to allow the formulation of conservation and repair strategies. Academic studies looking to clarify the architectural, chemical and physical performance of historic mortars for the development of replacement materials or the archaeological study of building technology and its associated social implications. The objective of testing for characterisation may primarily involve the determination of the essential properties of an old mortar, with a view to the formulation of the composition of an appropriate repair mortar. It may also be aimed at the exploration of the potential and limitations of a testing technique used for characterisation (Groot et al. 2000). For example this can involve (Groot op. cit. 2000): The identification of the limitations of testing methods, including wet chemical analysis (Blauer Bohm 2000; Martinet et al. 2000) and differential thermal analysis (papers by Moropoulou et al., Ellis 2000). The problems of the identification of types of additives and natural hydraulic lime components in old mortars (Sickels 1987, Krist et al. 1999, Van Balen et al. 2000; Charola 2000; Callebaut et al. 2000) and their differentiation. The identification of the provenance of natural hydraulic lime (Callebaut et crl. 2000). Diagnosis of the cause(s) of damage focused on a better understanding of damage mechanis~ns (van Hees 2000; Blanco-Varela et (71; Larsen 1999). The following sections deal first with sampling of mortars, and then with the variety of techniques currently used for the characterisation of the properties of historic mortars, both compositional and mechanical.
4.1. Sampling, damage diagnosis, hypothesis formation and on-site visual analysis The first stage in the analysis of mortar materials is a careful pre-analysis of the conservation objectives of a study or conservation effort. This is particularly important as historic buildings are special cases. Broadly applied renovation or wholesale replacement is not appropriate, and as the historic fabric is the valued historic and social material it must be protected as much as is practicable (Hoffinan 1998). This places considerable constraints on the analyst and the sampling operative (Hughes & Callebaut 2000, op. cit.). Two major controls operate on sampling practice: the objectives of an investigation and the analyses (physical, chemical or descriptive) needed to fulfil the objectives (Hughes & Callebaut 2000). The objectives of a study must be clearly stated before any sampling can take place. Minimum action is required in order to reduce effort and cost and minimise destructive intervention and damage. The materials, the construction method and stratigraphy of the building must be understood thoroughly before sampling begins, in order to ensure the collect materials are sampled and so that sufficient material can be obtained. Spatial and temporal distribution of materials must be understood to do adequate sampling (Binda and Baronio 1989, 1991, Pursche 2000, Hughes & Callebaut 2000, Blauer Bohm 2000, Leslie and Gibbons 2000, Cardoso 2000, Sass 2000). The formulation of hypotheses regarding damage mechanisms (van Hees 2000, op. cit.), the decay state of the building (Long et al. 1998) and the subject of study directs the choice of analytical method which in turn has a requirement for a minimum quantity of sample, but also a certain quality of sample, whether as a coherent lump preserving textural-component relationships or as a powdered sample. The choice of analytical method determines the sampling requirements (Hughes & Callebaut; Goins; Andersen; all 2000). Visual and other non-destructive evaluations assist in the assessment of ideas about the variations in the macroscopic characteristics of mortar materials, allowing choices to be made on the representative
nature of sample sets (Cardoso 2000, Vilek et 01. 2000, Long et 01. 1998). It is accepted that for historic structures the opportunities for statistically adequate sampling are limited due to the culturally precious nature of the materials. Samples should be representative, but if this is not possible the degree of bias must be understood (Hughes & Callebaut; Goins, Sass; all 2000). Sampling should be done by experienced people, who know what is requil-ed to achieve a specific test objective, and they should preferably have experience with the experimental technique and its sampling demands. British Standard BS 4551: Part 2: 1998 "Methods of testing mortars, screeds and plasters" sets guidelines for the sampling of hardened mortars. This standard is aimed primarily at the characterisation of mortar in more modern buildings, but the approach is applicable to older historic buildings. The main reasons considered for sampling are the variability in different par-is of the work, the con~positionat specific, often problematic points, and the average composition over an area of masonry. Where an averaged sample is needed to represent a large area or the sample needs to reflect variation, a large sample set is required. Minimum sample sizes are specified as being representative per 10m2 for brick/block work, plastering and floor screeds, and the method of obtaining a combined bulk sample is given. When sa~nplingmasonry mortar the whole thickness though the wall should be sampled, requiring the removal of masonry units, something not always feasible with a historic building. Where it is not possible to remove bricks or blocks to take a mortar sample, drilling can be used to generate a powder which can be used for a chemical composition, though this can cause segregation of materials and result in a nonrepresentative sample. Ashurst 1998 states that the samples taken "should be the minimuln necessary to gain the required information without doing damage to the historic structure". Technically of course taking any sample is doing damage, but this needs to be considered against the benefits gained by sampling and gaining additional information through analysis. Ashurst goes on to specify that sampling must be perfor~nedby someone familiar with the building, and that the analyst should also be involved. The sample itself should be of at least 50g and in a coherent lump. The location of the sample must be precisely recorded and sufficient sample must be taken in order to ensure some form of representative analysis. Ashurst also gives an example of a datarecording sheet to be completed whilst sampling. A similar form is also given by Hughes and Callebaut (2000). Ashurst (1998) and Hughes and Callebaut (2000), emphasise the usefulness of first performing an on-site
visual analysis of mortars, before physical sampling. A good idea of the general components of the moriar can be derived by an experienced person using a low level of optical magnification. Binder, aggregate and other inclusions, including particular nlortar additives, can be recorded in this way. Ashurst goes 011 to suggest gentle scraping to remove weathered surfaces to improve identification of components. This analysis will also clarify the method of construction and the profile of the joint, as well as highlighting any repointing or other later repairs. Groot et ril. (2000) suggest that features such as the number and thickness of coats or applications of bedding mortar or renders, the presence of cavities, fractures, cracks and macro porosity within the binder, the presence of hair and other additives and the abundance and distribution of unmixed binder (lime lumps) can be observed. Also the lithological characteristics of aggregate and pozzolanic additives. The general type of binder (hydraulic, cement, lime etc.) and the nature and size of the aggregate will be identified.
4.2. Methods used for technical characterisation A number of techniques used for the cl~aracterisationof old mortars are presented below with the basic properties which can be determined by the methods, and their limitations. For each a selection of papers is reviewed. It must be borne in mind however that the separation of these techniques does not suggest that they are applied in isolation, Many of the papers reviewed use several methods of analysis to characterise mortars, as often the identification of a component or property is not unequivocal using one method alone. 4.2.1. Acid dissolutiora and wet clzernical arzalysis The simplest form of mortar analysis involves the separation of the aggregate from the binder to determine their relative proportions to allow a replacement mortar to be fo].mulated. This form of analysis also allows the qualitative determination of the type of binder and the characteristics of the aggregate or other additives. The carbonate binder can be dissolved from the aggregate by the use of a dilute acid, most comn~onlyHydrochloric Acid (HC1). The main limitation of this technique is that if carbonate aggregate is present in a mortar then it will be dissolved along with the binder (Ashurst 1998, Leslie and Gibbons 2000). 111 Scotland almost all aggregate is composed of silicates which do not dissolve readily in acid, thus permitting its use for the majority of mortar characterisations. Ashurst (1998) gives a simple procedure that can be followed. It is often possible to get a good, though not exact, idea of the degree of hydraulicity of a mortar, the presence of cement and the use of admixtures and pozzolanas using acid
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF
dissolution combined with careful visual analysis before and after. The use of dissolution analysis also leads on to the further application of standard chemical analysis techniques. As the binder is put into solution this makes it amenable to instrumental chemical analysis. The soluble silica content can be determined, which is related to the hydraulicity of the mortar (van Balen et al. 2000). Soluble silica and other element concentrations can be analysed by various methods including, AAS, ICP, ion chromatography. However, the presence of pozzolanas in mortars Inay disrupt the determination of the original composition by wet chemical analysis, by changing the distribution of soluble silica due to soluble reaction rim characteristics around pozzolana grains (van Balen 2000, Charola 2000). Pozzolanas will also be reduced in size through acid digestion because of reacted sin1 compositions, resulting in inaccurate grain size distribution determinations (Blauer B o h ~ n2000). However, acid dissolution has not been standardised and there is some debate over the exact method that should be followed. This is particularly important for full elemental chemical analysis where the method of sample dissolution has been shown to alter the concentrations of elements in samples. Van Balen et al. (2000) demonstrate that the measured soluble silica varies with the temperature and the strength of the acid used in dissolution, due to contributions from aggregate and other additives. Stronger acid and higher temperatures of attack resulted in higher measured SiO, contents and relative errors up to 100%. The mineralogy of the aggregate was also proven to have an effect, micas and feldspars being more susceptible to solution by acids than pure quartz. Alvarez er al. (1999) recently looked at the effects of hot HC1 attack on historic mortar analysis. The same acid concentration was used to analyse the same samples, but in one test at room temperature with ~nechanicalstirring, and in the other hot acid was used also with mechanical stirring. Some significant differences in result were obtained. The hot acid method was found to dissolve a greater portion of the binder, as revealed by CaO contents of the soluble fraction and the total percentage of the insoluble residue. For the hot acid attack the insoluble residue contained no remnant CaO. Significant reductions in total Fe, A1 and Ti oxides were also seen in the insoluble residue from the hot acid method. The conclusion is that for quantitative analysis using acid dissolution, the neth hod must be chosen carefully and clearly stated. More significantly, however, the recorded amounts of insoluble residue, most often used as a measure for mortar forlnulation on a qualitative basis, also showed significant differences dependant on the method applied.
CONSERV~YI'ION, TECHNICAL AND SCIENTIFIC LITERXI'URE
4.2.2. Optical microscopyl Petrogrriphic analysis The use of optical lnicroscopy is a powerfi~ltechnique for the investigation of the components of historic mortars. After sampling, lnortar is cut, niounted onto a glass slide and ground to a thickness of 30 microns (30/1000 of a millimetre), for~ninga "thin-section" that permits the translnission of light through the components of the mortar. This is best performed on coherent samples of mortar that preserve the full texture of the original tnaterial, though powders are still amenable to compositional investigation using this method if mounted in a resin before cutting and grinding. Samples are commonly inlpregnated with a coloured epoxy resin to ensure integrity during cutting. The thin-section can be examined using a petrographic, polarising, microscope. A specialist investigator fanliliar with mineral recognition can then docurnent the co~npositionof the aggregate, binder (including anhydrous clinker), additives (organic and inorganic including pozzolans) and secondary mineral fornlation including salts. The two-dimensional cross-sectional texture of a lnortar can also be described, for example the size and shape of the aggregate and porosity. This form of analysis is called "petrographic" analysis. The study of hydraulic cements using petrographic techniques, both of fresh clinker and hydrated cement pastes in modern mortars and concretes is well established. Campbell (1986) provides a comprehensive guide to the recognition of hydraulic clinker phases in reflected and transmitted light. St. John et al. (1998) also cover the subject of concrete petrography very thoroughly, in what is often considered the standard work on this subject. Petrographic studies of concrete often focus upon aspects of durability (e.g. Idorn 1967). These include sulphate resistance ( e.g. Hooton 2001, Hagelia et al. 2001, Sibbick and Grammond, 2001, Oberholster et al. 1984) and issues such as determining the watercement ratio (Elsen, 1995, St. John et al. 1998). The petsographic examination of historic mortars and concretes has lagged behind that for concrete, but has risen in importance over the past few decades. Idosn and Thaulow examined a very early Portland Cement concrete from England dated 1847, made from Portland Cement produced by William Aspdin. They were able to identify though microscopy the nature of the aggregates, but also that the cement produced was coarsely ground, with a low water:cement ratio, deliberately air entrained and well compacted, resulting in a highly durable material. The concrete was only carbonated to a depth of 5mm. Unhydrated and hydrated fragments of clinker were also observed preserved in the cement phase.
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSERVATION, TECHNICAL AND SCIENTIFIC LITERATURE
,Arran) and new (apprux 1895, right,fiom F1 4.1: Two photomicrographs of old (16th C lefi,from Loch Inveriochy Castle, Highlands) mortars. Both images were taken iri r L U ~ Kr ~ ~ u r i s eLight d and show how the distribution of bznder (B),aggregate (A),porosity (P, in blue) and other components within a mortar can be imaged using a polarising petrographic microscope. The OM mortar shows distinctive large rounded pores and the edge of a lime inclusion to the bottom of image. The new mortar shows a more homogeneous binder plzase, thin, arcuate shrinkage cracking and in this case two fragments of carbonate shell material (echinoid fragment, left, and mollusc shell fragment, right). The field of view in both images is about 4mm. This form of analysis allows for determination of binder to aggregate ratio using point counting or image analysis. (1984, and reports referenced therein 1983) analysed ancient Roman and Greek mortars, using optical petrography as part of a wider analytical scheme. They were able to identify the aggregates and other, mostly pozzolanic additives and the degree of carbonation of the material. Rassineux et al. (1989) also studied Ancient Roman mortars from this perspective, combining optical petrography with Scanning Electron Microscopy (SEM) and X-Ray Diffraction (XRD). Optical studies confirmed the degree of carbonation and the location of secondary degradation products such as ettringite.
Figure 4.2: Photomicrograph of internal plasterffom early 18th Century. Section through hair in plaster is clearly visible, running lower centre from left to right across image. High binder content is apparent. Field of view Imm.
Rayment and Pettifer (1987) studied lime mortar taken from the core of Hadrian's Wall using a variety of instrumental techniques. Using optical petrography they were able to describe the aggregates, the rock types of the masonry blocks, and the presence of hydraulic C-S-H phases. In a paper on the petrography of some ancient Indian plasters, Karanth et al. (1986), describe the types of aggregates present, commenting that they were apparently screened for size before use, and the presence of pieces of unburnt carbonate interpreted as the raw materials used for preparation of the lime. The study of ancient mortars has been stimulated in part by the search for stable, highly durable materials in which to store nuclear wastes. Langton and Roy
Middendorf (1991) presents thin-section analysis of historic mortars in the context of a comprehensive analysis scheme involving chemical analysis and XRD. He compares the petrographic appearance of modern lime, gypsum mortars and Portland Cements with historic equivalents. Aggregates including shells, wood, charcoal, anhydrite, brick and gypsum are identified by petrographic analysis. Baronio and Binda (1987) also use optical methods to study the interface between binder and aggregate and "cocciopesto" (brick dust pozzolan) additives. The brick dust and flint aggregate were observed to have reacted with the lime to form a reaction layer surrounding the grain. Cementbased mortars were observed visually to have a poor bond between brick dust and the binder, with large voids present. Lime mortars displayed a much better bond between the brick dust and the lime binder. Optical petrography has also been used to identify hydraulic components in 19th Century historic mortars from Leuven, Belgium, by Callebaut et al. (2000), backed up by XRD and Scanning Electron Microscopy.
MORTAIIS IN HISTORIC BUILDINGS: h. REVIEW 01- I l l E COHSERVATION, TECHNICAL A h D S L I ~ N ~LITERATURE IFIC
The presence of gel~lenite(C2AS), alite (C3S) and belite (C,S) indicate that the material analysed was a natural hydraulic lime, and not a cement. The hydraulic components were also do~ninated by C$, further supporting the hydraulic liine arguinent. Gehlenite also forms at temperatures below 1200째C, much too low for sintering and vitrification needed for celnellt production. The occulsence of C$, which o~ilyforms at over 1 25OUC,is i~lterpretedas being due to localised "hot spots" in the kiln.
inclusions are also identified in these mortars, and a clear origi~lin burnt li~nestoneis suggested due to the presence of relict 'psuedomorl~h'carbonate textures in the inclusions.
Leslie and Hughes (200 1 ) describe the occurrence and characteristics of clinker grains in early 19th Century niortars froin Charlestow~~, Fife. These grains have a mineralogy consistent with lilne production, wit11 concentratio~lof silica froin hydraulic lime production into these grains, but also higher kiln tenlperatures tha11 Hughes alld Cuthbert (2000) discuss tlie petrographic would normally be expected. They also indicate that analysis of 12th and 13th Century inortars from the the material from Charlestown was not ground prior to West of Scotland, drawing conclusions for tlie practical use, but that tlie clinker inay have contributed some formulation of replace~nentmortars. The binder of hydraulic set to the mortars, though acting pri~narilyas these mortars is observed to be locally inhomo,oe~leous, an aggregate. with variations in density over a small scale. Extensive The application of optical petrographical techniques porosity has developed in some parts of the nort tars are a powerful means of deriving infor~nationabout the through the dissolution of carbonate binder material. coinposition and history of historic Inortars. Their This porosity is delineated by secondary readoption in more routine analysis is advised, but not crystallisation of carbonate around the pores, frequently adopted. In addition the application of indicating long saturatio~lof pores with carbonate petrographic analysis requires specialist skills and saturated waters. These features indicate clear changes should only be atte~npted by properly trained in texture of the mortars though time implying that personnel, who are most often geologically educated analysis of the current coinposition of tlie mortar, (Middendorf et (11. i l l p ~ ~ s s ) . especially of the binder:aggregate ratio would furnish a result different froin the original coinpositio~~ of the mortar. This cautions against the use of simple analysis 4.2.3. X-ray Dijfructiolz (XRD) techniques that do not consider the detailed texture of 111addition to chemical and ~nicroscopicala~lalyses,Xthe mortar. ray diffraction (XRD) analysis is suitable for the Hughes and Cuthbert (2000) also describe the presence identification and differentiation of binders and of fragments of what are interpreted to be u~iburnt aggregate within a mortar, if they are crystalline. For pieces of limestone in the mortars they analysed, which example, the differentiation of cement and natural now act as a component of the aggregate. This allows l~ydraulic lime is only possible by n~ineralogical the original raw material source for the lime-binder analyses (Godicke-Dettmering and Striibel, 1996; production to be identified and analysed. Lime Callebaut et al. 2001). In X-ray diffraction a flat
Figr11.e 4.3 Esclr~rl~le of rru X-r.cry cl(fifi.ricfiorl (XRD) phcrse clictgr.anr of rr historic linre 17zo1.tci1.(Dz~lkscrnzl~le).F1.on7 Miclcle~rclo~f e f 01. (ill p~.e,ua~.ntiorz 2002).
MORTARS IN HISTORIC BUILDINGS: A REVIEW 01: T11E CONSERVATION, TECIINICAL AND SCIENT~FIC LITERATURE
powdered sample is exposed to a collimated X-ray beam which interacts with the sample and is diffracted back from the sample to a detector. The pattern of intensity of refraction with changing angle of incidence of the X-ray beam is characteristic of the mineralogy of the sample. In this way the composition of a mortar call be deter~nined.However, XRD is a bulk material analysis method. It can give no information on the spatial interrelationships of mortar components, or their structure. Figure 4.3 gives an example of an Xray diffractogra~nof a historic mortar. Lewin (1 98 1) makes use of x-ray diffraction to confirm the identification of mineral phases in specially prepared mortars in conjunction with SEM studies of ~nicrostructureand crystal shape. He states that XRD provides more useful information than that derived from chemical, ele~nental analysis by X-ray Fluorescence or wet chemical methods, which tend to mask the individual contributio~ls from different minerals. However, XRD cannot cope with the identification of amorphous components, cominonly C-S-H components of hydraulic mortars. Marchese (1980) studied the composition of nonhydraulic lime mortars forming the substrate of some 12th Century Mosaics in Salerno, Italy. Thermal analysis of the materials clearly identified the presence of Ca(OH), and CaCO,. However, the XRD analysis failed to pick out Ca(OH),. This discrepancy was attributed to the presence of Ca(OH), in an amorphous form. This emphasises the need for phases to be crystalline for XRD to identify them and the importance of not relying on one analysis technique. The application of XRD in combination with thermal analysis in this case revealed more about the nature of the constituents of the mortar than would have been apparent from using only one technique of analysis. Rayment and Pettifer (1987) in their study of the mortars from Hadrian's Wall, used XRD to positively identify C-S-H phases and Wollastonite (CS) in the mortars. Moropoulou et al. (2000) used XRD to study the mineral constituents of historic mortars from Rhodes, identifying mainly the mineralogy of the aggregates (better done visually by optical microscopy), the calcite binder and some hydraulic phases in some mortars. Franzini (2000) used XRD to conlplement electron microprobe and XRF chemical analyses of mortars from Pisa. They noted that the binders are composed of Ca-Carbonate phases, calcite, aragonite and vaterite. More than 100 ancient mortars from Italy, Greece, Crete and Cyprus of age ranging from 1400-3000 years, were examined using XRD by Langtoa and Roy (1984). They identified that calcite is the predominant crystalline phase in these ancient mortars. They also detected sn~aller quantities of hydrogarnet and analcime in pozzolanic Roman
mortars. Amorphous C-S-H phases were also detected even though the samples were LIPto 3000 years old. Middendorf and Knijfel (1991) also place XRD analysis within the context of a larger scheme for the analysis of historic mortars, to complement chemical analysis. They determined the composition of the aggregate from mortars in Northern Gerniany and also the presence of salts. Gulec and TLI~LIII (1997) present the results of the analysis of Roman, Byzantine and Ottoman mortars from Anatolia, using XRD, as well as optical petrography, aggregate grading and porosity ~neasureme~lts. The XRD analysis of the bulk mortars identified the phases present in the aggregate, the carbonate nature of the binder and some gypsum which was interpreted to be due to atmospheric pollution effects. Alvarez et al. (2000) perfornl a similar analysis on 13th Century mortars from Pa~nplonain Spain, identifying a lime (calcium carbonate) binder and a silica rich aggregate, and in co~nbinationwith chemical analysis and thermal analysis, deriving the original mix proportions of the mortars. XRD is also applied to the detection of crystallised alteration products that can be the cause of damaging reaction in mortars or cementitious binders, for example ettringite (Martinet & Quenee 2000) or thaumasite (Collepardi 1999). In summary XRD is a very useful technique for the determination of the crystalline, inineralogical components in a mortar. It is limited by being a bulk technique that does not reveal anything about texture or spatial distribution of the components in a mortar. However, it is quick and relatively inexpensive to use, but is best used together with other supporting che~nicaland textural analysis techniques.
4.2.4. Zizfm Red Spectromzetry This method of analysis relies on the interaction between applied infrared radiation and the molecules in compounds. Bonds between atoms have distinctive geometrys and natural states of rotation and vibration. Incident infrared radiation will excite these vibrations and rotations when a critical wavelength is reached that can impart energy to the bond. At this point the atomic bond that is being excited will absorb that wavelength of infrared. If the sample is placed between the source of infrared radiation and a detector, these times of abso~ptionof the infrared radiation can be recorded as reduced intensity and can be related to specific types of atomic bonds characteristic of particular functional groups in compounds, for example CO3 in carbonates. Infrared spectrometry is therefore suitable for the identification of materials and the study of chemical structure and the nature of inter-atomic bonds. For our purposes we are solely interested in the identification of mortar materials, primarily in the binder, and the possibilities for the quantification of their abundance.
Lee er al. (1997) demonstrate the potential for the use of infrared spectro~netryin the detern~inatiollof the Calcium Carbonate content of limestones. The benefits they showed are its ready calibration to other methods and the reduction in time and resources compared to conventional wet che~ilical methods. In another experimental study Hakanen and Koskikallio (1982) demonstrate that infrared spectrolnetry can be applied to the quantificatioil of artificial inixtures of aragonite and calcite with an accuracy of 3%, and Featherstone et al. (1984) quantified the content of carbonate in artificial carbonated apatites (Calcium phosphate) to a high level of certainty, using the ratios of transmission, absorption and extinction of carbonate correlated against known carbonate content. Though not directly collcerlled with the identification or quantification of materials in historic mortars, these studies demonstrate the potential for accurate determination of nlaterial quantities of carbonates using infrared spectrometry. In addition the technique appears relatively easy to use, requires small sanlples and is not time consuming. Studies of historic mortars that employ infrared spectrometry rarely use the technique in isolation. Most commonly it is used in co~llbinationwith X-ray diffraction (XRD), Ther~nogravimetry (TG) or Differential Thermal Analysis (DTA). For example P a a ~ n aet crl. (1998) studied mortars from a 13-14th Century church in Estonia. Simultaneous TGA and the analysis of the evolved gas by Fourier Transform Infrared Spectronletry (FTIR) was used in addition to Inductively Coupled Plasma Atonlic Emmissio~l Spectro~netry(ICP-AES) to characterise the materials in order to supply infornlation for the specification of replace~nentrestoration mortars. The combination of FTIR with TG confirms the evolution of water and CO2 from the samples. In two papers Luxan et 01. (1995, 1996) describe a comprel~ensive analysis scheme which includes infrared spectrometry. Gypsum was easily identified and confirmed by other techniques such as XRD and SEM analysis. In the later paper (1996) analysis of lime mortars from the Dominican Republic show that carbonate is easily recognised. Silicates (as SiO,) were revealed on the spectra, and the presence of CSH fibres confirmed by SEM investigations. The potential for recognising hydraulic components therefore also exists. Furthermore, Luxan et crl. also identify the presence of organic compounds, which the infrared method is particularly suited to identifying. Indeed, DomCnech Carbo e f crl. (1996) describe the application of FTIR to the study of the materials used in 16th-18th Century wall and canvas painting in Spain. Varnishes, pigments and other organic based substances can be identified easily. In addition the inorganic grounds of wall paintings are amenable to analysis also, with quartz calcite, gypsum and
anhydrite being revealed. The FTIR technique can use very sluall samples of less than 0.5mg with an area of less than 0.5mm2,making it well suited to the study of val~iableobjects or indeed building fabric. 111 another study, Appolonia (1995) applied infrared analysis to thc study of a latc plastcr coating coveri~lg l l th Century frescoes in Aosta Cathedral, Northern Italy. A large scale study of the nlaterial was mounted to facilitate its effective removal. Over 100 samples were taken and analysed by microdiffsaction, and FTlR with photoacoustic equipment. Both these techniques allowed the non-destructive measureme~~tof the samples 011 exterior and interior surfaces. The plaster was found to be linle with gypsunl that illcreased in quantity to the exterior surface. Finally, Bruni et crl. (1998) was able to distinguish between three mortar types colltaini~lg calcite, nlag~lesiteand hydromagnesite using FTIR and n~icroFTIR analysis as part of a schenie with thermal analysis (TG and DSc) and chemical analysis using ICP. Bruni concluded that it was possible to characterise all of these minerals successfully with FTIR, though no attempt was rtlade at quantification.
4.2.5. TIzei.rtzal Aizalysis (DTA aizd TGA, also known a s TG) Thermal analysis can be applied to mortars using three basic techniques, Therlnogravimetry (TG), Differential Thermal Analysis (DTA) and Differential Scanning Calorinletry (DSC). Each method, though having its distinct features gives approximately the same information, being based on the physical transformations that cornpounds experience on being heated in controlled conditions. Ther~nogravimetry measures the weight loss in a sample as it is heated. Weight loss during heating can be related to specific physical deco~npositionsin the materials that are due to the effects of increasi~ig temperature. For example gypsum can be recognised by weight loss between 120 and 200째C as it loses water and transforms to anhydrite. Differential Thermal Analysis (DTA) and Differential Scanning Calorimetry (DSC), are the most useful, and most used methods. In DTA a graph is continuously plotted during heating that shows the temperature difference between the sample and an inert standard of aluminium, which is heated at the same rate at the same time. Endotherrnic peaks are recorded when the standard continues to increase in temperature and the sample does not. At these times the sample is absorbing heat energy and using it to drive decolnposition or a mineralogical transformation, usually the loss of chemically bound elements, for example water from Gypsum or carbon dioxide from
MOKTAKS IS HISTORIC B~JII.DINGS: A REVIEW OF THE CONSER\~AI'ION, TECHNICAL ,\ND SCIENTIFI(' I.ITERAI'IIRE
Calcite and Dolomite. The endotherlnic or exotl~erlnic Ellis (op, cit.) however, does not deal with the analysis transitions are characteristic of particular minerals, of magnesian, or dolomitic, nort tars. Bruni et (11.(1998) which can be identified and quantified using DTA. st~ldiedinternal and external renderings ageing fro111 the 6th - 17th century. using TG and DSc. They were Differential Scamling Calorirnetry (DSC) follows the able to identify calcite (CaCO, 650°C), brucite (also same basic principle as DTA. Whereas temperature called hydrornagnesite Mg(OH), 350-400°C) and differences are measured in DTA, during heating using magnesite (MgC03 480-500°C). DSC, energy is added to maintain the sample and the reference material at the same temperature. This Newton and Sharp (1987, 19871) report in their study energy use is recorded and used as a measure of the of re~laissance plaster from the Sheffield area of calorific value of the thermal transitions that the England a majority of magnesian binders in their sample experiences (Willard et al. 1981). DTA and sample set. They successfully identify brucite and D S c possess another advantage over TG in the magnesite as well as calcite by XRD. Further study identification of minerals in mortars in that they are using DTA and TG corlfir~nedthis identification, but capable of resolving polymorphic tra~lsformatiollsin with added clarity. However, some uncertainty exists compounds that do not involve weight loss. A11 over the attribution of the endotherm often observed in example of this is given by Newton and Sharp (1987) the range 490-570°C, which could be due to either where quartz aggregate in plasters undergoes the ~nagnesite or portlandite (Ca(OH),- Calcium transition from p-quartz to a-quartz at 573°C. Hydroxide). Marchese (1980) studied 12th Century something they suggest could be usefully employed as lime based mosaic substrates from the Duolno in an internal temperature calibration. Salerno in Italy, and had identified the endotherm at Adams et (11. (1992, 1993 and 1998) use thermal 510°C as being due to portlandite. However, XRD of analysis as the primary technique in the the same samples failed to reveal ally portlandite, but characterisation of historic mortars and as the basis for only magnesite. Newton alld Sharp (op. cit.) contelld the study of the for~nulation alld behaviour of that the 5 10°C endothenll is due to magnesite, alld only replacement mortars, presumably for use in repairing found in their samples of dolomitic origin, quantified the historic structures in question, namely medieval by atomic absorption spectrometry. On preparing cathedrals in France and England. They are also experimental mixtures of pure magnesite and concerned with the study of the carbonation of the portlandite and testing them by DTA, it was found that historic mortars. However, the results are vague. The the endotllerms for ~nagnesiteand portlandite were first paper presents the most rigorous treatment of missing, but ones for calcite and brucite were present. mortar characterisation, with a straightforward A reaction between the portlandite and inagllesite was identification of calcite and gypsum. However, many clearly occurring during heating to generate calcite and related issues relating to sampling and sample brucite. Newton and Sharp convincingly confirm the preparation remain unclear thus lessenillg the utility of identification of the endotherm for ~nagrlesiteat around the results (the fraction of the mortar that was analysed SOOT, They also identified an important limitation in the use of thermal analysis to analyse inagnesian is not specified). binders that contain free ullcarbonated portlandite. Ellis (2000) introduces thermal analysis clearly and Paama ef ril. (1998) using TG-DTA provide progressively by presenting a range of examples of identifications of brucite at 350-420°C, magnesite at analysis of historic mortars, and classifying them 450-520°C, and also demonstrate how portlandite according to their contents, whilst acknowledging that decolnposes between 400-520°C allowing confusion similarities between mortars could be misleading, and with the identification of magnesite. They overcome hard and fast classification is near in~possiblegiven the this probleln by performing parallel analysis usillg variety of individual materials utilised historically. A FTIR and ICP-AES elemental analysis. range of colnpositions are identified, though some ambiguity is evident in the attribution of endotherll~ic The identification of hydraulic components in historic and exother~nicreactions seen in the ther~nographs. mortars using thermal analysis has not yet been For example Ellis suggests that an endotl~er~nic peak convillcingly demonstrated. The analysis of the between 100-130uC could be due to water loss from hydraulic components of Portland Cement is however CSH or from clays. The presence of Calcium Silicates well understood (Taylor 1990). The main hydraulic was suggested by correlation with chemical analysis clinker phases of Portland Cement C3S and C,S which revealed a proportion of Silicon, though it is not undergo phase transitions at a range of discrete made clear if this was derived from the binder or from temperatures from SOOT to 142S°C. This in principle the bulk mortar. Ellis concludes by cautioning against permits the identification of unhydrated C,S alld C,S in the use of thermal analysis in isolation and suggesting hydraulic mortars. However, C,S, which is likely to be the use of other chemical and mineralogical analysis more coinnlon in natural hydraulic lime and mortars methods to confirm identifications. found in historic buildings due to the lower
MORTARS IN HISTORIC BUILDINGS: A REVIEW
OF TIlE CONSERVATION,TECHNICAL ABD
SCIENTIFIC L11 ER141 LIRT
Fig1rr.e 4.4 . Historic G ~ I I S L I ~ ~ I 1iror.tcrr: The 111orp11oIogy of tile crystcrls visible aicl iri the iclerrt(ficrrtiorl gf gypsrrri~.Field
Figure 4.5: A tl11.eerlirlierlsiorlal ~ ~ i eofn a11 , isopach~rscolcite 11o1.elirlirlg irz N 12th Cerltzrly ~iio1.tc11.J.01li Il7i~el.IochyCastle. Bir~cler. s~rbstrateis to the left,follo~~erl by cr coalescerl layer. of perperidic~rlcricr>~stalg1.o11'tl7, topper1 by oper7 blaclecl cl:,utol g1.01~tl1 to the right. This is a cletcrilerl view of calcite c~:ystcils thrrt have gr.ouv~~'ithirlpore s l ~ c e sivithir~a11 historic nlortrrr; the ccrlrse o f ~ ~ l risa t C O I ~ ~ ~ ~ Irefel.rerl O ~ I I ~ to ~ as "rr~rtogerleozrshecrlir7gn ill olrl lin~e171o1.to1.s. Field of viei17 about 30 nricro1l.s (0.03 171177).
Figure 4.6: Scarzrliiig electron n~ic.l.oscope( S E M ) , RcrckSccrtterecl Elect~.oii(BSE) ilzlage sho~~~irlg enharicecl pol.osiy (Black) it7 Ilzl,er.lochy Castle 171ol.trr1: Pores li~zeclby ~~ecl:,~stcrlliserl calcitefr.i/lge, see111zer.e ir~liglzt grey. Field of l'iew 800 niicr.ons (0.8 1z1171). Sue11 ir71agesdepend 0 1 7 the cor7tr.ast irl atori7ic 11zr1irbera17d clensity of the mcrtericrls ill the saniple. 111\~estigatiorlof n~citerialszrsirzg BSE in7agirzg ~.eqzriresa flat polisher1 szrrlfnce to be p/.eparerl or7 c1 c1,osssection cut tl11.orrghthe scrrlll~le.
MORTARS IN HISTORIC BUILDINGS: A REVIEW
Hughes et crl. (1998) and Hughes and Cuthbert (2000) also make use of Back-Scattered Electron (BSE) i~nagingin the SEM on flat polished thin-sections. This technique is connnoaly used to study the microstructure of cementitious binders (Scrivener and Pratt 1984, St. John et al. 1998, Diamond 1999, Hooton and Brown 2001, Farny er al. 2001). The advantage of BSE imaging is that the grey level contrast in the images is based on the composition of the phases present within the material. This technique can therefore pick out col~lpositionalvariations and also be combined with chemical element analysis, that can be mapped across the sample, over a large area or in a single spot. The combinatioll of these two is very powerful and can aid in the identification of hydraulic conlponents (e.g. Callebaut et al. 2001) and hydration products in binders. Rayment and Pettifer (1987) apply BSE imaging to the characterisation of the hydraulic components of mortars from Hadrian's Wall and the reaction rims around chest grains in the aggregate. Lewin (1981), used the SEM to study the nature of a range of specially prepared mortars containing lime, hydraulic lirne, pozzolana, cement and normal aggregate. Several distinctive features of these could be identified by SEM, and the presence of hydraulic components in particular were identified. However, Lewin also used XRD to study the mortars and concluded that neither technique alone could provide an adequate characterisation of the mortars. He states that SEM reveals the "sizes, shapes, and textures of the internal structures in the mortar.. ., but morphology is not an una~nbiguous key to composition". He recommended an integrated analysis of which SEM plays a key role.
A new development in SEM technology, the Environmental Scanning Electron Microscope has recently become available to researchers. This version of the SEM allow samples to be viewed under wet conditions, controlled gas atmospheres and also during heat to up to 1000째C. This therefore permits the study, in real time of dynamic processes in materials, for example the hydration of quicklime, the calcination of stone or the carbonation of lime mortars (Allen et al. 2000, Radonjic et al. 2001). 4.2.7. Electrorz Microbeam arzalysis Another method of analysing the chemical composition of a nlaterial is to use electron beam methods. In these a beam of electrons is directed through a vacuum onto the sample to be analysed. Once hit by the electrons the material will emit x-ray radiation of varying wavelengths dependant on the elements present. The intensity of this radiation can be detected and its intensity related to the proportions of elements within the sample at the point the electron
CONSERVATION, TECHNICAL AND SCIENTIFIC LITERATURE
beain hits. Specialist analytical equipment exists called the Electron Microprobe, but the nleasurernent technique is now available on all Scanning Electron Microscopes, commonly referred to as EDS, or EDX Energy Dispersive X-ray analysis. The method is routinely used to confirm the identification of mineral species in historic mortar studies, especially when imaging of n~icrostructures is taking place (e.g. Callebaut et crl. 2001). However, quantitative analysis can also be applied to very accurately measure the chemical compositioll of mortar constituents, if a flat polished surface is prepared, in a polished thin-section or polished block. For example, Rayment and Pettifer (1987) applied the method to the characterisation of hydraulic phases (CS-H) and found that the ratios of CaO: SiO, in these phases was similar to those found in modern C-S-H phases, consistent with formation from P-C,S. Franzini et crl. (1999) studied the composition of 90 samples from Pisa to compare them with ancient pozzolanic mortars. They used EDX analysis to characterise the composition of the binder. They discovered pure non-hydraulic lime and hydraulic binders. They analysed the composition of the lime inclusions in both and found that the composition was approximately the same. Interpreting this as the original composition of the binder, being unmixed 'clots' in the mortar, it is suggested that the formation of the apparently hydraulic binder is due to the addition of a reactive siliceous aggregate, probably a diatomaceous earth. This will have acted as a pozzolan, even though no obvious pozzolan is identified in the mortar. In a later study Franzini et al. (2000) continue their investigations of mortar from Pisa. Normative calculations of the chemical composition of the binders are performed combining data from bulk analysis by X-ray Flourescence analysis, and the weight fractions of binder and aggregate, to derive volatile C 0 2 and H 2 0 contents of the mortars. The mortars consist of crystalline calcium carbonate mixed with an amorphous calcium silicate hydrate phase. Electron Microbeam techniques promise detailed and precise chemical analysis of mortars, that can be related to textures and component assemblages and reactions between them. Combined with SEM studies and BSE imaging it is another powerful method that has not yet seen much use in historic mortar studies.
4.2.8. Plzysical and Meclzaizical testing Physical testing of mortars predonlinantly encompasses the determination of properties such as the pore structure characteristics (capillarity, density, shrinkage, porosity, permeability, water absorption
MORTARS IN HISTORIC BUILDII~GS: A REVIE\\(
etc.) and also thermal expansion characteristics of mortar. Mechanical testlrlg includes measuring the strength characteristics of the mortar, the rnodulus of elasticity, adhesion bond and surface hardness, for example. Charola & Henriques (2000) considered that the characterisation of the physical and nlechanical properties may be sufficient for the compatible matching of mortars, and that the characterisation of composition is not necessary (see below section 4.4). Physical properties, especially porosity are frequently measured, but mechanical properties are not, due to difficulties over obtaining sufficient sample (Groot et al. 2000). Schouenborg et cr1..(1993)analysed the mechanical and physical properties of mortars froin three medieval churches in Sweden. In the field an adhesion test was performed by drilling a core and then recording the force required to pull the sample out. Compressive strength was measured in the laboratory, by halving the rather small samples and reassembling them with a thin layer of mortar in order to achieve the required thickness for the test. Most mortars achieved a strength of >4.5MPa, enough to satisfy Swedish Standards. Porosity was also nleasured by determining the weight, density and the bulk volume of the samples. The apparent density was measured by using a helium pycnometer. Frost resistance was measured along with capillary suction and drying. These tests were part of a comprehensive analysis scheme incorporating chemical and petrographic analysis. Binda and Baronio (1988) and Baronio and Binda (1988) characterise the densities of historic mortars in Italy, and also the Initial rate of absorption in a consideration of the nature of the brick-mortar bond. Moropoulou et al. (2000) tested the tensile strength of historic mortars using the method of Katsaragis (1987) and Tassios et al. (1989). They found an inverse relationship between this property and the ratio of C0,:structurally bound water. They found that as hydraulicity increases (with decreasing CO, levels) the tensile strength increases. Porosity can be measured in mortars using a variety of different methods ranging from the relatively simple to the complex and instrumental (Thomson ef al. 2002, in 11re11~1'afion).These can include indirect nlethods such as simple saturation density methods, mercury intrusion porosimetry, and indirect petrographic methods using automated image analysis. Some indirect methods such as mercury intrusion porosimetry are considered by some to be inappropriate for use on lime-based mortars as they damage the texture of the mortar and lead to incorrect estimations of porosity. See also sectioa 5.3.1. for more iaforrnation about mortar porosity.
CONSERVIYI'ION. TECHNICAL .\ND SCIENTIFIC LITEKATURE
VBlek et crl., (2000), experimented with the application of in-situ gas permeability measurements on nlortar and sandstone. This is a non-destructive test, where a probe is sealed by pressure against the surface of interest and nitrogen gas pumped under pressure into the material under test. The gas flow rate into the material and pressure are recorded once a steady state is reached and can be used to calculate the permeability. They were able to measure the perrueability of sandstone with reasonable repeatability, b ~ t tthe variability of the lneasurenlents was high due to variability in the cross-bedded sa~ldstonethat was tested. This was attributed to grain size variations in the sandstone and the nloisture content of the stone. Testing of laboratory prepared lime Illortars revealed a major control of results was due to surface finish, more than the effects of curing conditions. VBlek et al. (2000) conclude that the method was considered to have s o ~ u euse in the deter~ninationof the compatibility of original and new materials.
4.3. General Analysis Schemes Ma~iy attempts have been made to systemise the analysis of mortars fro111 historic buildings and to establish protocols for co11lparison of results derived froru different analyses. (For example Charola et 01. 1986, Middendorf and Knofel 1991, 1998, Dupas and Charola 1986, Goins 2000, van Bale11 ef crl. 2000, Martinet and Quenee 2000, Callebaut er al. 1999, 2000). Middendorf and Knofel (1991 and 1998) worked 011 the for~nulationof a number of flow charts to assist in mineralogical, chemical, and physical characterisation. These, as well as other schemes, can be applied as an aid to analysis - not as proscriptive schemes. These charts give a comprehensive idea of the possibilities for characterisation in the different fields as described above, and also put useful constraints upoil the sample requirements and sample preparation needed. They clarify the potential pathways for analysis, allowing analysts to chose that appropriate for their purposes, without precluding the later use of other methods. The conservative use of sample should be encouraged, if the range of potential analysis is understood, reducing the need for later re-sampling on-site (Van Hees 2000). Callebaut (2000) also presents a similar detailed procedure combining a full range of ~llineralogicaland chemical techniques. He emphasises how early analysis schemes concentrated mostly on wet chemical nlethods (Jedrzejewska 1960, Cliver 1974, Dupas 1981), whereas Inore modern approaches incoiyorate more mineralogical and petrographic methods. They are even beginning to incorporate inore physical
M O R ~ ~INI <HISTORIC S BUILDINGS: A REVIEW OF TllG CONSERVY~I'ION, TECHNICAJ~ AND SCIENTIFIC LITERATURE
characterisation as well as co~npositionalstudies, as the properties needed for the specification of new or replacement mortars develops its concept of compatibility. Physical characterisation for strength and porosity for example are becollling more common (Baronio and Binda 1991, Knofel and Schubert 1999, Van Bale11 1999). No standard coinbination of methods, and as we have seen, no standardisatio~l amongst inethods exists at present. This presents aproblem of comparability between results and between laboratories, also leading to some co~lfusion about the important parameters that should be measured.
4.4. Characterisation with a view to repair Groot ef al. (2000) discuss the need for the specification of parameters that should be characterised in order to better for~nulatea repair mortar that will be co~npatiblewith existing building fabric. The activities of the RILEM TC-167COM "Characterisation of Old Mortars with Respect to their Repair" have been aimed at clarifying this, and the ~nethods needed for characterisation. The publication of the workshop proceedings from the committee in 2000 (Bartos et al., 2000), contributed significantly to the debate. The relevance of detailed knowledge regarding the characterisation of old mortars is considered by Leslie and Gibbons (2000). One of the most important factors in the analysis of old mortars is an understanding of the surrounding building structure and conditions. The same applies to the existing function of the mortar. An interesting example ill this respect is the differences in f i ~ ~ l c t iof o ~'sealing' l inortars in dry stone build with no mechanical function (Maxwell 2000) and thick joint rnasoilry (Byzantine, Baronio and Binda, 2000) that have a significant mechanical function. Leslie and Gibbons also observed that the data that are relevant to the requirements of building conservation are in general: the hpdraulicity of the binder, the
relative weights of binder and aggregate and the aggregate grading in order to identify the necessary colnponents to produce a co~npatible mortar. This information can be obtained througl~ si~uple examination by eye and binocular microscope coupled with acid dissolutio~land aggregate separation, and does not necessarily require expensive analyses. More emphasis on porosity and strength characterisation was advocated by Charola & Henriques (2000). It would appear that the identification of actual hydraulic colnponents may not be necessary for either the characterisation of the mortar or the development of a successful formulation for its replacement. Determination of porosity characteristics related to strength may serve as a Illore important guideline for matching repair mortars to existing ones in historic structures, than detailed knowledge of hydraulic components. The work of Vilek et al. (2000) on the in-situ gas permeability of masonry Inay relate a porosity-related property indirectly to strength and hydraulic properties. This approach underlines the importance of the characterisation of moisture condition and behaviour within masonry. However, again it appears that a co~llbillatio~l of ~nethodsis perhaps more appropriate for characterisation. The notion of "external requireme~lts" having an influence on both the analysis of historic mortars and the forinulation of their replacements is now being discussed, though has not reached publication at the time of writing (early 2002). What is meant is the influence of issues such as conservation philosophy, authenticity (as defined by the Nara Document, 1995) cost etc. These are issues "external" to the technical analysis and characterisation of the mortars that will affect how they are sampled, analysed and reformulated (Van Balen et 01. 2002, in preparation). However, this is contentious and some believe best left to architects or building conservators, not scientists.
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSEKVKI'ION, TECHNICAL A N D SCIENTIFIC LITERATURE
DESIGN AND DEVELOPMENT OF NEW MORTARS
This section reviews current efforts in tlie development of mortars intended for the conservation of historic buildings. It concerns the design and testing of new mortars, and the final steps of the whole procedure before the ultimate application of conservation treatment. The previous chapter detailed evaluation and analysis of liistoric nlortars and masonry where all the infornlation was collected with an apparent aim to specify replacen~ents. In this chapter the extent to which this relationship affects the develop~nentof new mortars is explored further. Tlie latest results of practical, research, theoretical and experimental work are presented and assessed, together with a review of novel means of testing. Much of the following text also relates closely to tlie previous discussion on compatibility of materials in historic buildings.
tests should be apparently enlployed as well, since Inany standard tests are not suitable for testing traditional tnaterials (Cliarola and Henriques 1999). The method of testing, whether based on cornposition or performance, sliould be clearly identified. Confusion between these two may later lead to problenis (Henriques and Charola 1996). Both methods are based on a sinlilar procedure which extends from examination of liistoric nlaterials to testing and selection of the adequate mortar. The result, the new repair Inortar described by its performance characteristics, should in both cases be compatible with original materials. On the other hand, the difference between these two approaches is the range of criteria on which the materials are compared. Water vapour per~i~eability
5.1. Specification and performance of new mortars Whenever a new repair lnortar is to be designed, the 'compatibility testing approach' should be used. It ensures that the new lnortar is compatible with the original one. Gonqalves (1998) described a methodology used for the design of a new compatible render, which typifies the latest ideas behind the compatible design of new mortars. It stemmed from the definition of compatibility which stated that a new material should fulfil all the functions required from it and should not introduce any new damaging actions. This definition of compatibility describes general requirements which have to be interpreted for its practical application. It has to be expressed with regard to the particular conservation treatment, materials and conditions. In general, it is known as specifications for new repair mortar. For example, one of the compatibility specifications used by Gonqalves (1998) was that the new render should 'not block the passage of the water vapour that circulates due to the gradient of water vapour pressure between the interior and the exterior of the building, by retaining it inside the wall'. The specifications for new mortars should reflect their nature. They should be based on scientific results from research into material properties (Von Konow 1998). A number of specification criteria are usually defined. In order to find the right material which complies with these particular specifications, appropriate testing methods have to be detelmined. Standardised and approved testing methods are usually utilised, but new
Capillarity Capability for i~l~pel.~neabilisation
PH and soluble salts content (chlorides, sulphates and alkalis) Adherence to support Resistance to cracking Resistance to inipact of a round body Resistance of renders to salt cl.ystaIlisation Artificial ageing tests - lieatlrain, hot/cold, fi.eezeltliaw
Tnble 5.1: Esnn~pleo f solne per;for.n~n/zcechrirncter~isticsto to Conc.rih~es be nieas~rreclfor rlew r.er1r1er.sricco~.rlir~g
(1998). Criteria and tests for selection of new compatible mortar have been the subject of research for some time now (Peroni et al. 198 1, Rossi-Doria 1986). Peroni et al. (1981) recognised the importance of defining technical criteria in order to ensure a inore appropriate selection of lnortars for conservation purposes. The authors suggested a number of tests which should be accon~plishedto describe a perfor~nanceof mortars. They also imposed certain limits which should ensure compatibility of mortars. These limits were designed to inhibit the known cases of masonry decay, i.e. high soluble salt content, or too high co~npressivestrength. To summarise the procedure from the literature above, the best way to design a new compatible mortar seems to be to determine the properties relevant to potential damage of the host masonry and consequently ensure that the new ~nortai-fits within the range of these imposed limits.
MORTARS IN HISTORIC BUILDINS: A REVIEW
Mortars should have optirnum workability
Three days maximum. although for some applications tcn days Illay be tolerated
Compressive strength New inortars should not be much stronger than the ones used in the old masonry (0.5 3.0 MPa is advisable).
C O M ~ R V A ITLCI-~NICAL ~ O N , AND SCIENTIFIC LITERATURE
rendering. The inortars were compared on a basis related to their ability not to contribute to any further damage. The requirements from the new lnortar were as follows: not to transmit any I~ighstress to the substrate
It is dcsirablc for this to be reasonably large but not exceedingly so (0.4 2.5 MPa)
not to retain water within the construction not to have a high salt content.
Tliere is no exact range recotnmended
Minimum 20% \vith at least 65% above 0. l Lr
Ililporta~itfactor but sug_pestcd
Water vapoul. pei~ileability
Minimum value may be desirable but no exact range was suggested
As low as possible. 8111gJkg might be reasonable.
Tnble 5.2: Ceizercrl c~.itrr.irrfor. selectior~o f r.eprri1. ir~or.tnr.s nccordirlg to Per.oni et 01. (1981)
The successful design of a compatible mortar lies in the ability to characterise properties of mortars and a selection of appropriate tests. Standard tests are often designed for testing modern materials only and therefore they are not relevant to traditional materials. There is a need to study and modify these tests, and it has been described during a conference 'The Use of and Need of Preservation Standards in Architectural Conservation' (Sickels-Taves (ed.) 1999). On the other hand, the selection of appropriate tests is more difficult as it is not certain what is a measure of quality of mortar in general. There is not a single characteristic that would bc able to describe coinpatibility and a number of tests have to be used instead. However, how Inany tests are needed and their hierarchy have not yet been satisfactorily defined. Therefore, the general list of properties to be tested can extend to a large number of tests in order to cover all possible sources of damage. Usually, colnpressive strength, porosity, permeability, composition, thermal expansion etc. are Inore or less relevant depending on the particular case. However, it should be understood that every conservation project has slightly different requirelnents and therefore different criteria for selection of a new mortar. Carefully defined criteria for the selection of a new mortar, based on the understanding of original material and required remedial actions, should lead to the selection of an appropriate material. However, there is a need for more relevant tests which would deal directly with the problems related to the applications of new mortars. An example of the development of more appropriate tests can be studied in a work of Veiga and Carvalho (1998) who coinpared performance of lime, cement and lime gauged with cement lnortars used for
Judged by these criteria, the lime-based mortar was considered to have the nlost suitable behaviour. On the other hand, the linle mortar failed the freezelthaw testing. If the nlortar had been evaluated according to durability represented by the freezelthaw testing, then it would not have been the most suitable. This fact illustrates the i~nportanceof selection criteria.
5.1.1. Exanzples of design of rzew ntortars The following are three examples of how co~npatibility and design of new repair Inortars have been approached. (i) Papayianni et crl. (2000) suggested designing a new lnortar according to its 'functional behaviour'. This ineans that conlpatibility should be measured by properties characterising the functions of mortar in the structure. According to the authors (op. cit.) the characteristics were as follows: colour and surface structure strength, elasticity and deformability porosity and porosity properties coefficient of thermal dilation First of all, historic mortars were analysed (microscopic examination, aggregate grading, porosity, colnpressive strength, chemical composition and soluble salts). All the historic mortars except one appeared to be lime-based. Different mortar nlixes were designed col-sespondingly to cover the variety of mortars present in the different parts of the structure. The design of the new mortar was controlled mainly by colnposition (binder and filler proportions) combined with porosity and strength. Colour of the mix was adjusted by the colour of aggregate. Porosity and compressive strength were tested to confirnl the compatibility of mortars. Although the strength of the new mortars was slightly higher than that of the historic mortars the authors concluded that the nlortars are compatible. No further evaluation of the perforlnance was carried out after the application. It should be noted that the materials used in the composition of new lnortars were not of the same provenance as that contained by the original mortar and
MORTARS IN HISTORIC BUILDINGS. A RE\JIE\V
CONSERVATION, TFCHNICAL /\NI) SCIENTIFIC LITERATURE
a white celnent was even added into some mixes. Although the design seemed to be based predominantly it did not try to copy the colnposition on compositio~~, of tlie original mortar. Rather, it considered the general properties which these original mortars possessed. On the other hand, the paper did not explain why and how relevant the tested properties (such as the co~npressive strength and porosity) were to compatibility. No exact specificatio~ls or criteria that would relate to the historic masonry, other than the general ones lnentioned above, were specified. Although the design was not based purely 011 coniposition or performance parameters, it represented the conlmon approach towards it. The validity of tlie method and the compatibility of the lnortars are yet to be confinned. (ii) Veiga and Carvalho (1998) studied the appropriateness of using lime-based lnortars for renders. The aim was to collipare lime, lime-cement and celnent lnortars in relatio~lto their application for conservation projects. Testing procedures were developed to describe the most crucial characteristics relevant to the compatibility specification of renders (Veiga and Carvalho 1998). The testing was divided into the following three main sections.
permeable. The drying phase especially was ~nuch faster for linle Inortars in conlparison to mortars with cement. No significant degradation was observed for heatlcold and heattrain cycles for all mortar specimens, however the freeze/thaw caused degradation of the lime nlortars in a few cycles. The overall conclusion was that lime-based renders have the most suitable perforlnance characteristics compared with mortars gauged with cement or pure celnent mortars. The comparison and subsequent selection was based on the requirement that new nlortar should not cause any further damage to the original masonry. This was a simplified definitio~iof compatibility and the lnortars were studied strictly from this point. However, the paper did not have tlie scope to describe and verify the results on any real application, apart from the general experience of using lime-based renders. The research should be backed up with some practical results.
(iii) Van Balen et cil. (1999) described a case study of the use of epoxy resin and fibreglass rods as binding materials for anastylosis of the late Hellenistic Nymphaeum in Turkey. The paper explained not only compatibility, but also the authenticity, retreatability and reversibility requirements on the design of joints E~~cilucrfionof stress ~.z'ifhir?the ~uortur u11c1 between individual stones. The design also reflected e~wlzrutior~ o f fensile I-esistcrnce.Transmission of a the conditions in whicli the Nymphaeu~nis situated. It stress from mortars (renders) to the substrate lies in a seismic zone where earthquake is one of the masonry could cause damage to the substrate. major threats to the historic buildings. Therefore such translnission should be limited. The The use of ~llodernmaterial with a high mechanical authors focused on stresses caused by restrained strength ensured that intervention was kept to a shrinkage measured by a methodology (evaluation minimum. The connection between individual building of cracking susceptibility of renders) described by blocks was based on the installation of dowels which Veiga (1998). The method operates with two criteria should resist the stresses between stones. On the other for description of cracking susceptibility. The first hand, the design of the dowels incorporated a criterion is a coefficient of opening of the first crack limitation that the new connection between the stones (maximum load force divided by tensile strength). should break first, before any damage is caused to the The second criterion is a coefficient of resistance to original masonry. Retreatability was considered in the cracking evolution (tensile rupture energy divided design as a case of saving the stones undamaged, by tensile strength). should an earthquake strike tlie building, to allow the reconstruction to be repeated. E~~nlrratiorz of the crhrlltj to protect the lull ugni~zst
ingl-ess of wwtei.. An electric resistance of lnortars was measured to determine the time taken for water to reach the substrate and consequently to dry out. E~~crl~rcitrorz of tlze clurubility c o ~ ~ c e r i ~cli7natic i~~g actions. Speci~nens of different renders were exposed to heatlcold, heat/rain and freezelthaw cycles. Fro111 the results obtained, the authors (Veiga and Carvalho 1998) concluded that forces developed due to restrained shrinkage in lime mortars are much smaller than those developed in cement mortars. Moreover, nlortars based on lime were less susceptible to cracking than mortars with cement or pure cenient mortars (Veiga 1998). Lime nlortars were the most water
The technical part of the project dealt mainly with a test of tlie epoxy joints to design a proper balance between the strength of the stone and epoxy resin. Compatibility was considered on the basis that the stone should not be damaged by mechanical stress. The epoxy resin in the joint should fail before any damage to the stone occurs. The adhesion of the epoxy resin was reduced by the addition of a filler whicli contained powdered limestone. Construction details of vertical and horizontal joints bridged by the fibreglass dowels were another part of the design which had an effect on the behaviour of the structure and therefore on colnpatibility and retreatability. The fibreglass dowels were designed to break instead of being pulled out when under an excessive load and therefore to give a
MORTARS 1R HISTORIC BUILDINGS: A REVIEW
limited ductility to the joints (Van Balen et 01. 1999). This last example illustrates that under certain circumstances a nod ern material (non-original) can be used in conservation. In such a case its use has to be fully co~npatiblewith the historic material, and other conservation requirements such as reversibility and/or retreatability have to be fulfilled. In this design, the compatibility of the mortar and the binding elenients was considered mainly from a structural point of view. On the other hand, any potential weathering problelns have not been taken into account. The paper delnonstrates that the criteria for a compatible repair mortar should cosrespo~ldto the conditions in which the structure is situated and which are relevant to potential damaging processes.
5.1.2. Design based on coi?zpositiorzaizdlor properties Groot et al. (2000) and Gonqalves (1 998) described the design of new mortar as a trnditiorzal one, based on composition, and a rnodel.rz one, based on properties. Groot et al. (2000) pointed out that there should be a mutual understanding of these two ways of design. Understanding what are the distinctions and common points of these two approaches helps to define the most important parameters when designing a new compatible mortar. Factors Affecting the Design of N ~ M Mortar , Basecl on Co11100sitio11 The analysis of historic mortars allows a copy of original mortar to be designed and such an approach is now common in the conservation of historic masonry (e.g. Florez de la Colina 2000, 'Analysis of old mortars from ancient ugoru of Thessaloniky, Greece'). However, properties of mortars based on composition similar to the original ones are not compatible a prio7.i and should be tested. VBlek & Bartos (2001) pointed out that to copy properties of historic lime-based
CONSERVATION, TECHNICAL AND SCIENTIFIC LITERATURE
mortars, such as strength and porosity, lnerely by composition was very unpredictable, as there were other influences that affected the properties. The performance of lime Illortars is influe~lcedby Inany factors. Even the co~npositio~l itself can be highly variable depending on the original limestone, burning and slaking conditions and type of aggregate (Jedrzejewska 1981). Sonle material researchers even suggest that there are too nlany influencing factors on old lnortars that they are impossible to copy (Von Konow 1993). A si~nilarconclusion was reached by Hughes et 01. (1999) when the authors pointed out that physical changes of li~llemortars caused by ageing Inay inhibit the deterlninatio~lof the original mortar composition. When a new mortar is based on a coinpositional copy of the original mortar, a question of the accuracy of such a copy should be considered. In some cases the provenance of the raw nlortar materials (limestone, sand, pozzolana, etc.) or exact production techniques can be very significant. From a conservation point of view it may be argued that when mortar requires a periodic maintenance and repair the traditional techniques should be employed (see Declaration of San Antonio 1996). Hughes et crl. (2000) initiated a new research project into traditional lime burning. A newly built replica of a traditional lime kiln equipped with a monitoring system aims to research traditionally burned limestone in Scotland. Durability and performance of non-hydraulic lime lnortars are limited not only by the material itself but also by workmanship, ageing and curing conditions and stone and mortar interaction (Bartos and Lawson 1996). Because the performance of lime lnortars is influenced by so many factors, the specification of repair mortar based on the colnposition of the historic mortar should consider information about the repair work to be carried out, the type of masonry and climate (Leslie & Gibbons 2000). One of the most important influential factors on non-
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSERVATION, TECHNICAL AND SC~ENTIFIC LITERATURE
properties to the historic masonry (e.g. Torraca, 1988). Conservation literature in many cases (e.g. Gibbons 1995) simplifies the problem of compatibility as the decision to use lime-based mortar instead of cement mortar. This results from bad experiences of using cement mortars in the past. When assessing past conservation attempts the two following points often appear:
fundamental properties of new lime mortars is therefore required to back up the demands from conservation practice to use original materials (lime mortar) for conservation works (Furlan 1991, V6lek 2000).
Firstly, the lime technology and skills were partially forgotten (Gibbons op. cit.). Secondly, Portland cement superseded lime because of its superiority in strength (Gibbons op. cit.) but other qualities of lime mortar were not properly considered. These two points can be seen from a compatibility perspective. Correct application of lime mortar requires special training and care to be successful (Maxwell 1998, Gibbons 1995). Although the use of cement-based mortars was widespread, their compatibility was not considered and they were often found later to be incompatible with the original Figure 5.2: Is this mortar compatible with the masonry? masonry material. There is a general consensus Red sandstone ashlar masoniy in Pazsley. Cement based between scientific and conservation literature pointing mortar together with moisture and salt transport is often thought to cause such typical decay round the joints. regarding these two points. However, the preceding The adjoining white sandstone is not suffering such review of the latest trends in conservation science extensive damage, suggesting the mortar is more compatible indicates that a detailed acquaintance with many with that stone I-egardlessof its composition. material properties is vital in designing a compatible material. It can be said that the better a particular material is described in terms of its properties, the better result is obtained in terms of material compatibility. A serious study of the apparent causal relationship between the use of cement-based mortars and stone and brick decay is still lacking, so statements regarding the incompatibility of cement and its rejection by the conservation practitioners are not backed by detailed quantitative evidence. Research into mortar and concrete based on Portland Cement appears much more advanced and profound than that on lime (e.g. Hewlett 1998). The research reflects the use of cement and concrete in the modem building industry. This point illustrates the fact that there are no international lime oriented research journals (some national journals exist, e.g. The Journal of the Building Limes Forum) and research articles about lime and lime mortars are often found in journals (oriented mainly towards cement and concrete) such as Cement and Concrete Research, Concrete International, Materials and Structures, Magazine of Concrete Research, Construction and Building Research, Brick N e w s , Magazine of Masonry Constructions, Thermochimica Acta, Masonry International, Journal of American Ceramic Society
etc. In future it may appear that a lack of exact scientific knowledge of lime and lime mortars will be the greatest drawback in its proper use as a compatible material. A more detailed understanding of
Figure 5.3: Is this nzortar compatible with masonry? Red sandstone masonry has weathered due to wind exposure zn combination with moistui-e evaporation. However, the Izai-d pointing mortar has determined the weathering pattern and helped the weathering rather than protecting the masonry. It could also be said that the combination on a masonry surface of such materials with contrasting durabiliv (related to the bond between components and overall hardness) has resulted over time in this aesthetically problematical weathering pattern, as the sandstone weathers away more readily than the cement-based mortal:
Figure 5.4: Is this nzortar compatible with masonly? Cenzent-based mortar is a good binder and can locally support the adjacent stone to nzortar joint. Howeller; the n~asonrystill weathers and its appearar~ceis changing. The nzortar in joints is protruding and visually expanding but stones are dinzinishing.
5.2.1. General composition and strength Suter and Song (1995), in their review of historic stone masonry properties, suggested that the compressive strength of the original mortars can be expected within the range of 0.1 and 3.5 MPa. The binder to aggregate ratio was found in the range of 1:0.4 and 1:s with the majority being 1:3 (Suter and Song 1995). Durability of lime based mortars can vary depending on their ageing conditions but examples of historic mortars surviving well over 600 years old are available worldwide. Longevity of the surviving masonry of historic structures is a proof of the quality of workmanship and empirical knowledge of the past. However, the exact reasons for such longevity and durability are difficult to determine due to their complexity.
Figure 5.5: Historic m r t a r sample@m Tantallon Castle, E& Lothian. The paper label attached EO the sample is around 3 cm across. The general texture offhis i~rternal fracture s d a c e of an hktoric mortar (early 16th Cent* can be seen clea~ly.Poorly serted aggmgate contains ruunderl dark basaltic rack Ji-agments and red cnloured intermediate $0siliceous extrwive igneous wckfiagmertts. There are also some more angd@fiagments of charual in this specimen.
New non-hydraulic lime based mortars are expected to have a relatively low compressive strength, approximately 0.5-3MPa (recommended by Peroni et al. (1981)) and are expected to adjust to seasonal and minor structural movement without damage (Gibbons TAN 1 1995, Binda et al. 2000). Their durability is considered rather poor, especially in conditions where the temperature drops below zero.
5.2.2. Properties and compatibility of non-hydraulic lime mortars Sass and Snethlage (1997) defined limits within which the properties of a new repair mortar should fall to ensure its compatibility with the original one (see Chapter 3). The limits were expressed as a percentage
Figure 5.6 Nistoric mortar smiplefrom S t Andrews Cafhedrcalprecinct wall fwrly 16th Century). 7;hB image shows an external weathoed sadace ofthe mortar, which is darkened compared $0 aj-esh unweathered s f a c e . The weathering c m accentme features dike the aggregate, especially iJ: the lira bindfr is prefert3ntialSy weathered away.
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSERVATION, TECHNICAL A N D SCIENI II.1C
of properties of mortars over properties of stones. Bromblet (2000) evaluated this method of compatibility determination. Mortars were made of hydrated lime and fine sand with the addition of a powder from the particular stone relevant to the repaired masonry. The mortars and stones were both tested for compressive and flexural strength, porosity, thermal and hygric dilatations, and adhesion to the surface. The results concluded that the mortars were all porous, capillary materials with a negligible amount of soluble salts, low adhesion and a great crack sensitivity. The porosity and capillarity of the mortars were affected by the addition of the stone powder. The mortars made with stone powder were found to be closer in some properties (porosity) to the stones from which the powder was made (Bromblet 2000). In terms of compatibility with the properties of the stones only one mortar fulfilled the requirements based on the research of Sass and Snethlage (1997). It was concluded that the mortars which failed the compatibility requireme~lts possessed too low capillarity, adhesion and mechanical strength. Or, conversely, the value of these properties in the stones was too high. The results question the appropriateness of these general compatibility limits for lime-based mortars in relation to masonry.
5.2.3. Modern and traditioital renders Marie-Victoire & Bromblet (2000) carried out a comparative experimental study on five modern cement-based mortars and t h e e traditional lime-based mortars used for rendering in France. A number of tests was canied out including water retentivity, settingtime, shsinkage, porosity, capillarity, water and water vapour permeability, compressive and flexural strength, surface hardness and adhesion. The results confirmed that the moder11 ready-mixed rendering mortars are in general too impermeable and strong for co~lservation purposes (Marie-Victoire & Bromblet 2000). However, some of them had a number of parameters comparable with the lime-based renders which seemed to be more compatible with the masonry. Each mortar could be appropriate for different specific requirements of different masonry collservation works. This conclusioa supported the use of modern materials and stressed the need for specifications of good compatibility criteria. 5.2.4. Hot inixiizp Callebaut et al. (2000) examined properties of new non-hydraulic lime mortars in relation to a production technique known as hot mixing (sometimes also called dry mixing). Their experimental work stemmed from analysis of historic mortars and observatioll of a
presence of white rounded lime lumps (lime inclusions) which can be associated with the hot mixing method (Leslie and Gibbons 2000). In this method quicklime is slaked while mixing with sand and water. The mortar can be applied cold, while still warm and even mixed and slaked within the structure (Gibbons 1993). Some papers indicated that these hot mixed mortars possess a better bond between the aggregate and binder as a result of etching of the surface of aggregate grains (Jedrzejewska 1967). The results from mechanical testing showed that the hot lime mixing method produced mortars with a relatively high strength (Callebaut et al. 2000). Specimens were prepared from non-hydraulic lime slaked with sand and kept together for 7 days prior to casting. The values of cornpressive and tensile strength were compared with the results of Van Balen's (1991) earlier testing of a commercial hydrated lime mortar mix. The curing and ageing conditions were kept the same to maintain the comparability of the results. The hot mixing method produced mortars with higher mechanical strength. Calleba~itet al. (2000) suggested that the hot mixing method had been used in the past to produce high strength and durable lime-based mortars. Armelao et al. (2000) suggested that when a hot mixed mortar had been applied still hot, the higher temperature of the mortar could have favoured an interaction of calcium and silica and consequently it could have led to the creation of a better adhesion bond between these materials. The authors' objective was to study a bond between lime mortar and clay brick and they concluded that the calcium penetrates into the clay brick's pore system where it forms a layer of calcium silicate.
5.2.5. Ageing of linze putty The effect of ageing on lime putty was studied by Hansen et NI. (2000). The authors measured viscosity (consistency) and workability (water retention) of an aged lime putty, and flow of a mortar mix made of the aged putty. They concluded that the aged putty (16 years) performed better due to the reduction of lime particles in size with ageing. The water retention, consistency and flow tests implied that water absorbed in the older (16 years) lime putty was harder to remove by mechanical action in comparison with the younger putty (2 years). However, ageing alone may be insufficient to ensure improvement for certain types of lime. Factors such as limestone source, burning temperature, particle reactivity and slaking conditions can influence the size of crystals and affect the ageing characteristics of lime putty (Hansen et al.). Thomson (2000) used a surface area test to compare particle sizes of dolomitic hydrates and putties, high
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSEIIVATION, TECHNICAL AND SCIENT~FIC LITERATlJRE
calcium putty and a high calcium hydrate. The lime putty (made i11 laboratory) possessed very small particles. Thomson (2000) concluded that, in this case, a further reduction of the particles was very unlikely and therefore the ageing of lime putty to reduce the particles in size nlay not be coinpletely relevant. According to Tholnson (20001, the ageing (maturing) of lime putty provides mainly a colnpletioll of the slaking process.
5.2.6. Addition of brick dz~st Addition of brick dust into lime mortars can improve their strength and durability. The results from the Smeaton project (Teutonic0 1994) suggested that the clay type and its firing temperature are the factors which affect the performance of mortars. Hughes & Sugden (2000) followed this research in experimental work on hydraulic lime mortars. The authors concluded that the fineness of tlie brick dust and the curing conditions are the most relevant parameters to be altered in order to maximise improvement i11 strength. Papayianni & Theocharidou (1993) concluded that the addition of brick powder contributes to strength but it also lowers the capillary rise rate. It could also increase the water retentivity of mortars (Papayianni & Theocharidou 1993).
5.2.7. Carborzation of lime nzortars Carbonation of non-hydraulic lime mortars is considered to be the most important process of hardening and it has a direct influence on durability and strength of the mortars. Carbonation of new lime mortar call take several months, but there are also examples when carbonation of a mortar inside masonry took more than several hundred years (Hosek and Muk 1989). Hughes et al. (1998) suggested that the factors that affect initial carbonation (and hardening) i11 the short term might have less influence on tlie durability and physical properties of historic mortars in the long term. Calcium carbonate is soluble and when water is present the carbonated particles can be dissolved and consequelltly precipitate, changing completely the pore structure and strength of a mortar. When mortar carbonates, it gains mass and its porosity decreases (Parrot 1991-92). However, in a longer term, porosity can increase due to the dissolutioll of calcium carbonate, mechanical deterioration, micro cracks caused by load, salt and frost attacks. As a result of this the strength and other properties of mortars vary significantly depending on ageing conditions. In Scotland there are examples of very friable mortars as well as very hard and dense mortars both made from non-hydraulic lime but exposed to different
environme~ltal coilditio~ls (Hughes 1998). Some of these relatively hard and strong mortars have a very high porosity. During the initial hardening of mortars the rate of carbonation depends on the mortar surface finish and its permeability (Vklek et al. 2000 Madrid). Carbonation call be slowed down by a reduction of permeability and diffusivity. Such reduction may occur due to a reduction of pore sizes induced by a progressioll of the carbonation iiiwards from the surface (Hilsdorf et N I . no date) and inhibiting CO, entering deeper into the mortar.
5.3. Research into nature of nort tar properties Torraca (1988) described deterioration mechanisms of porous materials. Moisture (and its movement) is the most common degradation agent in conservation. Pore structure and various moisture transport mechanisms are therefore often cosselated to durability of porous materials. A great deal of literature has been written about moisture transports in porous materials (e.g. Meng 1994). However, practical i~lterpretatio~l of this theoretical research is still loose. A recent example of research on salt and moisture trailsport in porous ~naterialsand its trallslatioll into practical suggestions for desalination of painted brick vaults has been presented by Larsen (1999). Even the properties such as porosity and/or permeability, which are commonly tested, are not well col-selated to practical applications. Marie-Victoire & Bromblet (2000) pointed out the difficulties with the interpretation of porosity and permeability measurements on rendering mortars. Urlderstanding of the nature of properties is crucial in interpretation of the results from testing. The most significant seem to be the mechanical properties (such as compressive strength) as they relate to hardening and carbonation, and the physical properties (porosity, permeability) as they relate to durability and transport of processes within the mortars. However, the interpretation of general research for a practical application often needs additional testing and examination. One of many examples could be the research work of Papayianni & Theocharidou (1993) who tested a number of new mortar mixes in order to relate their composition, strength, absorption, absorption rate and efflorescence. The research confirmed that the pore structure is the most significant factor when describing the efflorescence tendency as it describes the moisture transport (in this case capillarity) within mortar. On the other hand, the authors concluded that open porosity and natural absorptioll are not good criteria for the description of moisture movement and therefore for susceptibility to efflorescence. More tests are needed to confirm these conclusions in general.
M~RTA IN R HISTORIC ~ RIJIIDINGY: A RFVIFW
C~NSFRVATION, TFCHNICAI AN11 SCIEN I IFIC
The following paragraphs inform about the latest research into properties of mortars. A great deal of papers related to material research of historic and modern m nor tars can also be found in RILEM conference proceedings (Bartos et al. 2000) about 'Historic Mortars: Characteristics and Tests'.
5.3.1. Porosity, pore structure & transport process The amount of water in a lime mortar mix and the manner in which the water evaporates in time during setting controls the eventual porosity and the pore structure of mortars. The water content of the mix is also directly related to workability, which consequently has an influence on the quality of the co~npactionof mortars. Studies on cement mortars (Kroon and Crok 1961) suggested that the extent to which the mortar was compacted affected pores of 5mm in diameter and larger. During setting, as the moisture evaporates, a pore structure of the mortar is formed. The pore structure has a direct influence on perlneability and other characteristics related to transport processes in the mortar. Banfill and Forster (2000) suggested a hypothetical relation between degree of hydraulicity of rnortars and their gas and vapour permeability (breathability). The more hydraulic a Inortar is (e.g. Portland Cement, an eminently hydraulic mortar), the less permeable it is. Size of pores defines and limits the transport process in the porous materials as shown by Meng (1996) on studies of sandstone. For a description of the relevant porosity a correct method or cornbination of methods have to be used. A range of different methods and the porosity relevant to the transport processes in sandstone is shown in Figure 5.7 and Figure 5.8 taken from literature (Meng 1996). The pore structure is usually described according to pore size distribution, where the pore volume is divided into fractions col~espondingto the equivalent cylindrical pore radius. It is most often measured by means of mercury intrusion porosimetry. This method allows a basic colnparison of the pore structure between porous materials. It can therefore be used to characterise the most relevant transport process in a given material, i.e. a high proportion of capillary pores suggests a potential danger of capillary rise and easy transport of water. However, the porosity itself obtained by mercury intrusion does not describe the interconnection of the pores, the perlneability. Moreover, only the pores which are accessible from outside are the most relevant to the weathering and the transport processes Meng (1996).
10-9 10-8 10-7 10-6 10-5 10-4 10-3 I O - ~ Pore radius in m Figure 5.7: Meosz/r.i17gi.crirges of dijj'ererif rrrethoclsfor. deterniiirafiorr ofpor.osir-)~crr1rlpor.e sfr.~ccture(Merrg 1996)
Pore radius in m Figure 5.8: Rorzges of r.ele,>criifporosih to trcri~sl~ort i7iecliniiisi7zs ( M e q 1996).
The porosity of historic mortar (from the church of Santa Marta fronl XV century) was nleasured by Biscontin et al. (1993) who carried out research on historic mortars in Venice. Biscontin et al. (1993) pointed out that all historic mortar samples analysed had similar values of pore size distribution in the range of 0.01 to 0.5mm which he related to formation during carbonation process. Another useful characteristic of porous materials is their total porosity. It is usually measured by water absorption, a method co~nlnonlyused in a building practice which covers a wide range of pores, see Figure 5.7 and Figure 5.8. Although this method may still not include exactly the whole range of pores, it ~neasures porosity relevant to the moisture transport.
-c cl :s2.3 +11:s3
13:cl:s12 -m- h~storicmortar
Tliis pore size clistr.ihlrtior~grc11111~lcis cr~ecrfccl fi.0~11por.osity menslri~enierits p~rl~lislreel irl 1iter.rrtrcr.e to e.vplnin hy e.1-crrrzple tile cl(fe~~erlces iri pore str.lrc.tl~r.c.of'lristor.ic c111clriioc1er.11 r1zor.tcir.s. Fr~)rr~ tlic gr.crp11it is ob~~iolts thcit the c'enie~~t 11ior.tur coritriirls N Icrr~er.rllrrlrber of sr7znll ~~o~~esflrcrrr tlie plr1.e liirze rriar.tar; arzcl the ccJnierltgcr~rgedrlroi.tnr. lies bi hehveerr then,. Tlre liistoric. r71ortni. hercl higher tote11por.osi@ crricl fe11.e~ pores ir,it11sri~nllr~cicli~rs. It sholrld be rlotecl rl~crrthe gr.cz11h is or11yrlei.iiied fi.0117 ci r ~ ~ ~ r ~s~ril(?~e d o r r ~ /~re~elltecl ir7 1iter.crtrrr.e.
Pore radius (micron)
Figure 5.9: Conil~misorzof clrr7ilrlcrfivep o x size clistr.iblrtiolrs of histor.ic niortrrr. (Bi~corztir~ et cil. 1993) nrlcl rlzocler.rl nior.ta1.s (Perorli et 01. 1981) bnsecl on i.es~rltsplrblisllecl iri literntlcre. ( p = tote11por.osit),, c-ceriler~t,S-sciricl,I-lime, nllrlzber. = pr.ol>or.tiorl).
5.3.2. Carborzation The carbonation process has been well documented. The main interest is in the carbonation of concrete in connection with corrosion of steel reinforcement (e.g. Pall-ot 1990). Research work on carbonation of limebased mortars has been carried out mainly as a part of complex analysis of historic mortars. One of the few studies on new lime mortars is Van Balen's (1991 and 1994) research into modelling of lime mortar carbonation. Carbonation of non-hydraulic lime mortars is a physical-chemical process when calcium hydroxide (&(OH),) reacts with carbon dioxide (CO,) fro111 the air in presence of moisture to form calcium carbonate CaC03. This reaction is often written as a chemical equation (l): Ca(OH),
+ CO, + CaCO, + H,O
More precisely, the CO, diffuses from the environment into pores of mortar. According to Fick's law, the carbon dioxide travels in the pores from regions with high concentration to regions with low concentration (Papadakis et (11. 1992). The diffusion of carbon dioxide into mortars is largely influenced by the moisture condition of the material. If the mortar is saturated, the pores are filled with moisture and the carbonation process is retarded. The diffusion of CO, in water is 10'-10' times slower than in the air, when the pores are empty (Van Balen & Van Gemert 1994). However, a small amount of moisture has to be present in pores should the reaction happen. Carbonation is in fact a two-stage reaction. Firstly, the carbon dioxide is dissolved in water present in pores (2a): CO, +H,O U
Secondly, the lime reacts with the carbonic acid to form calcium carbonate: Ca(OH),
+ H,C03 + CaCO, + 2H,O
The degree of pore saturation is therefore the main factor which contsols the whole process. According to Van Balen's and Van Gemert's studies on 'Modelling lime mortar carbonation' (1994) the optimal water content for carbonation is maximum adsorption of water on surface of pores before capillary condensation. Less exact but more practical is an expression of these optimal conditions as a relative humidity of the ambient environment. Papadakis et al. (1992) in his paper about mathematical modelling of carbonation of concrete suggested that the maximum carbonation rate occurs at relative humidity of around 50%. Other literature recommends values between 5060% (Hosek and Muk 1989) or 50-70% (Parrot 1991192). These values can be compared to an average relative humidity in UK, outdoor environment, which is about 80 - 85% (Meteorological Office 1970). The carbonation of lime mortars causes a change in their structure as well as chemistry. The formation of calcium carbonate leads to an increase in the mass and volume. This results in the gain of mass of mortar and the reduction of total porosity. Moorehead (1986) in his paper about carbonation of hydrated lime explains that the mass gain is about 35% of hydrated lime used, which may convert to an 11.8% increase of volume. The increase of volume is internal, inside the pore structure of the mortar, without any significant effect on the overall alteration. These changes of pore structure and the pore size distribution were reported in studies on concrete (Hilsdorf ef 01. 1995, Pihlajavaara 1968). In concrete, carbonatio~lcauses an increase of
MORTARS IN HIS~ORIC BUILDINGS: A REVIEW OF THE CONSERVATION, TECHNICAL AND SCIEN rlblC L ITERATURk
capillary porosity in the range of 0.00751nm to 0.100pm (Hilsdorf et al. 1995). For a hydrated lime mortar a graph of pore size distribution which showed a change in pore diameters was explained in the literature (Moorehead 1986). It described a reduction of pore sizes around lmm and larger, as well as an increase of pores of a smaller size within a range of 0.05pm to 0.5\im, see Figure 5.10 . However, the range of the pore sizes affected by carbonation depended on the initial porosity and the pore size distribution existing prior to carbonation. The external factors are: Relative humidity (moisture conditions), drying and wetting cycles, and wind speed. Temperature. Solubility of carbon dioxide decreases with increasing temperature. However, reactivity is better with higher temperature, The optimal temperature is therefore about 20째C (Van Balen & Van Gernert 1994).
. Content of carbon dioxide in the ambient environrncnt.
Content of CO2 in the air is nornlally around 0.03% (Hosek and Muk 1989). The internal factors are:
(i) Diffusion of carbon dioxide becomes more difficult with depth and therefore carbonation in deeper parts of mortar is slower; in the case of combination with other conditions which are unfavourable for carbonation, it can be retarded or stopped altogether. (ii) Reduction of porosity and permeability should enhance durability of mortars as was pointed out in literature (Hilsdorf et al. 1995). However, this may in general be a positive effect for concrete, but mortars with high perlneability are sometimes required in conservation works. The increase of mass due to carbonation can be used as an indirect measurement of the carbonation progress. Parrot (1991-92), following the work of others (Kamimura e f al. 1965), examined an increase of mass of concrete due to carbonation. In his experimental work he concluded that the mass gains are directly related to gains of carbon dioxide as presented in Figure 5.11 . From this relationship it was suggested that the kinetics of carbonation could be assessed indirectly by monitoring the increase of mass in time.
Potosity and pe~meab~llty of the illaterial This goveins t ~ a n s p o of ~ t moisture, and diffusion of caibon t y pelmeabil~tydepend on the composition dioxide ( p o ~ o s ~ and of the moltar m ~ x )
'Secondary' C a r b o ~ ~ a t i oand n Other Reactio17s
Carbonation reaction results in the formation of calcium carbonate, which is chemically relatively Com~osition,aualitv of lime and quality of slaking, etc stable. This has a positive effect overall on the Table 5 3 Scm~nznryof the factors lrfluenclr7g the durability of mortars. During the carbonation process, cal bol?atlonp1ocess dnvded 111toexterilal and wtel rzal o ~ ~ e s the pH value of 12.5 of uncarbonated calcium A reduction of pore sizes induced by carbonation hydroxide is reduced to a pH value of around 8.4. results in reduction of permeability and diffusivity of mortars (Hilsdorf e f al. 1995). This consequently leads to the following conditions:
Figure 5.10: Change ilz po7.e size clistribzrtiorl of hyclrated lime co~~il~cict accordi~lgto Moorel~ecrcl'sstcrclies (1986).
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE CONSERVATION, TFCHNICAL AND SCIENTIFIC LITERATURE
TGA carbonate loss:glcm3 paste
Figure 5.11: Mass gains due to carbonation against calcium carbonate loss from thermogravimetric analysis, according to Parrot (1991-92).
However, calcium carbonate is not an entirely insoluble material and further chemical reactions, which affect the durability of lime mortars, can occur. This can be a process of dissolution of Ca, which is described by a chemical equation (3):
Internally. It can precipitate inside the mortar pores, cavities, cracks, between layers of two mortars or in the interface of mortar and masonry. The existence of this process should be considered when assessing long term durability of the mortars. In some cases the carbonates precipitate in cracks, commonly called re-healing, which can be seen even as a positive and durability enhancing feature. To some extent the dissolution of the calcium carbonate occurs in all lime-based mortars. This is sometimes called two-stage carbonation, where the second stage is the dissolution of calcium carbonate and its recrystallisation, which brings about an increase in the size of crystals and binds them more tightly together. It gives greater tightness and strength to the mortars (Chandra 1998).
In this process calcium carbonate reacts with carbonic acid to form calcium bicarbonate. A higher solubility of the calcium bicarbonate leads to a gradual dissolution of Ca, which often means enlargement of pores and a gradual decrease of the strength and durability of the mortar (Cowie and Glasser 1991-92). In building practice, this process is called lime leaching. It requires the presence of water and therefore, once a mortar is carbonated, water should not be allowed to flow through. Lime leaching can be Internal lime leaching has been observed on many denominated according to the place where the historic mortars, e.g. historic harling from Gylen precipitation of calcium carbonate occurs, which Castle, see Figure 5.12. mainly depends on the water transport mechanisms.
Figure 5.12: Example of internal lime leaching on the inkr3cace between lime mortar harling and stone masonry from Gylen Castle. From left: external side of harling (scale in cm), internal side of hurling- internal lime leaching (scale in cm), detail of internal lime leaching (scale: 7.3mm across the picture).
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF THE GONSERVATION, TECHNICAL AND SCIENTIFIC LITERATURE
Externally. The dissolved carbonate is transported by water out from the mortar, where it precipitates on the external masonry or render surface. It can be caused by unidirectional flow of water through the mortar. From a conservation point of view, external lime leaching is highly undesirable. It not only weakens the mortar but also leaves hard lime staining on the masonry face, see Figure 5.13.
conditions - air free of atmospheric pollution - cannot be fulfilled today in urban areas. Zappia et al. (1994) described the reaction between airborne sulphur compounds and mortars. In general, it leads to the formation of calcium sulphate, which crystallises as gypsum and subsequently forms a black crust commonly observed on limestone monuments. The pattern of such soiling is determined by the construction and detailing of the masonry. Calcium sulphate can be washed away by rainwater but it precipitates in sheltered areas. In the case of cement mortars and hydraulic mortars, the gypsum and the hydraulic constituents can interact to form other salts such as ettringite and thaumasite (Zappia et al. 1994). The formation of gypsum, ettringite and thaumasite is accompanied by a series of physico-chemical processes such as decomposition of binder, volume expansion and cracking, which brings about a loss of cohesion in the mortars (Sabbioni et al. 2001).
A parallel phenomenon to lime leaching is the transport of uncarbonated lime in the mortar. For example, very rapid drying can draw the lime particles (calcium hydroxide) to the surface and make the surface whiter (Gibbons TAN l). Too high water content in the fresh mortar mix can have the same effect (Gibbons TAN 1). An example of such whitening of the surface is presented in Figure 5.13 Dissolved calcium carbonate and uncarbonated calcium hydroxide can be transported by water and both are available for further reactions. The recrystallisation process of carbonate particles within the mortar is a common process. Perander and Raman (1985) pointed out that the conditions required for this type of repeated carbonation consist of open pore structure (mortar's surface), prolonged period of time and moist air. The air however, has to be free of airborne pollutants, namely free of sulphur dioxide. Sulphur dioxide is the most aggressive towards mortars containing lime (Sabbioni et al. 2001). However, these
5.3.3. Strength Strength development and testing of cements and other hydraulic compounds have been explained elsewhere (Neville 1963, Hewlett 1998). According to Hosek and Muk (1989) the strength of non-hydraulic lime mortars is gained from three processes.
Figure 5.13: Doune Castle; external lime leaching on the left Izand side and new lime repointing, slightly pink colour is becoming whiter by tlze uncarbonated lime transported on the surface on the right hand side. m
MORTARS IN HISTORIC BUILDINGS: A RE\'IE\V
Drying of linle mortars. *
A long-ten11 dissolutioil of silica in tlie alkaline environment of calciu~llhydroxide and consequent fnrnlation of solid phases of calcium silicate. Carbonation of lime mortars.
In ge~leral, carbonation is co~lsidered to have the biggest influence on strength development. However. this requires deeper studies, as the main influence on strength seems to differ depending on tlie ageing stages and the curing conditions. The initial stage of hardening seems to be more influenced by the drying out process than carbonation (Vilek and Bartos 2001). Schafer & Hilsdorf (1993) tried to relate type of binder, binderJaggregate proportion and porosity in order to indirectly estimate compressive strength and elastic ~nodulusof historic mortars. The authors introduced a formula to calculate the strength purely from results of chemical and visual analysis.
CONSERVATION. TECHNICAL AND SCIEN~IFIC LI'TERAI'URE
research results for traditional lime and stone masonry. The literature review by Goodwin & West ( I 980) show that the quality of the bond is supposed to be influenced ~nainlyby mortar (composition, consistency and water retentivity), bricks (absorption and texture) and workmanship. A good quality bo~ldbinds units well together providilig stl-ucturally sound and watertight masonry. The quality of the bond should not be measured solely by the adhesive strength. It was indicated that conditiolls which provide the high strength bond may not be thc same as those which provide resistance to water penetration of the bond (Goodwin & West 1980). Durability and quality of mortars is affected by the suction of the bricks. High suctio~lcan lead to a shortage of water when hydration takes place and affect the bond. On the other hand, Harrison (1986) in his experimental work deino~lstrated that high suction bricks improved the durability of cement based mortars colnpared with specimens cast within 'zero' suction bricks.
Suter and Song (1995) pointed out that when describing strength of llistoric mortars it is important to perform a relevant test rather t11a11 rely on the wide range of data presented in publications. A great variety of mortars with various proportions of binder and aggregate have been reported in literature (Suter and Song 1995). However, the size and number of samples available fro111 historic masonry restricts the mechanical testing. Often non-destructive, 'in-situ' testing is necessary for testing mortars within historic masonry.
The most important single factor affecting the bond was concluded to be the absorption rate of masonry units (Goodwin & West 1980). Groot (1993) described the effects of water on ~nortar/brickbond by ~neasuring water content changes and flow rates immediately after bricklaying using a neutron transmission technique. He concluded that no relation could be established between the water content at the interface and the bond strength. The flow rate was more critical. For the tested specimens, the most significant differences in flow rates occurred during the first 100-200 seconds after Testing standard specimerls of a new mortar may not bricklaying. Transport of fine particles of binder correspond to the characteristics of mortars from towards the interface was observed. Interestingly, within masonry. Henzel and Karl (1987) derno~lstrated neither the transport nor the bond was affected by prethat strength obtained from standard laboratory wetting. The type of brick influenced the flow rate specimens was lower than that obtained from a normal much more than aggregate grading. Groot (1995) later mortar joint. The inortar from within masonry was on suggested a model for water transport between subjected to various influential factors which affected Inortar and brick immediately after bricklaying. The its properties. One of the differences is the contrast brick mortar model was described by means of a between inortar prepared in a steel mould and mortar in hydraulic diameter model (brick) and a particle masonry units with certain moisture conditions and capillary pressure theory (mortar). Such a theory can be used for tlie design of a 'compatible' mortar-brick suction. combination.
5.3.4. Bond between Inortar and rnnsonv The bond between nort tar and masonry is important for both stress-strain transmission and durability. If the bond is poor, water can peaetrate much more easily inside masonry and cause degradation. This applies to bedding mortar but also to plasters and renders. The bond between mortar and Inasonry unit has been studied for a nu~nberof years. The investigations are mainly into Portland cement based mortars and bricks, and there seem to be few direct applications of these
It is possible that lime can penetrate into bricks and carbonate in their pores, therefore creating a physical adhesion between the mortar and the brick (Armelao er al. 2000). Similar observation was presented earlier by Baronio and Binda (1987) who studied a mortar-brick interface on samples of historic and modem mortars. The authors noticed that the extent and conditions of a lime-based mortar/brick contact was better than the one of a cement-based inortar as the lime penetrates to the open porosity of the bricks. Cement based mortars presented long narrow voids on the contact with bricks.
MOI~TAIIS IN HISTORIC BUILDINGS: A REVIEW
CONSERV/\TION, TECHNIC~L AND SCIENIIFIC I ITERAI U K L
5.4. Testing of mortars
Ob,jective of the treatillerit (e.g. consolidation. repainting)
Any new mortar should be tested prior to its application for various reasons. 111 conservation, testing can be seen as part of a cornplex logical procedure to ensure correct selection and application of the mortar (see Table, Charola et 01. 1997). The range of the tests varies depending on the mortar's functions and applications (described by Sass and Snethlage 1997). For example, performance characteristics of mortars should be tested to ensure their compatibility with historic materials.
Requisites of tlie treatment (specifications e.g. matching the original Inortar in colour and texture. new mortar should be less strong than the origirial mortar and masoiiry)
Most tests currently available for evaluation of properties of Inortars are standardised. However, these tests are not always applicable for conservation purposes. In the case of lime mortars especially, the testing requires a better understanding of their perforlnance and their correct application. A typical example is the standardised testing of con~pressive strength of non-hydraulic lime mortars, which requires completely different specimen preparation and curing than cement-based lnortars for which the standards are written. As a consequence of the lack of appropriate tests the standard tests have to be modified and new tests designed to be applicable in conservation. This problem is well known and discussed (Sickels-Taves 1999, ASTM congress on 'The Use of and Need for Preservation Standards in Architectural Conservation'). It is generally recognised that one of the main values of standard testing is the ability to compare the results on an international level. However, the con~parison of the results is not always straightforward, as there are a number of national standards with different testing methods (Henriques and Charola 1996). In conservation, the aim of standard testing is to avoid the introduction of potentially harlnful treatment (Teutonic0 et al. 1997, Dahlem workshop). New standard methods for testing compatibility of mortars are still under development. However, there have been a nurnber of suggestions and first attempts which are currently under discussion.
Selectin11of weathering coilditions (e.g. natural. standardised, accelerated)
Selection of tlie relevant pliysico-clie~l~ical parameters needed to evaluate tlie effects of the treatment and of the experi~~lc~ital methods to lileasure above parameters. Selection of suitable samples (e.g. type, size) Selection of applicatioil method and its implementation (e.g. correct work~nansliip,standardised p~.eparationof speci~llenscubes. prisms)
Comparison and critical evaluatio~iof the results obtained on treated and uiitreated samples, and before and after ageing (compatibility. comparison of parailleters of historic and new mortars, carboiiatio~lof non-hydraulic limes is a slow process tlie age factor is very important)
Trthle 5.4: The steps ($0 testirlg protocol to fo1lo11, srrggesterl by C h a r o l a e t ril. (1997) i+,itl?c<~cir~rl~les gii)er~,for. ~.epoirltirzgofnrttsor~l:\l.
The new standard testing of lime lnortars should consider two main aspects (Charola & Henriques 1999): How to prepare, treat and test the specimens What kind of tests should be carried out to characterise the lnortars One of the main problems of laboratory testing is that it does not conform to the behaviour of mortar in masonry. The specimens should be prepared according to the appropriate practice. Tests, such as compressive strength, should incolporate the slow nature of the hardening process. The size of the specimen can influence the results. For exa~nple,the smaller a specimen of non-hydraulic lime mortar is, the faster it is completely carbonated (Baronio et cil. 2000). The other aspect considers the appropriate tests to be carried out in order to characterise mortars. A selection of tests is available (e.g. Peroni et a l . 1981, RossiDoria 1986), however the aim should be to define a ~ n i n i ~ n unurnber ~n of tests sufficient to characterise the mortar (Charola & Hensiques 1999). For compatibility compliance, a range of optirnal performance within which the results should fall must be resolved (Charola & Henriques 1999).
MORTARS IN HISTORIC BUILDINGS. A REVIEMT OF THE C~NSER\~J\TION, TECHKICAL AND SCIENTIFIC LITFR/\TURZ
Time of setting Cornprcsaive resistance Modulus of elasticity Adherence strength Thennal and lig~groscopicexpansion Release of soluble salts Capillary water abso~l~tion Water vapour periiieability
24-h i~i-rmersionwater absorption (for brick masonry) Resistance to chlorides and sulvliates
Tcible 5.5: Pi.ol~osedtests for stcrr~rlcii.rltestiiig oj'linle basecl n~oi.tars(ol~enj'oi.cliscrrssiorz) by Chcrr.olci & Her~riqrres (1999).
A definition of the exact number of tests and the range of optimal results expected from the mortars is, however, difficult since the conservation tasks are unique, the historic buildings are unique and they require individual solutions (Busman 1997). The selection of tests should be based on a holistic acquaintance with all relevant information incorporating the uniqueness of historic structure. At the moment it can be confirmed that the testing itself can be standardised as there has been a number of tests completed on mortars. This should improve the descriptions of the properties related to the function of the mortars in real structures. However, what tests should be carried out, and the limits for the co~npatibilityrequire~nentswhich would provide the selection of the right repair mortar, still need further studies.
5.4.1. Exarnples of experimerztal studies arzd testirzg of mortars Research projects dealing with the experimental study and testing of new mortars often developed from a practical design of a new repair inortar (e.g. The Smeaton Project, Teutonico et al. 1994, Perander and Rzman 1985, Fontaine 1999). These projects set up certain standards and often serve as examples for similar projects in the future. Some of them are reviewed in the following paragraphs. (i)
phenolphthalein pH solution with the nlaxilllu~n depth 17mm (fully carbonated mortar). The coinpressive strength was tested on 1001ni11cubes and, prior to testing, the samples biere i~n~nersed in water for 24 hours. Other tests, such as moisture content, stiffening ratio, water vapour perlneability and sodium sulphate crystallisation were carried out. This briefly suininarises phase 1 of the project, which led to the following conclusions: Addition of brick dust alters the properties of lime mortars. The low-fired brick dust seems to have the most positive effect on durability and strength of the mortars. Addition of a small quantity of cement has a negative effect on the strength and durability of the mortars. (Note that in literature similar conclusions were reached (Holmstrom (1995), however, opposite ones also exist e.g. Von KOBOW(1998).) Further research investigated pozzolanic additives. It identified the positive influence of brick dust on strength and durability of mortars. The effect of the addition of brick dust later on became the objective of a consequent research. The results indicated that brick dust with a lower size particle range (range <75 microns) could act as reactive pozzolanas. Also, a lowfired brick dust (temperature < 900째C) seemed to have the most positive effect on the strength and durability of lime: sand: brick dust mix (Teutonico et al. 2000). Based on the Smeaton project a new experimental research was initiated into hydraulic limes aild their blend with different proportions of non-hydraulic lime (Teutonico et crl. 2000). The preliminary results suggested that water vapour permeability appears to be lower with hydraulicity. The addition of a significant proportion of lime putty into hydraulic 1irne:sand mortar mix significantly reduces its colnpressive strength and durability perforinance from a salt crystallisation test.
The Smeaton Project evaluated the inortar specimens according to compressive strength, which was assumed English Heritage, ICCROM and Bourne~nouth to be the appropriate measure of their performance and University joint research project (Teutonico et al. related to their durability. The mortar mixes used were 1994) started as an identification of a suitable not designed to be compatible with any particular mortar for repair of Hadrian's Wall. Three types of properties of the original mortar or masonry. Instead, mortars were examined (Lime: Sand: Brick dust; general specificatio~lswere used. A significant number Lime: Sand: Cement; Lime: Sand: Brick dust: of various mortar mixes was tested and similar tests Cement). Pure lime: sand mortar was not were used for all mortar mixes. As such it offered a examined. The Inortars were prepared to the same good deal of comparison between different mortars. workability by an English Heritage craftsman and The main contribution of these projects may be seen in were cast into wooden moulds. The specimens the formulation of testing procedures and obtaining were cured at 2.5" and 90% RH for 120 days. background information about properties of different Depth of carbonation was deterrnined by inortar mixes.
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF TT-IE CONSERV~ITION, TECI-IKICAL A N D SCIENTIF~C LITERATLIRE
(ii) Perander and R h a n (1985) published a research report about mortars in Finland which, apart fro111 general information and analysis of historic mortars, comprised also a design of a new repair mortar. The authors described the variability of historic lime inortars including different burning, slaking and mixing. However, they concluded that the differences between the lime slaking had no significant influence on the properties of lime mortars examined in the laboratory. Moreover, they foulld the non-hydraulic lime-based mortars unsuitable for exterior renders in the Finnish climate. Their recommendation for repair mortar was based on composition of 60% of lime and the remaining 40% of some hydraulic additives (cement, fly ash, trass etc.). The recoillnlended ratio of binderaggregate was 1:4 - 1:5. In their research on develop~nentof new repair mortar the authors focused on the influence of hydraulic and air-entraining additives. A number of standard tests was cassied out to compare different inortar mixes (including consistency and stiffening, tensile and compressive strength, water absorption and porosity, frost resistallce etc.). However, the development of a repair mortar did not comprise any requirements of compatibility with historic mortars and the evaluation parameters were unclear. Determination of what the desired universal repair mortar was supposed to be was lacking. Although this research cannot be considered as a guide for design and direct selection of a repair mortar, it offered fundamental results for comparison between lime inortars with different hydraulic additives and described various methods of testing. (iii) Fontaiile ef 01. (1999) presented an overview of testing repair mortars. The study was based on experimental work with repair mortars and their practical application in the Canadian environment (Suter et al. 1995). The authors highlighted problems with the testing of repair mortars, as there were few standard tests directly applicable to them and virtually no standard test that would assess their durability. Modifications to incorporate the conservation view of some current standards designed for lnodeim buildings were suggested and discussed. The authors pointed out that every testing should be supplemented with specification criteria which should be fulfilled. Special focus was given to the frost resistance of Inortars and their nlechallical properties. Certain characteristics such as, for example, 'breathing' of rnortars were considered important but no tests had been developed to describe the relevant properties. Fro111 practical experience of testing repair rnortars and in-situ assessment of their perforinance certain performance criteria were recolnmended to ensure colnpatibility (see Table 5.6). The results offered
certain practical implications for mixing and co~llposition of mortars. Pure and hydraulic lime nlortars did not meet the performance (Table 5.6) criteria defined, mainly due to their poor frost resistance. Only the mortars gauged with cement were able to comply with these criteria. This was found to be in accordance with the findings from in-situ assessments, that lime mortars typically disintegrated within 5 to 10 years after their application. Performance characteristics
Limits Explanatory remarks
Compressive strength of mortar
1 to 8 MPa
Compromise between too strong and dense nort tar and too weak. which cracks and allows water ingress. Bedding mortar should be a ~llinimumof 2MPa.
Split tensile/ colllpressive strel~gtliof mortar
Low tensile strength results in cracking of mortars. This could bc considered as a material quality measure for brittle materials, which have a ratio between compressive and tensile strength of around 10. The tensile strength rarely exceeds the bond strength for celllent and lime mortars therefore there is no upper linlit defined.
Describes defornlabilitp of mortars under stress. Mortars are valued for ability to adjust to a minor movement. Too stiff mortar can cause cracking to the adjacent material. Hornever, this depends also on the elastic (Young's) l~loduli of all materials involved.
Flexural bond of masonry
Ideally the interface (the bond) of mortar and stone should be as strong as the mortar.
Expallsiol~ (freeze/thaw test) of lllasollry
Unidirectional freeze/thaw test where the damage is quantified by the change in the width of the Illortar joint. Expansion between 0.04 to 0 . 4 4 is considered
YoLtng'Sll'odL1lUS of rnortar
Tcrhle 5.6: Per:for.rllcrrzce cl-iter.icrfor. ileLt7poirltir7g n7or.tcrrs rrccor.ilirlg to For~trrir~e et crl. (1999) n~itllrerlicrl-ks to the tests' trl~l~lictrl~ility crrltl tlzeir. lirrlits.
Fontaine et 01. (1999) described testing and selection criteria for repair inortars with respect to the Canadian environment and therefore an emphasis was on durability (freeze/thaw). It recognised the need for compatibility and conservatio~~ related criteria for
MORTARS IN HISTORIC BUILDINGS: A RE\IIEU1 OF THE CONSERV~\.I.ION, TECHNICAL AND SCIENTIFIC LITERATURE
repair mortars in general. The values limiting the required performance were created fro111 realistic expectations of the ~naterial properties. practical experience with repair and research results. All considerations were put together, resulting in a limitation of the prope~.ties.However, two aspects should be highlighted which were missing in the research discussed above. The appropriateness of the limits related to compatibility should have been verified by testing the compatibility of both ~llaterials together. The compatibility is about two materials - not just the mortar. Exact limits may be applicable just for certain conditiolls e.g. Canadian environment. Traditional masonry in Canada is different from, for example, that of Europe, but certain differences may exist even on a smaller scale. Such variability should be considered when a new standard test is proposed. The overview of these three projects demonstrated the current situation in the search for a better repair mortar. Current standard tests were found to be not relevant, as they did not reflect any conservation require~nents.The selection criteria for mortars could be based on certain performance tests, but the relevance of these tests to the compatibility or conservation requirements is yet to be confirmed. Typically, when a design of new mortar was described it began with compatibility 'introduction' but the results and conclusions were only about tlie tests themselves, not about the ultimate objective - the design and selection of the compatible repair mortar. 111general, cornparative testing of mortar specimens in a laborator~lalways leads to the selection of some mortar but there is no proof of how this relates to real conditions and compatibility. It should be remembered that the mortar selected from a certain limited number of specinlens is only the best mortar available from the limited number of specimens, not necessarily the most appropriate for the repair. On tlie other hand, the practical approach to the design and testing of repair mortars is very effective as it narrows the number of variables to the most realistic ones. It means that each material has its certain range of achievable properties and use. Non-hydraulic lime mortar cannot be expected to possess a high compressive strength or good freeze/thaw durability. Througli experimental testing and practical experience it is possible to clarify these limits and use each ll~aterialin its proper way. 5.4.2. Factors affectirlg the preparation of specinzens and testing nzorturs
The performance of modern non-hydraulic lime mortars made of lime putty is considered to be strongly
dependent on workmanship (Gibbons 1995 TAN 1). The workmanship colnprises not only the application of mortar but also particular constructional details, adequate workability, final surface finish, in-situ protection and curing. The workmanship should reflect the actual state of masonry and environmental conditions. Also, the moisture suction parameters of masonry units together with ageing conditions affect the bond between mortar and masonry.
It has been suggested by Schafer et al. (1993) that a correlation between porosity of an ancient and new lime mortar could be used as a method to esti~natethe compressive strength. The alilount of water added determines porosity of a hardened mortar. The water in non-hydraulic lime nort tars can evaporate or be absorbed by the adjacent masonry. Together with a degree of compaction they characterise a volu~neof voids in the mortar. Higher porosity means lower strengtli. The nlechanical properties of lime mortars are improved if the amount of water is reduced (To~saca 1988). The same applies for cement-based or hydraulic lime mortars, however, a certain amount of water is needed for the hydraulic reaction (Neville 1963). Lime putty usually contains enough water for mortar (bedding and/or pointing mortar) to be prepared without a further addition of water (TAN 1 1995). Aggregate From research into concrete it is known that the influence of aggregate on strength of mortar is due not only to the mechanical strength of aggregate but also, to a considerable degree, to its absorption and bond characteristics (Neville 1963). Papayianni et al. (1993 Paris) suggested that historic mortars in Greece follow the same principles of aggregate proportioning as those which are valid for concrete. However, the grading of aggregate of historic mortars does not comply with current standards (it contains a considerable amount of fine argillaceous components and a relatively high proportion of course grains (Schafer & Hilsdorf 1993)). The strength of a mortar depends on the strength of a weaker component in the mortar mix. In the case of lime based mortar, it is usually the lime matrix whic11 determines the overall strength. Moreover, the shape of the aggregate and its surface control the mechanical bond between binder and aggregate. Type of sand influences the mechanical properties of hardened lime mortars (Callebaut ct al. 2000). Aggregate grading also affects workability and consequently sluinkage of mortars. Sinchez (1997) summarised that aggregate, its maximuin size, grading and proportion of the finest particles affect shrinkage of mortars. Mixtures of fine and coarse aggregate are
MORTARS IN HISTORIC B U I L D I ~AGREVIEW S. OF THE CONS~I<VATION, TECIINILAL AND SCIENT~FIC LITERATURE
co~lsideredthe best, as such mixtures occupy space in the most efficient way (Torraca 1995).
The contact surface of rnoulds with the specimens, suction and entrance of air influences maiilly limebased mortars (Charola & Henriques 1999). Therefore, properties of lirne mortar made in a steel mould are different from those of Inortar cast between masonry (Lawrence & Samarasinghe, 2000). They depend mainly on the mould surface, the size of the specimen and how long the specimen was left in the mould. Mortar specimens for investigation of properties should be prepared in a realistic way. Lawrence & Samarasinghe (2000) suggested producing and curing mortar specimens between two masonry units.
Type of aggregate, its grading, type of lime (age of lime putty) and liinelaggregate proportions control the amount of water needed to provide good workability. The optimal waterlbinder proportions differ depending on construction and application techniques. Good compaction of liine mortar is vital for its performance. Good workable lime mortar possesses a greater degree of plasticity; it is often described as similar to a modelling clay.
The mixing and production methods of lime mortars can also have a very strong influence on their performance. Maturing of some lime putties reduces their particle size and improves their water retentivity (Hansen et al. 2000). The sand carrying capacity of lime mortar should improve with reduction of particle size (Gibbons 1995 TAN 1). Hand and different mechanical mixing can produced mortars of different quality. From practice it is known that the mortar plasticity can be improved by the method of mixing. Traditional techniques of mixing 'by hand' involved beating, chopping and ramming on a wooden board until the mix was sticky and workable (Gibbons 1995 TAN 1). Ready-mixed mortar should be re-mixed before use. In relation to the performance of mortars assessed by standard testing, Henriques & Charola (1996) assessed the effect of mixing and preparation on compressive strength of pozzolanic lime mortars. The two standard procedures prescribed by British Standard (BS 4551) and European specifications (EN 196-1) resulted in pozzolanic inortar specimens with different mechanical properties. The pure liine mortar specimens, however, did not show any significant differences in their mechanical properties for these two
different preparation and mixing standards. The mechanical properties of both non-hydraulic and pozzolanic mortars were also affected by different curi~lgconditions prescribed by British Standard (BS 455 1 ) and French specifications (CSTB). Wetter conditions (BS 4551) favoured hydration but slowed down carbonatio~l(Henriques & Charola (1996).
The curinglagei~igconditions for non-hydraulic lime mortars proinote a combination of drying out and carbonation at such a rate that minimises shrinkage. The ideal environment to achieve a maximum rate of carbonation, has a temperature around 20째C and relative humidity between 50-70% (Van Balen & Van Gemert 1994). The strength development of limebased mortars due to carbonation is inherently a very long-term process, depending on the curinglageing conditions. Curing described by British Standard (BS 455 1: Part 1: 1998) for mortar specimens is not appropriate for nonhydraulic lime mortars. It assumes the presence of a hydraulic binder, which requires a damp environment or immersion to allow hydration of the hydraulic components. Moist curing in a container can possibly be used, however, the container should not be airtight. According to literature (Parrot 1991-1992) and considering the nature of the hardening process of lime mortar, such humid conditions can retard carbonation and do not represent ambient conditions encountered in practice. The common 28 days' curing is not sufficie~itfor nonhydraulic lime mortars (Cliarola and Henriques 1999). A length of curing to provide a comparable strength testing can be difficult to predict. It depends on the curing conditions, moulding and size of the sample. Accelerated curing where the specimens were exposed to a higher CO, concentration was described (Knofel and Schubert 1993). This accelerated curing was developed to make testing of lime mortars available at 28 days. The effects of the specimen size and the length of curing on the strength testing of lime mortars have been observed in Inany research papers (e.g. Baronio ef al. 2000).
5.4.3. Fresh nzortars Mortars, while fresh, are tested in order to ensure a certain standard quality. The tests are described in detail in national standards (e.g. British Standard BS 4551: Part 1 Methods of testing mortars, screeds and plasters) EN 1015 Methods of tests for Mortar for Masonry 1999. Of these tests, the workability test is the most beneficial for practice. It combines needs for appropriate consistency of the material regarding its
MORTARS IN HISTOKIC BUILDINGS: A REVIEW
CONSERVATION, TECIINICAL AND SCIENTIFIC LITERATURE
application but also its properties after setting and hardening. Wo~.kabilitjiTestirlg Recent research into properties of Inortars applied various methods to measure workability, as the standardised methods are not always suitable for mortar mixes used in conservation. The Smeaton project (Teutonico et (11. 1994) employed an English Heritage lnaster craftsinan to judge the suitable consistency to produce comparable specimens of mortar. In the experinlental work carried out by Papayianni et al. (1993) a flow table test (British Standard BS 4551) was used to achieve comparable consistency and workability between various mortar mixes. The water contents of lnortars were adjusted to achieve the same flow value (170 f lmm). Sickels (1987) in her PhD research used a British Standard test, Deterr~~ination o f Consistency 12~1 DI-upping Ball, to provide the same consistency between mortars. Schafer et al. (1993) did not measure the workability directly at all, but instead applied a theory of water demand for mortar. To achieve the same consistency, the water demand was calculated from water/binder ratio considering that different types of binder have different water requirements. The calculation was based on sizes of the binder particles. The smaller particles have higher surface area and therefore require tnore water in order to achieve the same consistency. However, the consistency and water demand based on particle sizes Inay not be fully relevant to the workability, especially not between binders of a different nature. Hamen e f al. (2000) in their research into ageing of lime putty demonstrated that the older lime with smaller particles and lower water content showed Inore plasticity and water retentively than the younger one (with larger particles). To achieve the same consistency, more water was needed for the lime with smaller particles. For the workability of lime, however, mortar characteristics such as plasticity and water retentivity were more important. British Standard BS 4551: Part 1 describes two tests which are used to assess the workability of nort tars Deterrninrrtion of Coizsistency by Dropping Ball and Detel-n7ir7ation of Flow (flow table). It should be secognised that these tests are designed for 'modern' mortars and ~noderil construction methods and therefore they are not fully applicable for assessment of lime based mortars used in conservation. Vrilek (2000) in his PhD thesis concluded that the co~lsistency measurement by dropping ball is not applicable for lime-mortars made of lime putty. However, he recornrneaded the flow table combined with determination of moisture content for a laboratory ~neasurement of workabil~tp. On the other hand,
Callebaut (2000, PhD thesis) pointed out that for practical use the flow table needs more research as the ineasured values vary depending on the mortar mix. Callebaut et (11. (2000) also considered the staildardised flow table test to be unsuitable for determination of consistency of different lime mortars. To a degree, for lime-based mortars the suitability and unsuitability of the flow table was explained by Hansen et al. (2000) in their research into ageing of litne putty. The authors suggested that for some lime mortars the flow test is less se~lsitivethan others to the water content of fresh mortars. Older lime putty with smaller particles (larger surface area) was less sensitive for variation of water content than younger lime putty. The flow table may not be precise enough to compare workability of lnortars with different binders or even with the same kind of binder but with different properties. An alternative to the flow table in the measurelnent of workability of conservation mortars could be the standard plasticity test (ASTM C 110) using the Emley plasticimeter. It is an American test which is not comtnonly used in Europe. Thornson (2000) used the Emley test in her comparative study of dolomitic and high-calcium lime mortars. She pointed out that this test incorporates two important workability characteristics (water retention and spreadability of mortars), hence the test relates to the workability of mortars. The subjective judgement of workability by a skilled craftsman should not be underestimated. It is an important factor which influences the quality of mortar; in fact, in practice the craftsman alone controls the amount of added water. The S~neatonProject (Teutonico et al. 1994) confirmed the precision of such judgement (English Heritage Inaster craftsman) by measuring moisture contents of the specimens. The moisture content ranged from 15 to 19%, which was considered to be relatively consistent.
5.4.4. Hardened inortars Properties of hardened mortars, as well as fresh mortars, should ideally be determined by means of standard testing methods. However, these standard testing methods often need to be modified to suit peculiarities of conservation practice. The following paragraphs deal with both standard and modified tests of hardened mortars with the objective of describing these tests within the context of their use. There are therefore described tests which were used recently in research and experimental projects, and also in practical designs of colnposition of new inortar and/or co~npatibilitytesting. The selection of the tests and testing procedures reviewed depended on available literature - it is not a compete list of testing methods applicable for mortars.
The shrinkage of mortar is its volulne reduction caused by changes of temperature due to a hydration process or to a loss of water through evaporation. Contraction caused by shrinkage generates internal stresses and, when restricted, it can result in cracks and a failure of mortar. Cracks call develop at any time before. during and after hardening when a mortar is not able to deform (SBnchez et rrl. 1997). Shrinkage is a complex phenomenon depending on Inally factors incolporating material properties, drying and hardening conditions. Faster shrinkage (for example mortar cured in fast drying conditions) produces a greater danger of cracks (Sgnchez et crl. 1997). SBnchez et al. (1997) tested shrinkage of lime based mortars on specimens according to standards for cement based mortars. The authors considered only shrinkage caused by evaporation (hydraulic shrinkage). Shrinkage due to carbonation was considered negligible because of its slow course. The authors compared shrinkage of lime mortars made with two sands, standard sand and sand found in historic mortars, during the first 28 days (starting at the day l). The main influential factors 011 the shrinkage of the mortars were considered to be the maximum size of aggregate and its compactness, waterllime ratio, content of fines, and strain module of aggregate. Testing confirmed the influence of some of these factors. The shrinkage (volume reduction) took place mainly during the first day. However, no cracks developed as the mortar was still in a relatively plastic state. The shrinkage was measured in a range fro111 1.15 to 1.6%. Application of the methodology from cement mortars to measure the shsinkage of lime mortars was successful.
Strength is an important property of mortars. In a design of a new mortar it should be a key parameter for the assessment of compatibility between mortars. However, unlike in modern industry, in conservation it should not be used as a sole measure of quality. In fact, for the determination of compatibility of non-hydraulic lime mortars the compressive strength alone may not be needed at all. Nevertheless, in a research into mechanical and physical properties of lime mortars, compressive strength testing is a standard way of assessing their hardening, setting and strength, and is related to carbonation, porosity and other physical properties (Viilek 2001). Baronio et crl. (2000) described experimental research into testing of mortars prepared according to the properties of historic mortars. The study comprised analysis of historic mortar, production of new mortar
and its curing followed by experimental testing on nonhydraulic lime mortar specimens made of putty and hydrate. The aut11ol.s tested the development of colnpressive and flexural strength on specilllens of different dimensions and preparation, and cured under different conditions. Comparison of the specimens of different sizes showed that the smaller ones ( 2 0 x 2 0 1201n111) ~ accluired maximum strength faster than the larger specimens (40x40x160mm). On the other hand, the results obtained from the larger specimens were more consistent and less scattered. The authors suggested that the larger specimens (7Ox70mm) possessed lower strength than the smaller specitnens due to the size of aggregate. The proportion between dimensions of specinlens and the lnaxilnum size particles of aggregate was co~lsideredto affect the strength. Additionally, the open porosity of the mortars was measured, however, 110 coivelation between open porosity and compressive strength has been drawn. Valek & Bartos (2001) examined the effect of curing conditions on strength development of non-hydraulic lime mortar specimens. The strongest specilne~lswere obtained from dry indoor conditions, where they also acquired strength faster than the ones cured outdoors. The drying out process appeared to be more significant for strength development in the early stages (first six months) than the degree of carbonation. Less variable curing conditions resulted in less variable strength. The authors also concluded that the addition of water increased the porosity and decreased the strength of non-hydraulic lime mortars. However, there was a certain margin within which the effect of added water on porosity and strength was not clearly recognisable and only a largcr amount of water added resulted in the changes of porosity and strength. Binda et al. (2000) studied mortar of thick jointed Byzantine masonry. Masonry prisms were built for laboratory trials as a reproduction of a historic masonry based on a complex analysis of mortar composition and in-situ testing. The prisms were used to study mechanical behaviour (deforn~ation)of the mortar and bricks under compression and its development with ageing of the specimens. Deformation in the mortar joints improved with age but, as expected, it remained higher than the deformation of the bricks. Stiffening of the 'wall' increased with age although its strength was not much affected by ageing. The authors concluded that the thick joints of Byzantine lnasollry allowed large defor~nationas hardening of mortar occussed slowly. For example, therefore, a soil settlement at early stages did not cause any significant cracks of the masonry construction. The high deformability of mortar also allowed withstanding of tensile stress caused by compression of bricks but without diminishing the overall strength of the masonry. This research confirmed one of the hypotheses about a
MORTARS IN HISTORIC BUILDINGS: A REVIEW
degree of deformability of lime mortars, which are often implied to possess high defor~nabilityand the ability to eliminate or reduce the local stresses in the nlasonry joints (Schafer & Hilsdorf 1993). Karaveziroglou & Papayianni (1993) studied the stress capacity of lnasonry with thick rnortar joints. In order to carry out the testing, lnasonry prisms were built using modern bricks ~llallufactured to match the properties (density, ~nodulus of elasticity and colnpressive strength) of the historic ones. Four different mortar colnpositions were used. All of then1 contained lime, pozzolana, brick dust and sand, and two mixes were 'enhanced' with cement. Bedding joints were 20 and 40mm thick. The compressive strength of masonry prisms increased with the compressive strength of mortar. The masonry with thicker joints had lower compressive strength than that with the 201111~1 joints. The conlpressive strength obtained was higher than usually assulned and the authors pointed out that the compressive strength of old masonry with thick joints might previously have been under estimated.
Budelrnann (1993) concluded that in order to achieve a high adhesion bond between lnortar and lnasonry a mortar mix based on hydraulic binder is needed. The author carried out tests on masonry units joined with mortars. Such lnasonry couples were mechanically tested in tension. Apart from the hydraulic binder, the adhesive strength was determined by some properties of the stone such as open porosity, pore size distribution and capillarity suction (Budelmann 1993). Marie-Victoire & Bromblet (2000) tested adhesion of modem and traditional renders by a pull out test. The outcome consisted of two results: the maximum load and the location of the failure. The test method therefore conveniently combined two main parameters. Maximurn load described a quality of the bond and in general a higher load was desirable. The other parameter, a location of failure, was a 'compatibility' limitation which determined whether or not the particular adhesion of the mortar could potentially cause any damage to the lnasonry when pulled away. The results confirmed that for traditional lime-based Inortars (hydraulic and putty mortar) the failure o c c ~ ~ r r ewithin d the thickness of render. For the rnodera ready-mixed renders the location of failure varied depending on the substrate lnasonry and probably on the quality of workmanship during application. T11e modern ready mixed renders performed quite well in terms of adhesion, however, the wrong type of failure occurred occasionally. The authors stated clearly that such material would be unacceptable for conservation of historic buildings.
CONSERVATION, TECHNICAL A h D SCIENTIFIC LITERATURE
Other simple adhesion tests can be carried out for a basic evaluatio~~. Perander and R?tman (1985) used a sinlple test for testing renders on bricks. Rendered brick was stroked from the back with a hammer and then the number of samples where rnortar remained attached to the brick was counted.
The most common way to determine the depth of carbonation of lime or cement based mortars is by a Phetlolphthalein pH indicator (a method recommended by the RILEM committee (RILEM draft recolnlnendation 1984)). The carbonation process reduces the pH value of 12.5 of Calcium hydroxide (Ca(OH)2) to pH values below 9 of Calcium Carbonate (CaCO,). When the sample is sprayed with the Phenolphthalein pH indicator it changes its colour from colourless to magenta in a region where the pH value is higher than 9. An advantage of this method is that it offers a non-destructive and very efficient measurement. However, this method does not recognise a partially carbonated lnortar - only fully carbonated mortar can be determined (Ohgishi et al. 1993). Therefore, the method cannot be used to evaluate quantitatively carbonation of lime mortars (Vrilek 2000). In addition, Parrot et al. (1989), who measured a gradient of neutralisation zone on 36-yearold concrete members, pointed out that a certain penetration zone should be considered when describing the carbonation depth. The detailed carbonation gradient was determined by therlnogravi~netric analysis (TGA) of samples taken by drilling at 51nm depth intervals (Parrot et al. 1989). Especially when a lnortar has aged in indoor conditions, the partially carbonated zone can be more than 20 or 30mm wide (Parrot et cil. 1989).
A good indication for laboratory observation of the carbonation progress of mortar specimens is a change of weight (Parrot 1991-92). Parrot (199 1-92) in his experilnental work on concrete, following findings of Kamirnura et al. (1965), concluded that the Inass gains of mortar are directly related to the gains of carbon dioxide. From this relationship it was suggested that the kinetics of carbonation could be assessed indirectly by monitoring an increase of weight in time. This method of measurement of carbonation was applied on lime mortar specimens by Vrilek (2000).
Measurement of porosity by water absol-ption is a method colnlnonly used in building practice. The method measures open porosity in total and it covers a wide range of pores. The porosity of mortars is deternlined by i~n~nersing the specimens in water under
MORTARS IN HISTOI~IC BUILDIKGS: A REVIEIV OF THE CONSERV,\TIOK, TECIINIC.\L I\ND SCIENTIFIC LITER/\IURE
were tested after 28 days of curing. Masonry prisllls were exposed to unidirectional freezing. Loss of bond was found to be the most colnmon failure as nearly all mortars showed a bond failure after 60 cycles. All mortars containing lime putty failed. It was noted that the stone properties affected the mortars. The rnortar which did not fail the test was the mortar with the higher proportion of cement (1:1:6). However, no comparison was made with pure lime mortars. Von Konow's (1998) work on the influence of aggregate grading on the performance of various mortar mixes used for repair pointed out a correlation between grain size of aggregate which affects the capillary suction and therefore the frost resistance. She concluded that a greater proportion of filler than normally recommended gives the mortar homogeneous and dense packing. This, together with a higher proportioll of a finer aggregate, improved the frost resistance. A new, interesting method for testing durability of mortars for abrasive damage was presented by Lawrence & Samarasinghe (2000). The authors tried to relate abrasive durability to surface hardness, not the strength or hardness of mortar in general. They suggested salt cycling test for laboratory testing and scratch test for in-situ testing. A salt (5% solution of sodium chloride) was used in an accelerated test to crystallise at the surface to cause mechanical degradation. The scratch test involved repeated scratching of a nort tar surface by a probe with a constant force. The correlation between these two tests suggested that both tests measure the same property.
5.4.6. 'In-situ' testing of properties of inortars 'In-situ' testing and determination of mortar properties is desirable and in conservation is often the only way of their determination due to sampling restriction. Ideally, the testing methods should be non-destructive. For determination of lnechanical properties of inortars and nlasonry a number of new methods are emerging but few of them are proven to be able to replace actual laboratory testing. 'In-situ', non-destructive testing measures other physical characteristics, which
conelate to the actual tested property. It is therefore obvious that the quality of the results often depends on the quality of the cosrelation. However, 'in-situ' testing offers one advantage over laboratory testing: it can determine the value of compressive strength, permeability, etc., under real conditions. To deternline mechanical properties of mortars or concretes core samples are usually taken and tested in the laboratory. The core samples required are too large (BS 1881 on testing concrete cores recommends min. lOOmln in diameter) to be drilled from historic masonry. A new research into minimising the core diameter is dependent on the size of aggregate. For example, for aggregate with a maximum size of particles of 30m1n in diameter, microcores with diameter of 28mm can be drilled (Indelicato 1993). The compressi\ie strength of mortars can also be determined fro111 correlation of the strength and energy needed to drill a small cavity. The method suggested by Gucci & Barsotti (1995) seems to be particularly applicable to mortars with lower compressive strength than 4MPa, in which case it offers a good value regardless of the mechanical properties of the sand. Although the damage is minimal, and in both cases the structural soundness and stability is not affected, the methods are not non-destructive. Hendry (1993) suggested that for the calculation of strength of historic masonry where lime mortar was used, and 110 direct tests can be carried out, a nominal 1.0 N/mm2 may be taken. Non-destructive testing call be used to assess uniformity and the presence of hidden defects in masonry (Hendry 1993). The hardness of mortars and their strength is usually assessed by subjective methods involving scrapiilg and scratching. A more objective way of assessment was described by Van Der Klugt (199 l), who suggested a classification of the quality of pointing mortars based on their hardness. The hardness was measured by modified Schmidt pendulum hammer where the bigger is the recoil of the pendulum hammer, the harder is the surface. The method is applicable to bedding mortar (measuring head is 51nm in diameter) or plasters.
MORTARS IN ~IISTORIC BUILDINGS: A REVIEW
CONSERVATION, TECHNICAL AND SCIENTIFIC LITERATURE
Adams, J., Kneller, W. and Dollimore, D., "Thermal analysis (TA) of lime- and gypsum-based medieval mortars", Thermocimica Acta, 21 1, (1992), pp. 93- 106. Adams, J., Dollimore, D. and Griffiths, D.L., "Thermal analytical investigation of ancient mortars from gothic churches", Journal of Ther~nalAnalysis, 40, (1993), pp. 275-284. Adams, J., Dollimore, D. and Griffiths, D.L., "Thermal analytical investigation of unaltered Ca(OH), in dated mortars and plasters", Thermochimica Acta, 324, (1998), pp. 67-76. Alvarez, J.I., Martin, A., Garcia Casado, P.J., Navarro I. and Zornoza, A., 'Methodology and validation of a hot hydrochloric acid attack for the characterization of ancient mortars', Cement and Concrete Research, 29, 1999, pp. 1061-1065. Amoroso, G.G. and Fassina, V., "Stone Decay and conservation: atmospheric pollution, cleaning consolidation and protection", Materials Science Monographs, Vol. 11. Elsevier, Amsterdam, 1983. Appolonia, L., "The scientific support of a preservation work: the frescoes in the aosta cathedral upper nave, from the diagnostic research to the completed restoratioa" (sic.), Therinochimica Acta, 2691270, (1995) pp. 769-777. Armelao, L., Bassan, A., Bertoncello, R., Biscontin, G., Daolio, S., Glisenti, A., 'Silica glass interaction with calcium hydroxide: a surface chemistry approach', Jou~llalof Cultural Heritage, 1, 2000, pp. 375-384. ASTM C 110-95b, Standard Test Methods for Physical Testing of Quicklime, Hydrated and limestone, American Society for Testing and Material. Philadelphia, U.S .A. Ashurst, J., 'Mortars, Plasters and Renders in Conservation', Ecclesiastical Architects' and Surveyors' Association, London. 1983. Ashurst, J. and Ashurst N., 'Practical Building Conservation', English Heritage Technical Handbook, volume 4 'Mortars Plasters and Renders', Gower Technical press ltd. 1990.
Ashurst, J., 'Coaservation of building and decorative stone, Part 2. Chapter 4 - Mortars for stone buildings', Butterworth-Heinemann Ltd, 1998, pp. 78-96. The 'Athens Charter' for the Restoration of Historic Monuments, Adopted at the First International Congres of Architects and Technicians of Historic Monuments, Athens, 1931, ICOMOS,
(http://www.icoinos.org/docs/athe~~s~charter.ht~nl) B Baer, N.S. & Snethlage R. (eds.), 'Saving our architectural heritage: the conservation of historic stone structures.' Report of the Dahlem Workshop, held in Berlin 1996, John Wiley & Sons Ltd., 1997. Bakolas, A., Biscontin G., Moropoulou A. and Zendri E. "Characterization of the lumps in the mortars of historic masonry", Thermochimica Acta, 2691270, (1995), pp. 809-8 16. Bakolas, A., Biscontin G., Contardi V., Franceschi E., Moropoulou A., Palazzi D. and Zendri E., "Thermoanalytical research on traditional mortars from Venice", Thermochimica Acta, 2691270, (1995), pp. 817-828. Bakolas, A., Biscontin G., Moropoulou A. and Zendsi E., "Characterization of structural Byzantine mortars by thermogravilnetric analysis", Thermochimica Acta 321, (1998), pp. 151-160. Banfill, P.F.G. and Forster A.M., 'A Relationship between Hydraulicity and Permeability of Hydraulic Lime', RILEM International Workshop, 'Historic Mortars: Characteristics and Tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, RILEM 2000, pp. 173-183. Baronio, G., Binda, L., and Lombardini, N., 'The role of brick pebbles and dust in conglomerates based on hydrated lime and crushed bricks', submitted for the Conv. 7NAMC, Notre Dame, 1996. (published in 'Studies on Mortars Sampled froill Historic Buildingsselected papers 1983-1996, Baronio G. and Binda L., Politechnico di Milano, Structural Engineering Department, 1996, pp. 287- 298).
MORTARS IN HISTORIC BUILDINGS: A REVILW
CONS~KVA~IOW, TECHNICAL AND SCIENTIF~C LITFRATURE
Dix, B., 'The manufacture of lime and its uses in the Western R o ~ n a n Provinces', Oxford Journal of Archaeology, 1(3), 1982, pp. 33 1-345. DomCnech Carbb, M.T., Bosch Reig, F., Girneno Adelantado, J.V. and Periz Martinez, V., "Fourier transfor~n infrared spectroscopy and the analytical study of works of art for purposes of diagnosis and conservation", Analytica Chimica Acta, 330, (1996), pp. 207-215.
E Eckel, E.C., 'Cements, Limes and Plasters', John Wiley and Sons Ltd, 2nd Edition, 1992. EN 196-1, ComitC EuropCen de Normalisatio~lCEN (1987): Methods of testing cement; determination of strength. CEN, Brussels, EN. EN 1015 Methods of tests for Inortar for masonry 1999.
Featherstone, J.D.B., Pearson, S. and LeGeros, R.Z., 'An infrared method for quantification of carbonate in carbonated apatites', Caries Research, 18, (1984), pp. 63-66. Feilden, B.M., 'Conservation of historic buildings', first published 1982, republished by Reed Education and Professional Publishing Ltd., St. Edmundsbury Press, Suffolk, 1998. Fisher, K., 'Traditional Craftsmanship in Modern Mortars - Does it work in practice?', Proc. of RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, RILEM 2000, pp. 281-285. Florez de la Colina, MA. and Ok, I., 'Analysis of Old Mortars from Ancient Agora of Thessaloniki, Greece', Proceedings of the 12th International Brick and Block Masonry Conference, Volu~ne1, Madrid, 2000, pp. 579-593. Folk, R.L. and Campbell, D.H., 'Are the Pyramids of Egypt Built of Poured Concrete Blocks?', Journal of Geological Education, 40, 1992, pp. 25-34. Fontaine, L., Thomson, M.L. & Suter, G., 'Practice and Research: The Need for Standards for Historic Mortars', The Use of crlzd Need of Prese~.vurlolz Stunclurc1.c 111 Al.chitectrll.al Consel.~wtiorl,ASTM STP 1335, L.B. Sickels-Taves, (Ed.), American Society for Testing and Materials, West Conshohocken, PA, 1999, pp. 158-171. Furlan, V., 'Causes, Mechanisms and Measureme~ltof Damage to Mortars, Bricks and Renderings', European sy~nposium 'Science, Technology and European Cultural Heritage', edited by Baer, N.S. et al., Oxford, 1991, pp. 149-159.
G Gibbons, P,, 'Hot Lime Techniques. Some prelilninary investigations', Proceedings of 2nd Inter~lational EUROLIME meeting, Copenhagen, 1993, pp. 21-27. Gibbons, P,, 'Training and standards', Proceedings of Historic Scotland International Lime Conference, September 1995, edited by J.D.D. Ward & I. Maxwell, Lime News, Vol. 4, No. 1, 1995, pp. 44-47. Gibbons, P,, 'Preparation and Use of Lime Mortars' Historic Scotland Technical Advice Note 1, Historic Scotland, Edinburgh, 1995. Godicke-Dettmering, T., Striibel, G., "Mineralogische und technologische Eigenschaften von hydraulischen Kalken als Bindelnittel fiir Restaurierungs~nortelin der Denkmalpflege", Giessener Geologische Sclxiften 56, 1996, pp. 131-154 Grimm, C.T., 'Durability of Brick Masonry: A Review of the Literature', Masonry: Research, Application, and Problems, ASTM STP 871, (Eds.) J.C. Grogan & J.T. Conway, American Society for Testing and Materials, Philadelphia, 1985, pp. 202-234. Groot, C.J.W.P, 'Effects of Water on Mortar-Brick Bond', ISBN 90-90006569-5, Delft University of Technology, Delft, 1993. Groot, C.J.W.P, 'Qualitative Modelling of Water Loss of Fresh Mortars I~nmediately after Bricklaying', Proceedings of the Seventh Canadian Masonry Symposium, McMaster University, Hamilton, Ontario, June 1995, pp. 689-699. Groot, C.J.W., Bartos, P.J.M. and Hughes, J.J., 'Historic Mortars: Characteristics and tests Concluding summary and state-of-the-art', Proceedings of RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, RILEM, 2000, pp. 443-454. Goins, E., 'A New Protocol for the Analysis of Historic Celnentitious Materials: Interim Report', proceedings of RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, RILEM 2000, pp. 71-80. G o n ~ a l v e s , T.D., 'Compatible renders for the conservation of ancient buildings', in Proceedings of the 'Workshop on Compatible Restoration Mortars for the Protection of European Cultural Heritage', National Technical University of Athens, Athens, December 1998. Goodwin, J.F. & West, H.M.H., 'A Review of the Literature on Brick/Mortar Bond', The British Cera~nic Research Association, Technical Note 308, 1980, pp. 23-37.
Gourdin, W.H. & Kingery, W.D. "The Beginnings of Pyrotechnology: Neolithic alld Egyptian Lime Plaster", Journal of Field Archaeology, 2, 1975, pp. 133-150. Gucci, N. & Barsotti, R., 'A non-destructive technique for determillatioll of mortar load capacity in-situ', Materials and Structures, vol. 28, 1995, pp. 276-283.
H Hakanen, E. and Koskikallio, J., "Analysis of aragonite and calcite in precipitated calciunl carbonate by x-ray diffraction and infrared spectroscopic methods", Finn. Chem. Lett, Pt 3-4, (1982), pp. 34-37. Hansen, E.F., Rodriguez-Navai~o, C. and Hansen, R.D., 'Incipient Maya burnt-lime technology: characterisation and chronological variations in preclassic plaster, stucco and mortar at Nakbe, Guatemala.', in 'Materials issues in art and archaeology V', Materials Society Symposium Proceedings, V. 462, Vandiver, P.B., Druzik, J.R., Merkel, F. and Stewart, J.V. (Eds.), 1997, pp. 207-216. Hansen, E.F., Tagle, A., Erder, E., Baron, S., Connell, S., Rodriguez-Navarro, and Van Balen, K., 'Effects of Ageing on Lime Putty', RILEM International Workshop, 'Historic Mortars: Characteristics and tests', edited by P.J. M. Bartos, C.J.W.P Groot and J.J. Hughes, held at the University of Paisley 12-14th May 1999, RILEM Publications, 2000, pp. 197-206. Hai-sies, K.A., 'Concrete construction in early Rome', Concrete International, January 1995.
Hewlett, P.C. (Ed.) 'Lea's Chemistry of Cement and Concrete', 4th Edition, Arnold, London, 1998. Hill, PR., David, J.C.E., 'Practical Stone Masonry', Donhead Publishing Ltd, London, 1995. Hilsdorf, H.K., Kroop, J. and Gunter, M., 'Carbonation, pore structure and durability', 1995. pp. 182-196. Hoffman, G.F., 'Introduction to COST Action C5 'Urban Heritage - Building Maintenance' , in 'Lime within and on top of the outside wall structure' Froschl S. (Ed.), Proceedings of a workshop organised by COST Action C% and EUROCARE, Vienna 18-19 February 1998, pp. 7-9. Hoffmann, D. & Niesel, K., 'Evaluation of lime mortar by physico-technical characteristics', Proceedings of 2nd International EUROLIME meeting, Copenhagen, 1993, pp. 37-40. Holmstrom, I., 'The Architectural Heritage in Sweden. Experiences of the Conservation', report on the Lime Workshop organised by Buildings Lime Forum and IoAAS, held in York, 22-25 October, 1992. Holmstrom, I., 'The usc of lime, Part 1. The general use of lime in Sweden', Proceedings of Historic Scotland International Lime Conference, September 1995, edited by J.D.D. Ward & I. Maxwell, Lime News, Vol. 4, No. 1, 1995, pp. 48- 55.
Harrison, W.H., 'Durability tests on building mortars effect of sand grading', Magazine of Concrete Research, Vol. 38, no. 135, June 1986, pp. 95 - 107.
Holmstrom, I., 'The use of lime, Part 2. Adding cement to lime mortars', Proceedings of Historic Scotland International Lime Conference, September 1995, edited by J.D.D. Ward & I. Maxwell, Lime News, Vol. 4, No. 1, 1995, pp. 56- 62.
Harrison, W.H. & Gaze, M.E., 'Laboratory-Scale Tests on Building Mortars for Durability and Related Properties', Masonry International, Vol. 3, No. l , 1990, pp. 35-41.
Holmstro~n,I., 'Cost C.5, Working Group No. 5, Lime Technology', Newsletter No.3, 3rd International EROLIME meeting, Mainz, 1st - 2nd May, 1998, pp. 105-106.
Hendry, E.A.W., 'Assessment of Stone Masonry Strength in Existing Structures', Proceedings of 5th international conference 'Structural Faults and Repairs', Edinburgh, 1993, pp. 265-268.
Holmes, S. and Wingate, M,, 'Building with Lime', Intermediate Technology Publications, London, 1997.
Henriques, F.M.A. & Charola, E., 'Comparative Study of Standard Test Procedures for Mortars', Proceedings of 8th International Congress on Deterioration & Conservation of Stone, Berlin, 1996, pp. 1521- 1528.
Hosek, J. and Muk,. J., 'Omitky historicksch staveb (Renders of Historic Structures)', Statni PedagogickC Nakladatelsvi, Praha, 1989 (original language only).
Henzel, J. and Karl, S., 'Determination of Strength of Mortar in the Joints of Masonry by Compression Tests on Small Specimens', Darmstadt Concrete, 2, 1987, pp. 123-136. Herm, Ch., Boehm, H.P. & Snethlage, R., 'The Influence of Additives on Lime Wash', Proceedings of 2nd Intelmational EUROLIME meeting, Copenhagen, 1993, pp. 32-36.
Holmes, S., 'Developing Standards for building Limes', Lime News, vol. 6, 1998, pp. 36-40.
Hughes, D. & Swan S., 'Hydraulic Limes - a preliminary investigation', Lime News, vol. 6, 1998, pp. 41-53. Hughes, D. & Sugden D.B., 'The Use of Brick Dust as a Pozzolanic Addition to Hydraulic Lime Mortars', Proc. of RILEM International Workshop, 'Historic Mortars: Characteristics and Tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P. Groot and J.J. Hughes, RILEM, 2000, pp. 351-359.
MORTARS IN HISTORIC BUILDINGS: A REVIEW OF TIIE CONSERVXI'ION, TI~CIINICAL A N D SCIENTIFIC LITERATURE
Hughes, J.J. et al., 'Microstructures in Historic Scottish Lime Mortars', Proceedings of Stone Weathering and Atmospheric Pollution Network '97: Aspects of Stone Decay and Conservation. Edited by M.S. Jones and R.D. Wakefield, Imperial College Press, 1998. Hughes, J.J. and Calleba~~t K., "Practical sampling of historic mortars", RILEM International Workshop, 'Historic Mortars: Characteristics and tests', edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, held at the University of Paisley 12-14th May 1999, RILEM Publications, 2000, pp. 17-26. Hughes, J.J. et al., 'The Experimental Lime Kiln: The Key to Future Mortar Compatibility?', Proceedings of the 12th International Brick and Block Masonry Conference, Volume 4, Madrid, 2000, pp. 903. Hughes, J.J., Cuthbert, S.J.C. and Bartos, P.J.M., "Alteration textures in historic Scottish lime-mortars and the i~nplicationsfor practical mortar analysis", in "Proceedings of the 7th E ~ r o s e m i n aon ~ Microscopy Applied to Building Materials, June 29th - July 2nd, 1999, Delft", Larbi, J.A., Pietersen, H.S. and Janssen, H.J. (eds), Delft University of Technology and TNO Building and Construction Research, 1999, p417-426. Hughes, J.J., Leslie, A.B. and Callebaut, K. 'The petrography of lime inclusions in historic lime based mortars', Proceedings of the 8th Eurose~ninar on Microscopy Applied to Building Materials, Athens, September 4-7th 2001, pp. 359-364. Hughes, P., 'The Need for Old Building to Breath', SPAB Information sheet 4, The Society for the Protection of Ancient Buildings, London, 1986.
I ICCROM, Proceedings of 'Mortars, Cements and Grouts used in the Conservation of Historic Buildings', ICCROM symposium held in Rome between 3 to 6 of November 1981. Indelicato, F., 'A Statistical Method for the Assessment of Concrete Strength through Microcores', Materials and Structures, vol. 26, 1993, pp. 261-267.
J Jedrzejewska, H., 'New Methods in the Investigation of Ancient Mortars', 'Archaeological Chemistry: a Symposium', edited by M. Levey, Philadelphia, 1967. Jedrzejewska, H., 'Ancient Mortars as Criterion in Analyses of Old Architecture', Proceedings of Mortars, Cements and Grouts used in the Conservation of Historic Buildings, ICCROM, 1981, pp. 3 11-329.
Johnston, D., 'Material and manufacture of lime and inortar in Scotland', Proceedings of Historic Scotland International Linle Conference, September 1995, edited by J.D.D. Ward & I. Maxwell, Lime News, Vol. 4, No. l , 1995, pp. 42-43.
Kamimura, K., Sereda, P.J. and Swenson, E.G., 'Changes in weight and dimensions in the drying and carbonation of Portland cement mortars', Magazine of Concrete Research, 17, No. 50, March 1965, pp. 5-14. Karaveziroglou, M. & Papayianni, I., 'Compressive Strength of Masonry with Thick Mortar Joints', Proceeding of the International RILEMJUNESCO Congress, Volume l , Paris, June 29 - July 1, 1993, pp. 212-219. Kingery, W.D., Vandiver, P.B. and Prickett, M,, "The Beginnings of Pyrotechnology, Part 11: Production and Use of Lime and Gypsum Plaster in the Pre-Pottery Neolithic Near East", Journal of Field Archaeology, 15, pp. 219-244, 1988. Kirst, G., Neubarth, K., Gotzenauer, J. and Schreiber, 0. (Eds.), "Decorated Renders around 1900 in Europe", EU-Rendec project Bundesdenkmalt, Wien, 1999. Klemm, D.D. and Klemm, R., 'Mortar evolution in the Old Kingdom of Egypt', in 'Archaeometry '90', International Symposium on Archaeometry, Pernicka, E. and Gunther, A. (Eds.), 1990, pp. 445-454. Van Der Klugt, L.J.A.R., 'The pointing Hardness tester an instrument to meet a need', Materials and Structures, vol. 24, 1991, pp. 471- 476.
Knight, J., 'The Repair of Historic Buildings in Scotland'. Advice on principles and methods. Historic Scotland, Edinburgh, 1995 Knofel, D. and Shubert, P., 'Zur Beurteilung von Morteln fiir die Instandsetzung von Mauerwerk', Mortel und Stein-erganzungsstoffe in der Denkmalpfledge, editors. D. Knofel and P. Schubert, Verlag Ernst & Sohn, Berlin, 1993, pp. 87-106. Kroon, B. and Crook, D.N., 'Studies of pore size distribution in mortars', Magazine of Concrete Research, 13, No. 39, November 1961, pp. 127-132. Kumar Mehta, P. and Monteiro P.J.M., 'ConcreteStructure, properties and materials', Prentice Hall, New Jersey, 2nd edition, 1993.
Lechtman, H. and Hobbs L.W., 'Roman Concrete and the Roman Architectural Revolution', in Ceramics and Civilization, Vol. 3, W.D. Kingery, Ed., American Ceramic Society: 1987, pp. 81-128.
MORTARS IN HISTORIC BUI~.D~NGS: A REVIEW
CONSERVATION, TECIINICAL AND SCIENTIFIC LI'E2RArURE
Larsen, K.P., 'Desalinatio~~ of painted brick vaults', Phd Thesis, Department of Str~rcturalEngineering and Materials, Technical University of Denmark, Series R, No. 52, 1999. Lawrence S. and Samarasinghe, W., 'Assessing the Durability of Masonry Mortars', Proceedings of the 12th I~lte~nationalBrick and Block Masonry Conference, Volulne 4, Madrid, 2000, pp. 1053-1062. Lee, S. H., Bae, Z. U., Kim, K. W., Yang, D. K. and Choi, S.S., "Detern~inationof Calcium carbonate in limestone by attenuated total reflectance fourier transform infrared spectrometry", Analytical Sciences, 13 (supplement), (1997), pp. 93-96. Leslie, A.B. and Gibbons P., 'Mortar Analysis and Repair Specification in the Co~lservationof Scottish Historic Buildings', Proc. of RILEM International Workshop, 'Historic Mortars: Characteristics and Tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P. Groot and J.J. Hughes, RILEM, 2000, pp. 273-280. Liu, Ch., 'Study of the Traditional Method of lime Slaking and Lime Products Making in Beijing, China', Proc. of RILEM International Workshop, 'Historic Mortars: Characteristics and Tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P. Groot and J.J. Hughes, RILEM, 2000, pp. 435-439. Littman, E.R., 'Ancient Mesoarnerican mortars, plasters and stuccos: Comalcalco, Part l ' , American Antiquity, 23, 2, 1957, pp. 135-140. Lucas, A., 'Ancient Egyptian Materials and Industries', third edition, Edward Asnold & Co., 1948. Luxin, M.P., Doi-rego, F. and Laborde, A., "Ancient gypsum Inortars from St. Engracia (Zaragoza, Spain): Characterization. Identification of additives and treatments" (sic.), Cement and Concrete Research, 25, No 8, (1995), pp. 1755-1765. Luxin, M.P. and Donego, F., "Ancient XVI century mortar from the Dominican Republic: its characteristics, lnicrostructure and additives", Cement and Concrete Research, 26, No 6, (1996), pp. 841-849. Lynch, G., 'Lime Mortars for Brickworks: Traditional Practice and Modern Misconceptions - Part One', Journal of Architectural Conservation, No. 1, March, 1998, pp. 7-20.
M Macias, A., de Frutos, J., Blanco, M.T. & Puertas, F., 'The Deterioration of Mortars in Toledo's Cathedral: Studies on Thermal and Hygric Expansion', Proceedings of 7th International Congress on 'Deterioration and Coilservation of Stone', edited by J. Delgado Rodrigues, F. Henriques and ET. Jeremias, Volume 3, Lisbon, 1992, pp. 1213-1221.
MacKinnon, J.J. and May, E.M., 'Small-scale Maya lime ~nakillg in Belize', Ancient Mesoamerica, 1, 1990, pp. 197-203. Malinowski, R., 'Durable Ancient Mortars and Concretes', Nordic Concrete Research, vol. 1, 1981, pp. 1-22. Malinowski, R. and Frifelt, K., 'Prehistoric hydraulic mortars', Research report, Swedish Council for Building Research, 1993. Manzano, E., Bueno, A.G., Gonzalez-Casado, A. and del O l ~ n oM., "Mortars, pigments and binding media of wall painting in the 'Cawera del Darro' in Granada, Spain", Journal of Cultural Heritage, 1, (2000), pp. 1928. Marie-Victoire & Bromblet, P., 'A New Generation of Cement-Based Renderings: an Alternative to Traditional Lime Based Mortars?', Proc. of RILEM Inter~lational Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P. Groot and J.J. Hughes, RILEM, 2000, pp. 37 1-393. Maurenbrecher, A.H.P., Suter G.T. Trischuk, K. & Fontaine, L., 'Contribution to Pointing Mortar Durability', Proc. of RILEM Interllational Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P. Groot and J.J. Hughes, RILEM, 2000, pp 361-369. Maxwell, I., 'I~lteractive?Scottish Sandstone and Lime Mortar', SPAB News, vol. 15, No 4., 1994, pp. 16-18. Maxwell, l., 'Introduction to lime in Scotland', Newsletter No. 3, 21.d International EROLIME meeting, Mainz, 1st - 2nd May, 1998, pp. 88-99. Maxwell, I., 'The use of lime nort tars in the context of dry stone build', Proceedings of RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P. Groot and J.J. Hughes, RILEM, 2000, pp. 314. Mazzullo, S.J. and Teal, C.S., 'Mineralogical and Crystallographic Evidence of Lime Processing, Santa Cruz Maya Site (Classic to Postclassic), Ambergis Caye, Belize', Journal of Archaeological Science, 21, 1994, pp. 785-795. McAfee, P,, 'Irish Stone Walls', The O'Brien Press, Dublin, 1997. Meek, T. et al., 'Case studies of traditional lime harling, a discussion document', edited by Gibbons, P., Historic Scotland, 1996. Meng, B., 'Calculation of moisture transport coefficients on the basis of relevant pore structure parameters', Materials and Structures, 27, 1994, pp. 125-134.
MORTARS IN HISTORIC BUILDINGS: A REVIEIV
Meng, B., 'Determination and interpretation of fractal properties of the sandstone pore system', Materials and Structures, 29 May, 1996, pp. 195-205. Meteorological Office, 'Averages of humidity for the British Isles', Her Majesty 'S Statio~leryOffice, London 1970,42 pages. Michoinova, D., 'Lime Based Mortars for Restoration of Historical Mortars Especially under wall paintings', Proceedings of RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P. Groot and J.J. Hughes, RILEM, 2000, pp. 287-295. Middendorf, B., 'Crystallization- and recrystallization process of gypsum mortars during weathering', in Proc. 8th Euroseminar on Microscopy Applied to Building Materials, Athens Sept. 4-7tl1, 2001, pp. 365372. Middendorf, B. Hughes, J.J., Callebaut, K. and Baronio, G., "Mineralogical and Chemical Characterisation of Historic Mortars", RILEM TC167COM document in preparation for publication in Materials and Structures. Milner, D. J., 'Masonry and Masonry Products: Mortar, Plaster/Stucco and Concrete', Proceedings of the North America International Regional conference 'Preservation and Conservation Principles and Practices', Preservation Press, 1972. Mishara, J., 'Early Hydraulic Cements', in 'Early Pyrotechnology. The Evolution of the First Fire-Using Industries', Wertime, T.A. and Wertime, S .F. (Eds.), Smithsonian Institution Press, 1982, pp. 125-134. Moorehead, D.R, 'Cementation by the carbonation of hydrated lime', Cement and Concrete Research, 16, 1986, pp. 700-708. Moropoulou, A., Bakolas, A. and Bisbikou, K. "Characterisation of ancient, byzantine and later historic mortars by thermal and x-ray diffraction techniques", Thermochimica Acta, 2691270, (1995)a, pp. 779-795. Moropoulou, A., Bakolas, A., Michailidis, P,, Chronopoulos, M. and Spanos, Ch., "Traditional technologies in Crete providing mortars with effective mechanical properties", Structural Studies of Historical Buildings Traditional Technologies.. . , 1, ch 50, (1995)b, pp. 151-161. Moropoulou, A., Bakolas, A., Moundoulas, P. and Camak, A. S., "Compatible restoration mortars for Hagia Sophia earthquake protection", Earthquake Resistant Enginneering Structures, Compatible Restoration ...., Ch. 78, (1999), pp. 522-531. Moropoulou, A., Bakolas, A., Bisbikou, K., "Investigation of the technology of historic mortars",
CONSERVATION: TECIINICAL AND SCIEKTIFIC LITERATURE
Journal of Cultural Heritage, 1, (2000)a, pp. 45-58. Moropoulou, A., Bakolas, A., Bisbikou, K., "Physicochemical adhesion and cohesion bonds in joint mortars imparting durability to the historic structures", Construction and Building Materials, 14, (2000)b, pp. 35-46.
Neville, A.M., 'Properties of Concrete', Sir Isaac Pitman & Sons, London, 1963.
Oates, T., 'Lime and Limestone, chemistry & technology, production & uses, ' Wiley-VCH, ISBN 3527-295-27-5, 1998. Oberholster, R.E., Du Toit, P. and Pretorius, J.L. 'Deterioration of Concrete containing a carbonaceous Sulphide-Bearing Aggregate', in Proc. Xth International Conference on Cement Microscopy, Albuquerque, March 1984, pp. 361-373. Ohgishi, S. and Ono H., 'Study to estimate the depth of neutralisation on concrete members', Cement Association Japan Review, 1993, pp. 168-170. Oleson, J.P., Hohlfelder, R.L., Rabaa, A. and Vann, R.L., 'The Caesarea Ancient Harbor Excavation Project (C.A.H.E.P.): Preliminary Report on the 19801983 Seasons', Journal of Field Archaeology, 11, 1984, pp. 281-305. Ontario Ministry of Citizenship and Culture, 'Annotated master specification for the repointing of historic masonry surfaces', The Ontario Ministry of Citizenship and Culture, revised edition, October, 1988.
Paama, L., Pitkanen, I., Ronkkomaki, H. and Pennamaki P,, "Thermal and infrared spectroscopic characterization of historical mortars", Thermochirnica Acta, 320, (1998), pp. 127-133. Papadakis, V.G., Fardis, M.N. and Vayenas, C.G., 'Effect of composition, envirollmental factors and cement- lime inortar coating on concrete carbonation', Materials and Structures, 25, 1992, pp. 293-304. Papayianni, I. and Tlieocharido~~, K., 'Efflorescence tendency of mortars used in interventions on old masonry', Proceedings of the International RILEMmNESCO Congress: Conservation of stone and other materials, volume 2, edited by M.J. Thiel, Paris, 1993, pp. 621-628. Papayianni, I., Miltiadou, A. and Charkiolakis, N., 'Study of the Existing Old Mortars of the Cells of Hosios Loukas Monastery and Proposal for Compatible Repair Mortars', Proceedings of 5th
International Congress on Restoration of Architectural Heritage, Firenze, 2000 (CD proceedings). Parrot, L.J., 'Carbonation, luoisture and empty pores', Advances in Cement Research. vol. 4, No. 15, 199192, pp. 111-118. Parrot, L.J. and Killoh, DC., 'Carbonation in a 36 year old, in-situ concrete', Cenlent and Concrete Research, vol. 19, 1989, pp. 649-656. Parrot L.J., 'Assessing Carbonation in Concrete Structures', 5th International conference on 'Durability of Building Materials and Components', 7-9 November, Brighton, 1990. Pasley, C.W. 'Observations on Limes', First published in 1838 by John Weale, High Holborn, London. Reprinted edition, Donhead publishing, London, 1997. Perander, T. and RBman, T., 'Ancient and modern mortars in the restoration of historical buildings', Technical Research Centre of Finland, Research Notes, Espoo, May, 1985. Peroni, S., Tersigni, C., Torraca, G., Cerea, S., Forti, M,, Guidobaldi, F.: Rossi-Doria, P,, De Rege, A., Picchi, D., Pietrafitta, F.J. and Benedetti, G., 'Lime based mortars for the repair of ancient nlasonry and possible substitutes', P~.oceeclingsofMor.tc/rs,Ce171e1zts crilcl Grozlts irsed in the Consei.vation of Histoi.ic Builclings, ICCROM, 1981, pp. 63-100. Perry, S.H. & Duffy. A.P., 'The Short Term Effects of Mortar Joints 011 Salt Move~nellt in Stone', Atmospheric Environment, Vol. 31, No. 9, 1997, pp. 1297-1305.
requirelnents and cluality control, Mrrter1rrls cr~zrl Str~ctzii-es,vol. 19, 110. 114, 1986, pp. 445-448.
Sabbioni, C., Piccolo, D., Bonazza, A.: Favoni, 0. and Zappia, G., 'Soluble and No11 Water Soluble Sulphates in Damage Layers on Hydraulic Mortars', Proceedings of Structural Studies, Repairs, and Maintenance of Historical Buildings V11 (STREMH) conference, Bologna 2001, (Ed.) C.A. Brebbia, WIT press, 2001, pp. 561-569. Sasse, H. R. and Snethlage, R., 'Methods for the Evolution of stone coilservation treatments', Report of the Dahlem Workshop on 'Saving our architectural heritage: the conservation of historic stone structures.' Edited by N.S. Baer and R. Snethlage, John Wiley & Sons Ltd. pp. 223-243, 1997. Salnuelli Fenetti, A., ' "Opus Caementicium" the Roman Concrete Do~uus Aurea and Basilica of Maxentius: Stress Analysis and Safety', Proceedings of the 12th International Brick and Block Masonry Conference, Volurne 2, Madrid, 2000, pp. 1589-1600. Sgnchez, J.A., Barrios, S., Barrios, A. and De Arellano Agudo, A.R., 'The Shrinkage in lime mortars', Materiales De Construcci6n, vol. 47, No. 245, 1997, pp. 17-28. Schafer, S. and Hilsdorf, H.K., 'Ancient and new lime mortars- the correlation between their composition, structure and properties', Proceedings of Conservation of Stone and Other Materials, edited by M.J. Thiel, UNESCO, Paris, 1993, pp. 605-612.
Sickels, L.B., 'Mortars in Old Buildings: an Historical Pihlajavaara, S.E., 'Some results of the effect of and Practical Treatise', PhD Thesis, University of carbonation on the porosity and pore size distributio~~ Edinburgh, Edinburgh 1987. of cement paste', Materials and Structure, 1, No. 6, Sickels, L.B., 'Organics vs. Synthetics: Their use as 1968, pp. 521-526. Additives in Mortars', Proceedings of ICCROM prEN The design, preparation and application of conference 'Mortars, Cements and Grouts used in the external renderings, CEN/TC 125, July 1996. Conservation of Historic Buildings', ICCROM, pp. 63100, 1981. Q
R Riccardi, M. P., Duminuco, P,, Tomasi, C. and Ferloni, P., "Thermal microscopic and X-ray diffraction studies on some ancient mortars", Thermoci~nicaActa, 321, (1998), pp. 207-214. RILEM draft recommendation, CPC-18, 'Measurement of hardened concrete carbonation depth', Materials and Structures, 17. 102, 1984, pp. 435-440.
Sickels-Taves, L.B., (ed.), 'The Use of and Need of Preservation Standards in Architectural Conservation', ASTM STP 1335, American Society for Testing and Materials, West Conshohocken, PA, 1999. S~neatonS., 'A narrative of the building . . . of the Eddystone lighthouse', 2nd edition, London, 1793. Soroka, I., 'Portland cement paste and concrete', Macmillan, London, 1979.
Ross, K. & Butlin, R.N., Durability tests for building stone, BRE Re1jo1.f BR 141, Building Research Establishment, Garston CRC, 1989.
Stambolov, T. and van Asperen de Boer, J.R.L., 'The Deterioration and Conservation of Porous Building Materials in Monuments', 2nd edition, Rome, ICCROM, 1976.
Rossi-Doria, P.R., Mortars for restoration: basic
Stewart, S., Glover, R., Houston, J., Seeley, N. &
MORTARS IN HISTORIC BUILDINGS: A KEVIEW OF THE CONSERVA~ION. TECHNICAL A N D SCIENTIFIC LITERATURE
Proudfoot, T., 'Field and Laboratory Assessment of Lime-Based Mortars,' Journal of Architectural Conservation, No. l , 200 1.
Torraca, G., 'Porous Materials Building, Material science for arch~tecturalconservation', ICCROM, third edition, 1988.
Suter, G.T., Thomson, M.L. & Fontaine, L., 'Laboratory Studies of Mortar for Historic Masonry: Mechanical Properties', Proceedings of the Seventh Canadian Masonry Symposium, Mcmaster University, Hamilton, Ontario, June 1995, pp. 700-71 1.
Torraca, G., 'Lime Technology in Architectural conservation', Proceedings of Historic Scotland International Lrrne Conference, September 1995, edited by J.D.D. Ward & I. Maxwell, Lime News, Vol. 4, No. 1, 1995, pp. 34-41.
Suter, G.T. & Song, X. 'Review of Historic Stone Masonry Properties', Proceedings of the Seventh Canadian Masonry Symposium, Mcrnaster University, Hamilton, Ontario, June 1995, pp. 872-883.
T Taylor, H.F.W., 'Cement Chemistry', Academic Press, London, 1990. Teutonico, J.M., McCaing, I., Burns, C., and Ashurst, J., 'The Smeaton Project: Factors Affecting the Properties of Lime-Based Mortars', English Heritage, Collaborative research in association with ICCROM and Bournelnouth University, English Heritage, September, 1994. Teutonico, J.M., Charola, A.E., De Witte, E., Grassegger, G., Koestler, R.J., Laurenzi Tabasso, M,, Sasse, H.R., & Snethlage, R., 'Group Report: How Can We Ensure the Responsible and Effective Use of Treatments (Cleaning, Consolidation, Protection)?', Report of the Dahlem Workshop on 'Saving our architectural heritage: the conservation of historic stone structures.' Edited by N.S. Baer and R. Snethlage, John Wiley & Sons Ltd., 1997, pp. 292-313. Teutonico, J.M., Ashall, G., Garsod, E., & Yates, T., 'A Comparative Study of Hydraulic Lime-Based Mortars', Proc. of RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, RILEM, pp. 339-349, 2000. Thiel, M.J., (ed.), 'Conservation of Stone and Other Materials', Proceedings of the International RILEMfUNESCO Congress, Volumes One and Two, Paris, June 29 - July 1, 1993. Thomson, M.L., 'Plasticity, Water Retention, Soundness and Sand Carrying Capacity: What a Mortar Needs', Proc. of RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, RILEM, 2000, pp.163171. Toumbakari, E.E., Vintzileou, E., Pisano, E and Van Gemert, D., 'Development of a Model Wall for the Experimental Study of Three-Leaf Masonry Walls', Proceedings of the 12th International Brick and Block Masonry Conference, Volume 3, Madrid, 2000, pp. 1865-1875.
v Van Balen, K., 'Karbonatatie van kalkmortels en haar invloed op historische structuren', (Lime mortar carbonation and its influence on historic structures), unpublished PhD thesis, K.U. Leuven, 1991. Van Balen, K. & Van Gemert, D. Modelling lime mortar carbonation, Mater.ials ci/~clStructures, 27, pp. 393-398, 1994. Van Balen, K.E.P., Ercan, S. & Patricio, T.C., 'Compatibility and Retreatability versus Reversibility: A Case Study at the Late Hellenistic Nymphaeum of Sagalassos (Turkey).', Tlre Use of a11d Need of Presel-vrrtion Stcir7darcls in Arrhitect~rr.alConsel-18ntio11, ASTM STP 1335, L.B. Sickels-Taves, (Ed.), American Society for Testing and Materials, West Conshohocken, PA, 1999, pp. 105-118. Van Balen, K.E.P. and Papayianni, I., " Van Hees, R.P.J., 'Damage diagnosis and co~npatible repair mortars', RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, RILEM 2000, pp. 27-36. Vilek, J., Hughes, J.J. and Bartos, P.J.M., 'Portable Probe Gas Permeability in the Testing of Historic Masonry and Mortars', RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C. J.W.P Groot and J.J. Hughes, RILEM 2000, pp. 185196. Vilek, J., Hughes, J.J. and Bartos, P.J.M., 'Gas Permeability, Porosity and Carbollation of Modem Conservation Lime Mortar Mix', Proceedings of EUROMAT 1999 conference, Volume 6, 'Materials for Buildings and Structures', edited by F.H. Wittmaan, WILEY-VCH, 2000, pp. 209-215. Vilek, J., Hughes, J.J. and Bartos, P.J.M., 'Portable Probe Gas Permeability: a non-destructive test for the in-situ characterisation of historic ~nasonry',Materials and Structures, vo1.33, April 2000, pp. 194-197. Vilek, J., 'Lime Mortars in Historic Buildings', PhD thesis, University of Paisley, 2000. Vilek, J., Hughes, J.J. and Bartos, P.J.M., 'Compatibility of Historic and Modern Lime Mortars',
MORTARS I N HISTORIC BUILDINGS: A REVIEW
Proceedings of the 12th International Brick and Block Masonry Conference, Volunle 4, Madrid, 2000, pp. 1839. VBlek, J. & Bartos, P.J.M., 'Influences Affecting Con~pressiveStrength of Modern Non-hydraulic Lime Mortars Used in Masonry Conservation', Proceedings of Structural Studies, Repairs, and Maintenance of Historical Buildings V11 (STREMH) conference, Bologna 2001, (Ed.) C.A. Brebbia, WIT press, 2001, pp. 571-580 Veiga, R. and Carvalho, F., 'Sorne Performance Characteristics of Lime Mortars for Use of Rendering and Repointing of Ancient Buildings', Proceedings of 5th International Masonry Conference, British Masonry Society, No. 8, 1998. Veiga, R., 'A Methodology to Evaluate the Cracking Susceptibility of Renders: Equipment, Tests and Criteria. Experimental Data', Proceedings of 5th International Masonry Conference, British Masonry Society, No. 8, 1998. 'Venice Charter', International Charter for the Conservation and Restoration of Monuments and Sites. ICOMOS, 1964, (http://www.icornos.org/docs/venice~charter.html). Venneltfoort, A.T., Groot, C.J.W.P. and Wijen, E., 'Thermal strains in repointed masonry: preliminary investigations using ESPI', Proc. of RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, RILEM, 2000, pp. 219- 228. Vicat, L., 'Mortars and Cements'. Translated by Captain J. T. Smith. First published in English in 1837 by John Weale, High Holborn, London, Reprinted edition, Donhead publishing, London, 1997. Vitruvius, P,, 'The Ten Books on Architecture', translated by Morgan H.M., Dover publications, New York, 1960. Von Konow, T., 'The secret of old mortar - can we solve it?', Proceedings of 2nd International EUROLIME meeting, Copenhagen, 1993, pp. 28-3 1. Von Konow, T., 'Reliable restoration mortarsrequirements and composition', 4th International Symposium on the Conservation of Monuments, Rhodes, May, 1997. Von Konow, T., 'Restoration Mortars
CONSERVATION, TECI-INICAL AN11 SCIENTIFIC LITERATURE
Defined Co~nposition and Informative Testing Methods', Lime News, vol. 6, 1998, pp. 83-86.
W Ward, J.D. and Maxwell, I., 'International Lime Conference', Proceedings of Historic Scotland International Lime Conference, September 1995, edited by J.D.D. Ward & I. Maxwell, Lime News, Vol. 4, No. 1, 1995. Waldum, A.M & Anda, O., 'Durability of Lime-Based Mortars in a Severe Climate. Results from Field and Artificial Ageing Tests', Proc. of RILEM International Workshop, 'Historic Mortars: Characteristics and tests', held at Paisley 1999, edited by P.J.M. Bartos, C.J.W.P Groot and J.J. Hughes, RILEM, 2000, pp. 297306. Walker, M.B. (ed.), 'Cambridge Dictionary of Science and Technology', Cambridge University Press, 1988. Walker, P.J. and Dickens, J.G., 'Intervention techniques in the conservation of dry stone structures', Proceeding of Conservation of Stone and Other Materials, edited by M.J. Thiel, UNESCO, Paris, 1993, pp. 452-459. Wallace, W., 'On Ancient Mortars', Chemical News, 11, 1865, pp. 185-186. Watt, D. and Swallow, P., 'Surveying Historic Buildings', Donhead Publishing, UK, 1996. Weber, J., Orcsik, E. and Gaggl, W., 'Scientific Background and Analysis of Hydraulic Plaster materials', in 'Decorated Renders around 1900 in Europe', EU-Rendec pro-ject, Kirst, G., Neubarth, K., Gotzenauer, J. and Schreiber, 0. (Eds.), Bundesdenkmalt, Wien 1999. Wingate, M,, 'Standards for building limes', proceedings of conference 'Lime and Other Alternative Cements', Intermediate Technology Publications, London, 1992.
z Zappia, G., Sabbioni, C., Pauri, M.G. & Gobbi, G., 'Mortar damage due to airborne sulphur cornpounds in a simulation chamber', Materials and Structures, vol. 27. 1994, pp. 469-473.
MORTARS IN HIsIOKIC
B U I L D T ~ SA: REVIEW OF TIIE
CONSLKVAI )ON, TECHNICAL AND SCICNTIFIC LITEKAIUKL
Published on Mar 21, 2014
A review of the technical and scientific literature relating to mortar in historic buildings. The publication considers compatibility and a...